495 84 26MB
English Pages 202 Year 1996
Carbon nanotubes have been studied extensively in relation to fullerenes, and together with fullerenes have opened a new
385 81 26MB Read more
Carbon nanotubes have been studied extensively in relation to fullerenes, and together with fullerenes have opened a new
481 55 7MB Read more
The book covers the chronological development of synthetic approaches to make carbon nanotube mimics. It starts with the
169 18 2MB Read more
Carbon nanotubes are exceptionally interesting from a fundamental research point of view. Many concepts of one-dimension
414 95 4MB Read more
The book covers the chronological development of synthetic approaches to make carbon nanotube mimics. It starts with the
167 74 5MB Read more
This Handbook covers the fundamentals of carbon nanotubes (CNT), their composites with different polymeric materials (bo
240 43 62MB Read more
Carbon Nanotubes takes a broad look at CNTs and the tools used to study them. It opens with a general introduction to th
486 82 5MB Read more
Elsevier Journals of Related Interest
Applied Superconductivity Carbon Journal of Physics and Chemistry of Solids Nanostructured Materials Polyhedron Solid State Communications Tetrahedron Tetrahedron Letters
CARBON NANOTUBES Edited by
MORINUBO END0 Shinshu University, Japan
SUM10 IIJIMA NEC, Japan
MILDRED S. DRESSELHAUS Massachusetts Institute of Technology, USA
Elsevier Science Ltd, The Boulevard, Langford Lane, Kidlington, Oxford OX5 lGB, U.K.
Elsevier Science Inc., 660 White Plains Road, Tarrytown, New York 10591-5153, U.S.A.
Elsevier Science Japan, Tsunashima Building Annex, 3-20-12 Yushima Bunko-ku, Tokyo 113, Japan Copyright
zyxwvut zyxwvu zyxwvuts 0 1996 Elsevier Science Limited
All Rights Reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, electrostatic, magnetic tape, mechanical, photocopying, recording or otherwise, without permission in writing from the publisher
First edition 1996
Library of Congress Cataloging in Pulication Data
A catalog record for this book is available from the Library of Congress British Library Cataloguing in Publication Data
A catalogue record for this book is available in the British Library ISBN 008 0426824 Reprinted from: Carbon, Vol. 33, Nos 1, 2, 7, 12
Printed and bound in Great Britain by BPC Wheatons Ltd, Exeter
zyxwvuts zyxw CONTENTS
M. ENDO, S. IIJIMA and M. S. DRESSELHAUS: Editorial , . . . . . . . . . . . . . . . . . . . . . .
M. S. DRESSELHAUS: Preface: Carbon nanotubes . . . . , . . . . , . . . . . . . . . . . . . . . . . . . . . . .
M. ENDO, K. TAKEUCHI, K. KOBORI, K. TAKAHASHI, H. W. KROTO and A. SARKAR: Pyrolytic carbon nanotubes from vapor-grown carbon fibers.. . . . . . .
D. T. COLBERT and R. E. SMALLEY: Electric effects in nanotube growth.. . . . . . * . .
V. IVANOY, A. FONSECA, J. B. NAGY, A. LUCAS, P. LAMBIN, D. BERNAERTS and X. B. ZHANG: Catalytic production and purification of nanotubes having fullerenescale diameters . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
M. S. DRESSELHAUS, G. DRESSELHAUS and R. SAITO: Physics of carbon nanotubes
J. W. MINTMIRE and C. T. WHITE: Electronic and structural properties of carbon nanotubes ..................................................................
C.-H. KIANG, W. A. GODDARD 111, R. BEYERS and D. S. BETHUNE: Carbon nanotubes with single-layer walls . . . . . . . . , . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
R. SETTON: Carbon nanotubes: I. Geometrical considerations . . . . . . . . . . . . . . . . . . . . . .
K. SATTLER: Scanning tunneling microscopy of carbon nanotubes and nanocones . . . . .
T. W. EBBESEN and T. TAKADA: Topological and SP3 defect structures in nanotubes
S. IHARA and S. ITOH: Helically coiled and torodial cage forms of graphitic carbon . .
A. FONSECA, K. HERNADI, J. B. NAGY, P. H. LAMBIN and A. A. LUCAS: Model structure of perfectly graphitizable coiled carbon nanotubes . . . . . . . . . . . . . . . . . . . . .
A. SARKAR, H. W. KROTO and M. ENDO: Hemi-toroidal networks in pyrolytic carbon nanotubes . . . . . . . . . . . . . . . . . . . . , . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105
X. K. WANG, X. W. LIN, S. N. SONG, V. P. DRAVID, J. B. KETTERSON and R. P. H. CHANG: Properties of buckytubes and derivatives.. . . . . . . . . . . . . . . . . . . . 111 J.-P. ISSI, L. LANGER, J. HEREMANS and C. H. OLK: Electronic properties of carbon nanotubes: Experimental results . . . . . . . . . . . . . . . . . . . . . . . . . . , . . . . . . . . . . . . . . . , . . . 121 P. C. EKLUND, J. M. HOLDEN and R. A. JISHI: Vibrational modes of carbon nanotubes: Spectroscopy and theory. . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 129
R. S. RUOFF and D. C. KORENTS: Mechanical and thermal properties of carbon nanotubes . . .. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . .. . 143
J. IF. DESPRES, E. DAGUERRE and K. LAFDI: Flexibility of graphene layers in carbon nanotubes. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.49 V
Y. SAITO: Nanoparticles and filled nanocapsules ...................................
D. UGARTE: Onion-like graphitic particles ........................................
U. ZIMMERMAN. N. MALINOWSKI. A . BURKHARDT and T. P. MARTIN: Metalcoated fullerenes ............................................................ 169
allotropes. Readers can then understand the fascination of graphene sheets when they are rolled into a nanometer size tubular form from a flat network corresponding to conventional graphite. This book also contains complementary reviews on carbon nanoparticles such as carbon nano-capsules, onionlike graphite particles and metal-coated fullerenes.
Carbon nanotubes have been studied extensively in relation to fullerenes, and together with fullerenes have opened a new science and technology field on nano scale materials. This book aims to cover recent research and development in this area, and so provide a convenient reference tool for all researchers in this field. It is a.lso hoped that this book can serve to stimulate future work on carbon nanotubes.
We hope this book will contribute to the dissemination of present understanding of the subject and to future developments in the science and technology of carbon nanotubes and fullerenes, and of carbon science more generally.
Carbon nanotubes have the same range of diameters as fullerenes, and are expected to show various kinds of size effects in their structures and properties. Carbon nanotubes are one-dimensional materials and fullerenes are zero-dimensional, which brings different effects to bear on their structures as well as on their properties. A whole range of issues from the preparation, structure, properties and observation of quantum effects in carbon nanotubes in comparison with 0-Dfullerenes are discussed in this book.
zyxw zyxwvutsrq The editors thank all authors who contributed so many excellent papers covering all aspects of carbon nanotubes and the related fields. We are indebted to the Editor-in-Chief of Carbon, Professor Peter A. Thrower, for his suggestion and kind efforts, and also to Dr V. Kiruvanayagam for her kind cooperation related to this book. Morinobu Endo Sumio Iijima Mildred S. Dresselhaus Editors
In order to review the wide research area of carbon nanotubes this book focuses on recent intensive work published in Carbon. The papers are written from the viewpoint that carbon nanotubes, as well as fullerenes, are the most interesting new carbon
efficiency and smaller nanotubes are discussed in the article by Ivanov and coworkers. The quantum aspects of carbon nanotubes, stemming from their small diameters, which contain only a small number of carbon atoms (< lo2), lead to remarkable symmetries and electronic structure, as described in the articles by Dresselhaus, Dresselhaus and Saito and by Mintmire and White. Because of the simplicity of the single-wall nanotube, theoretical work has focussed almost exclusively on single-wall nanotubes. The remarkable electronic properties predicted for carbon nanotubes are their ability to be either conducting or to have semiconductor behavior, depending on purely geometrical factors, namely the diameter and chirality of the nanotubes. The existence of conducting nanotubes thus relates directly to the symmetry-imposed band degeneracy and zero-gap semiconductor behavior for electrons in a two-dirnensional single layer of graphite (called a graphene sheet). The existence of finite gap semiconducting behavior arises from quantum effects connected with the small number of wavevectors associated with the circumferential direction of the nanotubes. The article by Kiang et al. reviews the present status of the synthesis of single-wall nanotubes and the theoretical implications of these single-wall nanotubes. The geometrical considerations governing the closure, helicity and interlayer distance of successive layers in multilayer carbon nanotubes are discussed in the paper by Setton. Study of the structure of carbon nanotubes and their common defects is well summarized in the review by Sattler, who was able to obtain scanning tunneling microscopy (STM) images of carbon nanotube surfaces with atomic resolution. A discussion of common defects found in carbon nanotubes, including topological, rehybridization and bonding defects is presented by Ebbesen and Takada. The review by Ihara and Itoh of the many helical and toroidal forms of carbon nanostructures that may be realized provides insight into the potential breadth of this field. The joining of two dissimilar nanotubes is considered in the article by Fonseca et al., where these concepts are also applied to more complex structures such as tori and coiled nanotubes. The role of semi-toroidal networks in linking the inner and outer walls of a double-walled carbon nanotube is discussed in the paper by Sarkar et al.
Since the start of this decade (the 1990's), fullerene research has blossomed in many different directions, and has attracted a great deal of attention to Carbon Science. It was therefore natural to assemble, under the guest editorship of Professor Harry Kroto, one of the earliest books on the subject of fullerenes 111, a book that has had a significant impact on the subsequent developments of the fullerene field. Stemming from the success of the first volume, it is now appropriate to assemble a follow-on volume on Carbon Nanotubes. It is furthermore fitting that Dr Sumio Iijima and Professor Morinobu Endo serve as the Guest Editors of this volume, because they are the researchers who are most responsible for opening up the field of carbon nanotubes. Though the field is still young and rapidly developing, this is a very appropriate time to publish a book on the very active topic of carbon nanotubes. The goal of this book is thus to assess progress in the field, to identify fruitful new research directions, to summarize the substantial progress that has thus far been made with theoretical studies, and to clarify some unusual features of carbon-based materials that are relevant to the interpretation of experiments on carbon nanotubes that are now being so actively pursued. A second goal of this book is thus to stimulate further progress in research on carbon nanotubes and related materials. 'The birth of the field of carbon nanotubes is marked by the publication by Iijima of the observation of multi-walled nanotubes with outer diameters as small as 55 A, and inner diameters as small as 23 A, and a nanotube consisting of only two coaxial cyknders . This paper was important in making the connection between carbon fullerenes, which are quantum dots, with carbon nanotubes, which are quantum wires. Furthermore this seminal paper  has stimulated extensive theoretical and experimental research for the past five years and has led to the creation of a rapidly developing research field. The direct linking of carbon nanotubes to graphite and the continuity in synthesis, structure and properties between carbon nanotubes and vapor grown carbon fibers is reviewed by the present leaders of this area, Professor M. Endo, H. Kroto, and co-workers. Further insight into the growth mechanism is presented in the article by Colbert and Smalley. New synthesis methods leading to enhanced production
zyxwv zyxwv zyx
From an experimental point of view, definitive measurements on the properties of individual carbon nanotubes, characterized with regard to diameter and chiral angle, have proven to be very difficult to carry out. Thus, most of the experimental data available thus far relate to multi-wall carbon nanotubes and to bundles of nanotubes. Thus, limited experimental information is available regarding quantum effects for carbon nanotubes in the one-dimensional limit. A review of structural, transport, and susceptibility measurements on carbon nanotubes and related materials is given by Wang et al., where the interrelation between structure and properties is emphasized. Special attention is drawn in the article by Issi et al. to quantum effects in carbon nanotubes, as observed in scanning tunneling spectroscopy, transport studies and magnetic susceptibility measurements. The vibrational modes of carbon nanotubes is reviewed in the article by Eklund et al. from both a theoretical standpoint and a summary of spectroscopy studies, while the mechanical that thermal properties of carbon nanotubes are reviewed in the article by Ruoff and Lorents. The brief report by Despres et al. provides further evidence for the flexibility of graphene layers in carbon nanotubes.
The final section of the volume contains three complementary review articles on carbon nanoparticles. The first by Y. Saito reviews the state of knowledge about carbon cages encapsulating metal and carbide phases. The structure of onion-like graphite particles, the spherical analog of the cylindrical carbon nanotubes, is reviewed by D. Ugarte, the dominant researcher in this area. The volume concludes with a review of metal-coated fullerenes by T. P. Martin and co-workers, who pioneered studies on this topic. The guest editors have assembled an excellent set of reviews and research articles covering all aspects of the field of carbon nanotubes. The reviews are presented in a clear and concise form by many of the leading researchers in the field. It is hoped that this collection of review articles provides a convenient reference for the present status of research on carbon nanotubes, and serves to stimulate future work in the field. M. S. DRESSELHAUS
1. H. W. Kroto, Carbon 30, 1139 (1992). 2. S . Iijima, Nature (London) 354, 56 (1991).
PYROLYTIC CARBON NANOTUBES FROM VAPOR-GROWN CARBON FIBERS
MORINOBU ENDO,'Kmn TAKEUCHI,' KIYOHARUKOBORI,'KATSUSHITAKAHASHI, I HAROLD W. K R O T O ,and ~ A. SARKAR' 'Faculty of Engineering, Shinshu University, 500 Wakasato, Nagano 380, Japan 'School of Chemistry and Molecular Sciences, University of Sussex, Brighton BNl SQJ, U.K.
(Received 21 November 1994; accepted 10 February 1995)
Abstract-The structure of as-grown and heat-treated pyrolytic carbon nanotubes (PCNTs) produced by hydrocarbon pyrolysis are discussed on the basis of a possible growth process. The structures are compared with those of nanotubes obtained by the arc method (ACNT, arc-formed carbon nanotubes). PCNTs, with and without secondary pyrolytic deposition (which results in diameter increase) are found to form during pyrolysis of benzene at temperatures ca. 1060°C under hydrogen. PCNTs after heat treatment at above 2800°C under argon exhibit have improved stability and can be studied by high-resolution transmission electron microscopy (HRTEM). The microstructures of PCNTs closely resemble those of vaporgrown carbon fibers (VGCFs). Some VGCFs that have micro-sized diameters appear to have nanotube inner cross-sections that have different mechanical properties from those of the outer pyrolytic sections. PCNTs initially appear to grow as ultra-thin graphene tubes with central hollow cores (diameter ca. 2 nm or more) and catalytic particles are not observed at the tip of these tubes. The secondary pyrolytic deposition, which results in characteristic thickening by addition of extra cylindrical carbon layers, appears to occur simultaneously with nanotube lengthening growth. After heat treatment, HRTEM studies indicate clearly that the hollow cores are closed at the ends of polygonized hemi-spherical carbon caps. The most commonly observed cone angle at the tip is generally ca. 20", which implies the presence of five pentagonal disclinations clustered near the tip of the hexagonal network. A structural model is proposed for PCNTs observed to have spindle-like shape and conical caps at both ends. Evidence is presented for the formation, during heat treatment, of hemi-toroidal rims linking adjacent concentric walls in PCNTs. A possible growth mechanism for PCNTs, in which the tip of the tube is the active reaction site, is proposed.
Key Words-Carbon nanotubes, vapor-grown carbon fibers, high-resolution transmission electron microscope, graphite structure, nanotube growth mechanism, toroidal network.
Since Iijima's original report[l], carbon nanotubes have been recognized as fascinating materials with nanometer dimensions promising exciting new areas of carbon chemistry and physics. From the viewpoint of fullerene science they also are interesting because they are forms of giant fuIlerenes. The nanotubes prepared in a dc arc discharge using graphite electrodes at temperatures greater than 3000°C under helium were first reported by Iijima[l] and later by Ebbesen and Ajyayan. Similar tubes, which we call pyrolytic carbon nanotubes (PCNTs), are produced by pyrolyzing hydrocarbons (e.g., benzene at ca. 110OoC)[4-9]. PCNTs can also be prepared using the same equipment as that used for the production of so called vapor-grown carbon fibers (VGCFs)[lOJ.The VGCFs are micron diameter fibers with circular crosssections and central hollow cores with diameters ca. a few tens of nanometers. The graphitic networks are arranged in concentric cylinders. The intrinsic structures are rather like that of the annual growth of trees. The structure of VGCFs, especially those with hollow cores, are very similar to the structure of arc-formed carbon nanotubes (ACNTs). Both types of nanotubes, the ACNTs and the present PCNTs, appear to be essentially Russian Doll-like sets of elongated giant ful,lerenes[ll,12]. Possible growth processes have
been proposed involving both open-ended1131 and closed-cap[l 1,121 mechanisms for the primary tubules. Whether either of these mechanisms or some other occurs remains to be determined. It is interesting to compare the formation process of fibrous forms of carbon with larger micron diameters and carbon nanotubes with nanometer diameters from the viewpoint of "one-dimensional)) carbon structures as shown in Fig. 1. The first class consists of graphite whiskers and ACNTs produced by arc methods, whereas the second encompasses vapor-grown carbon fibers and PCNTs produced by pyrolytic processes. A third possibIe class would be polymer-based nanotubes and fibers such as PAN-based carbon fibers, which have yet to be formed with nanometer dimensions. In the present paper we compare and discuss the structures of PCNTs and VGCFs.
zyxwv zyx 2. VAPOR-GROWN CARBON FIBERS AND
PYROLYTIC CARBON NANOTUBES
Vapor-grown carbon fibers have been prepared by catalyzed carbonization of aromatic carbon species using ultra-fine metal particles, such as iron. The particles, with diameters less than 10 nm may be dispersed on a substrate (substrate method), o r allowed to float in the reaction chamber (fluidized method). Both
M. ENDOet al.
Fig. 1. Comparative preparation methods for micrometer size fibrous carbon and carbon nanotubes as one-dimensional forms of carbon.
methods give similar structures, in which ultra-fine catalytic particles are encapsulated in the tubule tips (Fig. 2). Continued pyrolytic deposition occurs on the initially formed thin carbon fibers causing thickening (ca. 10 pm diameter, Fig. 3a). Substrate catalyzed fibers tend to be thicker and the floating technique produces thinner fibers (ca. 1 pm diameter). This is due to the shorter reaction time that occurs in the fluidized method (Fig. 3b). Later floating catalytic methods are useful for large-scale fiber production and, thus, VGCFs should offer a most cost-effective means of producing discontinuous carbon fibers. These VGCFs offer great promise as valuable functional carbon filler materials and should also be useful in carbon fiber-reinforced plastic (CFRP) production. As seen in Fig. 3b even in the “as-grown” state, carbon particles are eliminated by controlling the reaction conditions. This promises the possibility of producing pure ACNTs without the need for separating spheroidal carbon particles. Hitherto, large amounts of carbon particles have always been a byproduct of nanotube production and, so far, they have only been eliminated by selective oxidation[l4]. This has led to the loss of significant amounts of nanotubes - ca. 99%.
Fig. 3. Vapor-grown carbon fibers obtained by substrate method with diameter ca. 10 pm (a) and those by floating catalyst method (b) (inserted, low magnification).
3. PREPARATION OF VGCFs AND PCNTs
The PCNTs in this study were prepared using the same apparatus as that employed to produce VGCFs by the substrate method[l0,15]. Benzene vapor was introduced, together with hydrogen, into a ceramic reaction tube in which the substrate consisted of a centrally placed artificial graphite rod. The temperature of the furnace was maintained in the 1000°C range. The partial pressure of benzene was adjusted to be much lower than that generally used for the preparation of VGCFs[lO,lS] and, after one hour decomposition, the furnace was allowed to attain room temperature and the hydrogen was replaced by argon. After taking out the substrate, its surface was scratched with a toothpick to collect the minute fibers. Subsequently, the nanotubes and nanoscale fibers were heat treated in a carbon resistance furnace under argon at temperatures in the range 2500-3000°C for ca. 10-15 minutes. These as-grown and sequentially heat-treated PCNTs were set on an electron microscope grid for observation directly by HRTEM at 400kV acceleration voltage. It has been observed that occasionally nanometer scale VGCFs and PCNTs coexist during the early stages of VGCF processing (Fig. 4). The former tend to have rather large hollow cores, thick tube walls and well-organized graphite layers. On the other hand,
Fig. 2. Vapour-grown carbon fiber showing relatively early stage of growth; at the tip the seeded Fe catalytic particle is encapsulated.
zyxwv Pyrolytic carbon nanotubes from vapor-grown carbon fibers
b Fig. 5 . Heat-treated pyrolytic carbon nanotube and enlarged one (inserted), without deposited carbon.
This results in well-organized multi-walled concentric graphite tubules. The interlayer spacing (0.34 nm) is slightly wider on average than in the case of thick VGCFs treated at similar temperatures. This small increase might be due to the high degree of curvature of the narrow diameter nanotubes which appears to prevent perfect 3-dimensional stacking of the graphitic layers[ 16,171. PCNTs and VGCFs are distinguishable by the sizes of the well-graphitized domains; crosssections indicate that the former are characterized by single domains, whereas the latter tend to exhibit multiple domain areas that are small relative to this crosssectional area. However, the innermost part of some VGCFs (e.g., the example shown in Fig. 5 ) may often consist of a few well-structured concentric nanotubes. Theoretical studies suggest that this “single grain” aspect of the cross-sections of nanotubes might give rise to quantum effects. Thus, if large scale real-space super-cell concepts are relevant, then Brillouin zonefoiding techniques may be applied to the description of dispersion relations for electron and phonon dynamics in these pseudo one-dimensional systems. A primary nanotube at a very early stage of thickening by pyrolytic carbon deposition is depicted in Figs. 6a-c; these samples were: (a) as-grown and (b), (c) heat treated at 2500°C. The pyrolytic coatings shown are characteristic features of PCNTs produced by the present method. The deposition of extra carbon layers appears to occur more or less simultaneously with nanotube longitudinal growth, resulting in spindle-shaped morphologies. Extended periods of pyrolysis result in tubes that can attain diameters in the micron range (e.g., similar to conventional (thick) VGCFs[lO]. Fig. 6c depicts a 002 dark-field image, showing the highly ordered central core and the outer inhomogeneously deposited polycrystalline material (bright spots). It is worthwhile to note that even the very thin walls consisting of several layers are thick enough to register 002 diffraction images though they are weaker than images from deposited crystallites on the tube. Fig. 7a,b depicts PCNTs with relatively large diameters (ca. 10 nm) that appear to be sufficiently tough
Fig. 4. Coexisting vapour-grown carbon fiber, with thicker diameter and hollow core, and carbon nanotubes, with thinner hollow core, (as-grown samples).
PCNTs tend to have very thin walls consisting of only a few graphitic cylinders. Some sections of the outer surfaces of the thin PCNTs are bare, whereas other sections are covered with amorphous carbon deposits (as is arrowed region in Fig. 4a). TEM images of the tips of the PCNTs show no evidence of electron beam opaque metal particles as is generally observed for VGCF tips[lO,l5]. The large size of the cores and the presence of opaque particles at the tip of VGCFs suggests possible differences between the growth mechanism for PCNTs and standard VGCFs[7-91. The yield of PCNTs increases as the temperature and the benzene partial pressure are reduced below the optimum for VGCF production (i.e., temperature ca. 1000°-11500C). The latter conditions could be effective in the prevention or the minimization of carbon deposition on the primary formed nanotubules.
4. STRUCTURES OF PCNTs
Part of a typical PCNT (ca. 2.4 nm diameter) after heat treatment at 2800°C for 15 minutes is shown in Fig. 5. It consists of a long concentric graphite tube with interlayer spacings ca. 0.34 nm-very similar in morphology to ACNTs[ 1,3]. These tubes may be very long, as long as 100 nm or more. It would, thus, appear that PCNTs, after heat treatment at high temperatures, become graphitic nanotubes similar to ACNTs. The heat treatment has the effect of crystallizing the secondary deposited layers, which are usually composed of rather poorly organized turbostratic carbon.
zyxwvutsrqpo zyxwvu M. ENDOet al.
Fig. 7. Bent and twisted PCNT (heat treated at 2500T).
Fig. 6 . PCNTs with partially deposited carbon layers (arrow indicates the bare PCNT), (a) as-grown, (b) partially exposed nanotube and (c) 002 dark-field image showing small crystallites on the tube and wall of the tube heat treated at 2500°C.
and flexible to bend, twist, or kink without fracturing. The basic structural features and the associated mechanical behavior of the PCNTs are, thus, very different from those of conventional PAN-based fibers as well as VGCFs, which tend to be fragile and easily broken when bent or twisted. The bendings may occur at propitious points in the graphene tube network[l8]. Fig. 8a,b shows two typical types of PCNT tip morphologies. The caps and also intercompartment diaphragms occur at the tips. In general, these consist of 2-3 concentric layers with average interlayer spacing of ca. 0.38 nm. This spacing is somewhat larger than that of the stackings along the radial direction, presumably (as discussed previously) because of sharp curvature effects. As indicated in Fig. 9, the conical shapes have rather symmetric cone-like shells. The angle, ca. 20°, is in good agreement with that expected for a cone constructed from hexagonal graphene sheets containing pentagonal disclinations -as is Fig. 9e. Ge and Sattler[l9] have reported nanoscale conical carbon materials with infrastructure explainable on the basis of fullerene concepts. STM measurements show that nanocones, made by deposition of very hot carbon on HOPG surfaces, often tend to
Fig. 8. The tip of PCNTs with continuous hollow core (a) and the cone-like shape (b) (T indicates the toroidal structure shown in detail in Fig. 11).
Pyrolytic carbon nanotubes from vapor-grown carbon fibers
zyxwvutsrq zyxwvuts zyxwvu zyxwvut z
e = 180- (360/ n )cos-' [l - (n/6)]
(n : number of pentagons)
Fig. 9. The possible tip structure with cone shape, in which the pentagons are included. As a function of the number of pentagons, the cone shape changes. The shaded one with 19.2" tip angle is the most frequently observed in PCNTs.
have an opening angle of ca. 20". Such caps may, however, be of five possible opening angles (e.g., from 112.9" to 19.2") depending on the number of pentagonal disclinations clustered at the tip of the cone, as indicated in Fig. 9. Hexagons in individual tube walls are, in general, arranged in a helical disposition with variable pitches. It is worth noting that the smallest angle (19.2') that can involve five pentagons is most frequently observed in such samples. It is frequently observed that PCNTs exhibit a spindle-shaped structure at the tube head, as shown in Fig. 8b.
Growth direction 4
chiralsaucture Fig. 10. Growth mechanism proposed for the helical nanotubes (a) and helicity (b), and the model that gives the bridge and laminated tip structure (c).
5. GROWTH MODEL OF PCNTs
In the case of the PCNTs considered here, the growth temperature is much lower than that for ACNTs, and no electric fields, which might influence the growth of ACNTs, are present. It is possible that different growth mechanisms apply to PCNT and ACNT growth and this should be taken into consideration. As mentioned previously, one plausible mechanism for nanotube growth involves the insertion of small carbon species C,,( n = 1,2,3 . . .) into a closed fullerene cap (Fig. loa-c)[ll]. Such a mechanism is related to the processes that Ulmer et a1. and McE1vaney et a1. have discovered for the growth of
small closed cage fullerenes. Based on the observation of open-ended tubes, Iijima et a1. have discussed a plausible alternative way in which such tubules might possibly grow. The closed cap growth mechanism effectively involves the addition of extended chains of sp carbon atoms to the periphery of the asymmetric 6-pentagon cap, of the kind whose Schlegel diagram is depicted in Fig. loa, and results in a hexagonal graphene cylinder wall in which the added atoms are arranged in a helical disposition[9,1 I] similar to that observed first by Iijima[l].
M. ENDOet al.
It is proposed that during the growth of primary tubule cores, carbon atoms, diameters, and longer linear clusters are continuously incorporated into the active sites, which almost certainly lie in the vicinity of the pentagons in the end caps, effectively creating helical arrays of consecutive hexagons in the tube wall as shown in Fig. 10a,b[9,11]. Sequential addition of 2 carbon atoms at a time to the wall of the helix results in a cap that is indistinguishable other than by rotation[ll,l2]. Thus, if carbon is ingested into the cap and wholesale rearrangement occurs to allow the new atoms to “knit” smoothly into’ the wall, the cap can be considered as effectively fluid and to move in a screw-like motion leaving the base of the wall stationary- though growing by insertion of an essentially uniform thread of carbon atoms to generate a helical array of hexagons in the wall. The example shown in Fig. 10a results in a cylinder that has a diameter (ca. 1 nm) and a 22-carbon atom repeat cycle and a single hexagon screw pitch -the smallest archetypal (isolated pentagon) example of a graphene nanotube helix. Though this model generates a tubule that is rather smaller than is usually the case for the PCNTs observed in this study (the simplest of which have diameters > 2-3 nm), the results are of general semiquantitative validity. Figure 10b,c shows the growth mechanism diagrammatically from a side view. When the tip is covered by further deposition of aromatic layers, it is possible that a templating effect occurs to form the new secondary surface involving pentagons in the hexagonal network. Such a process would explain the laminated or stacked-cup-like morphology observed. In the case of single-walled nanotubes, it has been recognized recently that transition metal particles play a role in the initial filament growth process. ACNTs and PCNTs have many similarities but, as the vaporgrowth method for PCNTs allows greater control of the growth process, it promises to facilitate applications more readily and is thus becoming the preferred method of production.
6. CHARACTERISTIC TOROIDAL AND SPINDLE-LIKE STRUCTURES OF PCNTS
In Fig. 1l a is shown an HRTEM image of part of the end of a PCNTs. The initial material consisted of a single-walled nanotube upon which bi-conical spindle-like growth can be seen at the tip. Originally, this tip showed no apparent structure in the HRTEM image at the as-grown state, suggesting that it might consist largely of some form of “amorphous” carbon. After a second stage of heat treatment at 280O0C, the amorphous sheaths graphitize to a very large degree, producing multi-walled graphite nanotubes that tend to be sealed off with caps at points where the spindlelike formations are the thinnest. The sealed-off end region of one such PCNT with a hemi-toroidal shape is shown in Fig. 1la. In Fig. 1l b are depicted sets of molecular graphics images of flattened toroidal structures which are
Fig. 11. The sealed tip of a PCNT heat treated at 2800°C with a toroidal structure (T) and, (b) molecular graphics images of archetypal flattened toroidal model at different orientations and the corresponding simulated TEM images.
the basis of archetypal double-walled nanotubes. As the orientation changes, we note that the HRTEM interference pattern associated with the rim changes from a line to an ellipse and the loop structures at the apices remain relatively distinct. The oval patterns in the observed and simulated HRTEM image (Fig. 1lb) are consistent with one another. For this preliminary investigation a symmetric (rather than helical) wall configuration was used for simplicity. Hemi-toroidal connection of the inner and outer tubes with helical structured walls requires somewhat more complicated dispositions of the 5/6/7 rings in the lip region. The general validity of the conclusions drawn here are, however, not affected. Initial studies of the problem indicated that linking between the inner and outer walls is not, in general, a hindered process.
Pyrolytic carbon nanotubes from vapor-grown carbon fibers
The toroidal structures show interesting changes in morphology as they become larger-at least at the lip. The hypothetical small toroidal structure shown in Fig. 1 l b is actually quite smooth and has an essentially rounded structure. As the structures become larger, the strain tends to focus in the regions near the pentagons and heptagons, and this results in more prominent localized cusps and saddle points. Rather elegant toroidal structures with Dnhand Dndsymmetry are produced, depending on whether the various paired heptagodpentagon sets which lie at opposite ends of the tube are aligned or are offset. In general, they probably lie is fairly randomly disposed positions. Chiral structures can be produced by off-setting the pentagons and heptagons. In the D5dstructure shown in Fig. 11 which was developed for the basic study, the walls are fluted between the heptagons at opposite ends of the inner tube and the pentagons of the outer wall rim[l7]. It is interesting to note that in the computer images the localized cusping leads to variations in the smoothness of the image generated by the rim, though it still appears to be quite elliptical when viewed at an angle[ 171. The observed image appears to exhibit variations that are consistent with the localized cusps as the model predicts. In this study, we note that epitaxial graphitization is achieved by heat treatment of the apparently mainly amorphous material which surrounds a single-walled nanotube[ 171. As well as bulk graphitization, localized hemi-toroidal structures that connect adjacent walls have been identified and appear to be fairly common in this type of material. This type of infrastructure may be important as it suggests that double walls may form fairly readily. Indeed, the observations suggest that pure carbon rim-sealed structures may be readily produced by heat treatment, suggesting that the future fabrication of stabilized double-walled nanoscale graphite tubes in which dangling bonds have been eliminated is a feasible objective. It will be interesting to prove the relative reactivities of these structures for their possible future applications in nanoscale devices (e.g., as quantum wire supports). Although the curvatures of the rims appear to be quite tight, it is clear from the abundance of loop images observed, that the occurrence of such turnovers between concentric cylinders with a gap spacing close to the standard graphite interlayer spacing is relatively common. Interestingly, the edges of the toroidal structures appear to be readily visible and this has allowed us to confirm the relationship between opposing loops. Bulges in the loops of the kind observed are simulated theoretically[ 171. Once one layer has formed (the primary nanotube core), further secondary layers appear to deposit with various degrees of epitaxial coherence. When inhomogeneous deposition occurs in PCNTs, the thickening has a characteristic spindle shape, which may be a consequence of non-carbon impurities which impede graphitization (see below)- this is not the case for ACNTs were growth takes place in an essentially allcarbon atmosphere, except, of course, for the rare gas. These spindles probably include the appropriate num-
Fig. 12. As-grown PCNTs with partially thickened spindle shape (a) and the proposed structural model for spindle particles including 12 pentagons in hexagon cage (b).
ber of pentagons as required by variants of Euler’s Law. Hypothetical structural models for these spindles are depicted in Fig. 12. It is possible that similar two-stage growth processes occur in the case of ACNTs but, in general, the secondary growth appears to be intrinsically highly epitaxial. This may be because in the ACNT growth case only carbon atoms are involved and there are fewer (non-graphitizing) alternative accretion pathways available. It is likely that epitaxial growth control factors will be rather weak when secondary deposition is very fast, and so thin layers may result in poorly ordered graphitic structure in the thicker sections. It appears that graphitization of this secondary deposit that occurs upon heat treatment may be partly responsible for the fine structure such as compartmentalization, as well as basic tip morphology[ 171. 7. VGCFs DERIVED FROM NANOTUBES
In Fig. 13 is shown the 002 lattice images of an “asformed” very thin VGCF. The innermost core diameter (ca. 20 nm as indicated by arrows) has two layers; it is rather straight and appears to be the primary nanotube. The outer carbon layers, with diameters ca. 3-4 nm, are quite uniformly stacked parallel to the central core with 0.35 nm spacing. From the difference in structure as well as the special features in the mechanical strength (as in Fig. 7) it might appear possible that the two intrinsically different types of material
M. ENDOet al.
of ca. 10 nm (white arrow), observed by field emission scanning electron microscopy (FE-SEM). It is, thus, suggested that at least some of the VGCFs start as nanotube cores, which act as a substrate for subsequent thickening by deposition of secondary pyrolytic carbon material, as in the catalytically primarily grown hollow fiber. In Fig. 14b is also shown the TEM image corresponding to the extruded nanotube from a very thin fiber. It is clearly observed that the exposed nanotube is continuing into the fiber as a central hollow core, as indicated by the white arrow in the figure. It is interesting that, as indicated before (in Fig. 14a), the core is more flexible than the pyrolytic part, which is more fragile. Fig. 13. HRTEM image of an as-grown thick PCNT. 002 lattice image demonstrates the innermost hollow core (core diam. 2.13 nm) presumably corresponding to the “as-formed” nanotube. The straight and continuous innermost two fringes similar to Fig. 5 are seen (arrow).
involved might be separated by pulverizing the VGCF material. In Fig. 14a, a ca. 10 wm diameter VGCF that has been broken in liquid nitrogen is depicted, revealing the cylindrical graphitic nanotube core with diameter
Pyrolytic carbon nanotubes (PCNTs), which grow during hydrocarbon pyrolysis, appear to have structures similar to those obtained by arddischarge techniques using graphite electrodes (ACNTs). The PCNTs tend to exhibit a characteristic thickening feature due to secondary pyrolytic carbon deposition. Various tip morphologies are observed, but the one most frequently seen has a 20” opening angle, suggesting that, in general, the graphene conical tips possess a cluster of five pentagons that may be actively involved in tube growth. PCNTs with spindle-like shapes and that have conical caps at both ends are also observed, for which a structural model is proposed. The spindle-like structures observed for the secondary growth thickening that occurs in PCNTs may be a consequence of the lower carbon content present in the growth atmosphere than occurs in the case of ACNT growth. Possible structural models for these spindles have been discussed. The longitudinal growth of nanotubes appears to occur at the hemi-spherical active tips and this process has been discussed on the basis of a closed cap mechanism[9,11]. The PCNTs are interesting, not only from the viewpoint of the fundamental perspective that they are very interesting giant fullerene structures, but also because they promise to be applications in novel strategically important materials in the near future. PCNT production appears, at this time, more readily susceptible to process control than is ACNT production and, thus, their possible value as fillers in advanced composites is under investigation.
zyxwvu Acknowledgements-Japanese authors are indebted to M. S. Dresselhaus and G. Dresselhaus of MIT and to A. Oberlin of Laboratoire Marcel Mathieu (CNRS) for their useful discussions and suggestions. HWK thanks D. R. M. Walton for help and the Royal Society and the SERC (UK) for support. Part of the work by ME is supported by a grant-in-aid for scientific research in priority area “carbon cluster” from the Ministry. of Education, Science and Culture, Japan.
Fig. 14. PCNTs (white arrow) appeared after breakage of VGCF, (a) FE-SEM image of broken VGCF, cut in liquid nitrogen and (b) HRTEM image showing the broken part observed in very thin VGCF. The nanotube is clearly observed and this indicates that thin VGCF grow from nanometer core by thickening.
1 . S. Iijima, Nature 354, 56 (1991). 2. H. W. Kroto, J. R. Heath, S. C .O’Brien, R. F. Curl, and R. E. Samlley, Nature 318, 162 (1985).
zyxwvutsr zyxwvut zyxwvut zyxwvuts zyxwvu zyxwvutsr zyxwvu Pyrolytic carbon nanotubes from vapor-grown carbon fibers
3. T. W. Ehhesen and P. M. Ajayan, Nature 358, 220 ( 1 992). 4. M. Endo, H. Fijiwara, and E. Fukunaga, 18th Meeting Japanese Carbon Society, (1991) p. 34. 5 . M. Endo, H. Fujiwara, and E. Fukunaga, 2nd C60 Symposium in Japan, (1992) p. 101. 6. M. Endo, K. Takeuchi, S. Igarashi, and K. Kobori, 19th Meeting Japanese Carbon Society, (1992) p. 192. 7. M. Endo, K. Takeuchi, S. Igarashi, K. Kobori, and M. Shiraishi, Mat. Res. SOC. Spring Meet (1993) p.S2.2. 8 . M. Endo, K. Takeuchi, S. Igarashi, K. Kobori, M. Shiraishi, and H. W. Kroto, Mat. Res. SOC.FallMeet. 62.1 (1994). 9. M. Endo, K. Takeuchi, S. Igarashi, K. Kobori, M. Shiraishi, and H. W. Kroto, J. Phys. Chem. Solids 54, 1841 (1993). 10. M. Endo, Chemtech 18, 568 (1988). 11. M. Endo and H. W. Kroto, J. Phys. Chem. 96, 6941 (1992). 12. I-I. W. KrOtQ, K. Prassides, R. Taylor, D. R. M. Walton, and bd. Endo, International Conference Solid State Devices and Materials of The Japan Society of Applied Physics (1993), p. 104. 13. S. Iijima, Mat. Sci. Eng. B19, 172 (1993). 14. P. M. Ajayan, T. W. Ebbesen, T. Ichihashi, S. Iijirna, K. Tanigaki, and H. Hiura, Nature 362, 522 (1993).
15. M. S. Dresselhaus, G Dresselhaus, K. Sugihara, I. L. Spain, H. A. Goldberg, In Graphite Fibers and Filaments, (edited by M . Cardona) pp. 244-286. Berlin, Springer. 16. J. S. Speck, M. Endo, and M. S. Dresselhaus, J. Crystal Growth 94, 834 (1989). 17.. A. Sarkar, H. W. Kroto, and M. Endo (in preparation). 18. H. Hiura, T. W. Ebbesen, J. Fujita, K. Tanigaki, and T. Takada, Nature 367, 148 (1994). 19. M. Ge and K. Sattler, Mat. Res. SOC.Spring Meet. S1.3, 360 (1993). 20. G. Ulmer, E. E. B. Cambel, R. Kuhnle, H. G. Busmann, and 1. V . Hertel, Chem. Phys. Letts. 182, 114 (1991). 21. S. W. McElvaney, M. N. Ross, N. S. Goroff, and E Diederich, Science 259, 1594 (1993). 22. R. Saito, G . Dresselhaus, M. Fujita, and M. S. Dresselhaus, 4th NEC Symp. Phys. Chem. Nanometer Scale Mats. (1992). 23. S. Iijima, Gordon Conference on the Chemistry of Hydrocarbon Resources, Hawaii (1994). 24. A. Sarker, H. W. Kroto, and M. Endo (to he published). 25. M. Endo, K. Takeuchi, K. Kobori, K. Takahashi, and H. W. Kroto (in preparation).
ELECTRIC EFFECTS IN NANOTUBE GROWTH DANIEL T. COLBERT and RICHARDE. SMALLEY
Rice Quantum Institute and Departments of Chemistry and Physics, MS 100, Rice University, Houston, TX 77251-1892, U.S.A. (Received 3 April 1995; accepted 7 April 1995)
Abstract-We present experimental evidence that strongly supports the hypothesis that the electric field of the arc plasma is essential for nanotube growth in the arc by stabilizing the open tip structure against closure. By controlling the temperature and bias voltage applied to a single nanotube mounted on a macroscopic electrode, we find that the nanotube tip closes when heated to a temperature similar to that in the arc unless an electric field is applied. We have also developed a more refined awareness of “open” tips in which adatoms bridge between edge atoms of adjacent layers, thereby lowering the exothermicity in going from the open to the perfect dome-closed tip. Whereas realistic fields appear to be insufficient by themselves to stabilize an open tip with its edges completely exposed, the field-induced energy lowering of a tip having adatom spot-welds can, and indeed in the arc does, make the open tip stable relative to the closed one. Key Words-Nanotubes,
electric field, arc plasma
zyxwvutsrq 1. INTRODUCTION
the electric field concentrates, and never in the soots condensed from the carbon vapor exiting the arcing region, suggest a vital role for the electric field. Furthermore, the field strength at the nanotube tips is very large, due both to the way the plasma concentrates most of the potential drop in a very short distance above the cathode, and to the concentrating effects of the field at the tips of objects as small as nanotubes. The field may be on the order of the strength required to break carbon-carbon bonds, and could thus dramatically effect the tip structure. In the remaining sections of this paper, we describe the experimental results leading to confirmation of the stabilizing role of the electric field in arc nanotube growth. These include: relating the plasma structure to the morphology of the cathode deposit, which revealed that the integral role of nanotubes in sustaining the arc plasma is their field emission of electrons into the plasma; studying the field emission characteristics of isolated, individual arc-grown nanotubes; and the discovery of a novel production of nanotubes that significantly alters the image of the “open” tip that the arc electric field keeps from closing.
As recounted throughout this special issue, significant advances in illuminating various aspects of nanotube growth have been made[l,2] since Iijima’s eventful discovery in 1991; these advances are crucial to gaining control over nanotube synthesis, yield, and properties such as length, number of layers, and helicity. The carbon arc method Iijima used remains the principle method of producing bulk amounts of quality nanotubes, and provides key clues for their growth there and elsewhere. The bounty of nanotubes deposited on the cathode (Ebbesen and Ajayan have found that up to 50% of the deposited carbon is tubular) is particularly puzzling when one confronts the evidence of UgarteI.51 that tubular objects are energetically less stable than spheroidal onions. It is largely accepted that nanotube growth occurs at an appreciable rate only at open tips. With this constraint, the mystery over tube growth in the arc redoubles when one realizes that the cathode temperature (-3000°C) is well above that required to anneal carbon vapor to spheroidal closed shells (fullerenes and onions) with great efficiency. The impetus to close is, just as for spheroidal fullerenes, elimination of the dangling bonds that unavoidably exist in any open structure by incorporation of pentagons into the hexagonal lattice. Thus, a central question in the growth of nanotubes in the arc is: How do they stay open? One of us (RES) suggested over two years ago161 that the resolution to this question lies in the electric field inherent to the arc plasma. As argued then, neither thermal nor concentration gradients are close to the magnitudes required to influence tip annealing, and trace impurities such as hydrogen, which might keep the tip open, should have almost no chemisorption residence time at 3000°C. The fact that well-formed nanotubes are found only in the cathode deposit, where
2. NANOTUBES AS FIELD EMITTERS
Defects in arc-grown nanotubes place limitations on their utility. Since defects appear to arise predominantly due to sintering of adjacent nanotubes in the high temperature of the arc, it seemed sensible to try to reduce the extent of sintering by cooling the cathode better. The most vivid assay for the extent of sintering is the oxidative heat purification treatment of Ebbesen and coworkers, in which amorphous carbon and shorter nanoparticles are etched away before nanotubes are substantially shortened. Since, as we proposed, most of the nanoparticle impurities orig11
D. T.COLBERT and R. E. SMALLEY
inated as broken fragments of sintered nanotubes, the amount of remaining material reflects the degree of sintering. Our examinations of oxygen-purified deposits led to construction of a model of nanotube growth in the arc in which the nanotubes play an active role in sustaining the arc plasma, rather than simply being a passive product. Imaging unpurified nanotube-rich arc deposit from the top by scanning electron microscopy (SEM) revealed a roughly hexagonal lattice of 50-micron diameter circles spaced -50 microns apart. After oxidative treatment the circular regions were seen to have etched away, leaving a hole. More strikingly, when the deposit was etched after being cleaved vertically to expose the inside of the deposit, SEM imaging showed that columns the diameter of the circles had been etched all the way from the top to the bottom of the deposit, leaving only the intervening material. Prior SEM images of the column material (zone 1) showed that the nanotubes there were highly aligned in the direction of the electric field (also the direction of deposit growth), whereas nanotubes in the surrounding region (zone 2) lay in tangles, unaligned with the field. Since zone 1 nanotubes tend to be in much greater contact with one another, they are far more susceptible to sintering than those in zone 2, resulting in the observed preferential oxidative etch of zone 1. These observations consummated in a growth model that confers on the millions of aligned zone 1 nanotubes the role of field emitters, a role they play so effectively that they are the dominant source of electron injection into the plasma. In response, the plasma structure, in which current flow becomes concentrated above zone 1, enhances and sustains the growth of the field emission source-that is, zone 1 nanotubes. A convection cell is set up in order to allow the inert helium gas, which is swept down by collisions with carbon ions toward zone 1, to return to the plasma. The helium flow carries unreacted carbon feedstock out of zone 1, where it can add to the growing zone 2 nanotubes. In the model, it is the size and spacing of these convection cells in the plasma that determine the spacing of the zone l columns in a hexagonal lattice.
bias was controlled relative to an opposing electrode, and if desired, reactive gases could be introduced. Two classes of emission behavior were found. An inactivated state, in which the emission current increased upon laser heating at a fixed potential bias, was consistent with well understood thermionic field emission models. Figure l a displays the emission current as the laser beam is blocked and unblocked, revealing a 300-fold thermal enhancement upon heating. Etching the nanotube tip with oxygen while the tube was laser heated to 1500°C and held at -75 V bias produced an activated state with exactly the opposite behavior, shown in Fig. 2b; the emission current increased by nearly two orders of magnitude when the laser beam was blocked! Once we eliminated the possibility that species chemisorbed on the tip might be responsible for this behavior, the explanation had to invoke a structure built only of carbon whose sharpness would concentrate the field, thus enhancing the emission current. As a result of these studies, a dramatic and unexpected picture has emerged of the nanotube as field emitter, in which the emitting source is an atomic wire composed of a single chain of carbon atoms that has been unraveled from the tip by the force of the applied electric field (see Fig. 2). These carbon wires can be pulled out from the end of the nanotube only once the ragged edges of the nanotube layers have been exposed. Laser irradiation causes the chains to be clipped from the open tube ends, resulting in low emission when the laser beam is unblocked, but fresh ones are pulled out once the laser is blocked. This unraveling behavior is reversible and reproducible.
z zyxwvuts zyxwvut 4. THE STRUCTURE OF AN OPEN NANOTUBE TIP
A portion of our ongoing work focusing on spheroidal fderenes, particularly metallofullerenes, utilized the same method of production as was originally used in the discovery of fullerenes, the laser-vaporization method, except for the modification of placing the flow tube in an oven to create better annealing conditions for fullerene formation. Since we knew that at the typical 1200°C oven temperature, carbon clusters readily condensed and annealed to spheroidal fullerenes (in yields close to 40%), we were astonished to find, upon transmission electron micrographic examination of the collected soots, multiwalled nanotubes with few or no defects up to 300 nm long[lO]! How, we asked ourselves, was it possible for a nanotube precursor to remain open under conditions known to favor its closing, especially considering the absence of extrinsic agents such as a strong electric field, metal particles, or impurities to hold the tip open for growth and elongation? The only conclusion we find tenable is that an intrinsic factor of the nanotube was stabilizing it against closure, specifically, the bonding of carbon atoms to edge atoms of adjacent layers, as illustrated in Fig. 2. Tight-binding calculations[l 1J indicate that such sites are energetically preferred over direct addition to the hexagonal lattice of a single layer by as much as 1.5 eV
zyxw zyxwvut zy
3. FIELD EMISSION FROM AN ATOMIC WIRE
Realization of the critical importance played by emission in our arc growth model added impetus to investigations already underway to characterize nanotube field emission behavior in a more controlled manner. We had begun working with individual nanotubes in the hope of using them as seed crystals for controlled, continuous growth (this remains an active goal). This required developing techniques for harvesting nanotubes from arc deposits, and attaching them with good mechanical and electrical connection to macroscopic manipulators[2,8,9]. The resulting nanoelectrode was then placed in a vacuum chamber in which the nanotube tip could be heated by application of Ar+-laser light (514.5 nm) while the potential
zy zyxwv zyxwvu 13
Electric effects in nanotube growth
Laser On Laser Off
Fig. 1. Field emission data from a mounted nanotube. An activated nanotube emits a higher current when heated by the laser than when the laser beam is blocked (a). When activated by exposing the nanotube to oxygen while heating the tip, this behavior is reversed, and the emission current increases dramatically when the laser is blocked. The activated state can also be achieved by laser heating while maintaining a bias voltage of -75 V. Note that the scale of the two plots is different; the activated current is always higher than the inactivated current. As discussed in the text, these data led to the conclusion that the emitting feature is a chain of carbon atoms pulled from a single layer of the nanotube-an atomic wire.
per adatom. We also knew at this time that the electric field of the arc was not by itself sufficient to stabilize an open tip having no spot-welds against closure[l2], so we now regard these adatom "spot-welds'' as a necessary ingredient to explain growth of nanotubes in the oven laser-vaporization method as well as in the arc, and probably other existing methods of nanotube production. 5. ELECTRIC FIELD STABILIZATION OF AN OPEN NANOTUBE TIP
Fig. 2. A graphic of a nanotube showing a pulled-out atomic wire and several stabilizing spot-welds. Only two layers have been shown for clarity, although typical multiwalled nanotubes have 10-15 layers. The spot-weld adatoms shown between layers stabilize the open tip conformation against closure. The atomic wire shown was previously part of the hexagonal lattice of the inner layer. It is prevented from pulling out further by the spot-weld at its base.
The proposal that the essential feature of arc growth was the high electric field that concentrates at the growing nanotube tip prompted ab initio structure calculations[ 12,131 to assess this hypothesis quantitatively. These calculations, which were performed for single-walled nanotubes in high applied electric fields, showed that field-induced lowering of the open tip energy is not sufficient to make the open conformation more stable than the closed tip at any field less than 10 V/A. Whereas single-walled objects certainly anneal and at 12000c t' form 'pheroidal fullerenes[l4,151, open multiwalled species have other alternatives, and thus may be auite different in this respect. In particular, for multiwalled species, adatom spot-welds may be sufficiently stabilizing to allow before succumbing to the growth and conformation.
D. T . COLBERT and R. E. SMALLEY
In the absence of an electric field, the dome-closed conformation must be the most stable tip structure, even when spot-welds are considered, since only the perfectly dome-closed tip has no dangling bonds (Le., it is a true hemifullerene). At the 3000°C temperature of the arc, the rate of tip annealing should be so fast that it is sure to find its most stable structure (i.e., to close as a dome). Clear evidence of this facile closure is the fact that virtually all nanotubes found in the arc deposit are dome-closed. (Even stronger evidence is the observation of only dome-closed nanotubes made at 1200°C by the oven laser vaporization method.) Such considerations constituted the original motivation for the electric field hypothesis. Armed with these results, a direct test of the hypothesis using a single mounted nanotube in our vacuum apparatus was sensible. A dome-closed nanotube harvested from the arc deposit gave inactivated state behavior at -75 V bias. Maintaining the bias voltage at -75 V, the nanotube was irradiated for about 30 seconds with sufficient intensity to sublime some carbon from the tip (-3000°C). Now the nanotube exhibited typical activated emission behavior, indicating an open tip from which long carbon chains were pulled, constituting the emitting structures described in section 3 above. When the nanotube was reheated at 0 V bias, the tip was re-closed. Subsequent heating to 3000°C at -75 V bias re-opened the tip. These results can only be explained by the electric field’s providing the necessary stabilization to keep the tip open. The structure calculations on single-walled tubes show that the stabilizing effect of the field is at most about 10% of that required to lower the energy of the open below that of the closed tip, before reaching unrealistically strong field strengths. However, with our enhanced understanding of the structure of nanotube tips, much of the energy lowering is achieved by the adatom spot-welds (not included in the calculations), leaving less of an energy gap for the electric field effect to bridge. We emphasize that spot-welds alone cannot be sufficient to render the open tip stable relative to the dome-closed one, since the latter structure is the only known way to eliminate all the energetically costly dangling bonds. An electric field is necessary.
With expanding knowledge about the ways nanotubes form and behave, and as their special properties are increasingly probed, the time is fast approaching when nanotubes can be put to novel uses. Their size and electrical properties suggest their use as nanoprobes, for instance, as nanoelectrodes for probing the chemistry of living cells on the nanometer scale. The atomic wire may be an unrivaled cold field emission source of coherent electrons. Such potential uses offer the prospect of opening up new worlds of investigation into previously unapproachable domains.
Acknowledgements-This work was supported by the Office of Naval Research, the National Science Foundation, the Robert A. Welch Foundation, and used equipment designed for study of fullerene-encapsulated catalysts supported by the Department of Energy, Division of Chemical Sciences.
zyxw zyxw zyx
1. T. W. Ebbesen, Ann. Rev. Mat. Sei. 24, 235 (1994); S. Iijima, P. M. Ajayan, and T. Ichihashi, Phys. Rev. Lett. 69, 3100 (1992); Y. Saito, T . Yoshikawa, M. Inagaki, M. Tomita, and T. Hayashi, Chem. Phys. Lett. 204, 277 (1993). 2. D. T . Colbert et a/., Science 266, 1218 (1994). 3. S. Iijima, Nature 354, 56 (1991). 4. T. W. Ebbesen and P. M. Ajayan, Nature 358, 220 (1992). 5 . D. Ugarte, Chem. Phys. Lett. 198,596 (1992); D. Ugarte, Nature 359, 707 (1992). 6. R. E. Srnalley, Mat Sci. Eng. B19, 1 (1993). 7. T. W. Ebbesen, P. M. Ajayan, H. Hiura, and K. Tanigaki, Nature 367, 519 (1994). 8. A. G. Rinzler, J. H. Hafner, P. Nikolaev, D. T. Colbert, and R. E. Srnalley, MRS Proceedings 359 (1995). 9. A. G. Rinzler et al., in preparation. 10. T. Guo et al., submitted for publication. 11. J. Jund, S. G. Kim, and D. Tomanek, in preparation; C. Xu and G. E. Scuseria, in preparation. 12. L. Lou, P. Nordlander, and R. E. Srnalley, Phys. Rev. Lett. (in press). 13. A. Maiti, C. J. Brabec, C. M. Roland, and J. Bernholc, Phys. Rev. Lett. 13, 2468 (1994). 14. R. E. Haufler et al., Mat. Res. Symp. Proc. 206, 621 (1991). 15. R. E. Srnalley, Acct. Chem. Res. 25, 98 (1992).
CATALYTIC PRODUCTION AND PURIFICATION OF NANOTUBULES HAVING FULLERENE-SCALE DIAMETERS
V. I[vANov,~** A. FONSECA," J. B.NAGY,"+ A. LUCAS," P. LAMBIN," D. BERNAERTS~ and X. B. ZHANG~
"Institute for Studies of Interface Science, FacultCs Universitaires Notre Dame de la Paix, 61 rue de Bruxelles, B-5000 Namur, Belgium bEMAT,University of Antwerp (RUCA),Groenenborgerlaan 171, B-2020 Antwerp, Belgium (Received 25 July 1994; accepted in revisedform 13 March 1995)
Abstract-Carbon nanotubules were produced in a large amount by catalytic decomposition of acetylene in the presence of various supported transition metal catalysts. The influence of different parameters such as the nature of the support, the size of active metal particles and the reaction conditions on the formation of nanotubules was studied. The process was optimized towards the production of nanotubules having the same diameters as the fullerene tubules obtained from the arc-hscharge method. The separation of tubules from the substrate, their purification and opening were also investigated. Key Words-Nanotubules, fullerenes, catalysis.
production. The synthesis of the nanotubules of various diameters, length and structure as dependent on the parameters of the method is studied in detail. The elimination of amorphous carbon is also investigated.
The catalytic growth of graphitic carbon nanofibers during the decomposition of hydrocarbons in the presence of either supported or unsupported metals, has been widely studied over the last years[ 1-61. The main goal of these studies was to avoid the formation of "filamentous" carbon, which strongly poisons the catalyst. More recently, carbon tubules of nanodiameter were found to be a byproduct of arc-discharge production of fullerenes . Their calculated unique properties such as high mechanical strength[ 81, their capillary properties [91 and their remarkable electronic structure [ 10-121 suggest a wide range of potential uses in the future. The catalytically produced filaments can be assumed to be analogous to the nanotubules obtained from arcdischarge and hence to possess similar properties [51, they can also be used as models of fullerene nanotubes. Moreover, advantages over arc-discharge fibers include a much larger length (up to 50pm) and a relatively low price because of simpler preparation. Unfortunately, carbon filaments usually obtained in catalytic processes are rather thick, the thickness being related to the size of the active metal particles. The graphite layers of as-made fibres contain many defects. These filaments are strongly covered with amorphous carbon, which is a product of the thermal decomposition of hydrocarbons [ 131. The catalytic formation of thin nanotubes was previously reported[ 141. In this paper we present the detailed description of the catalytic deposition of carbon on various well-dispersed metal catalysts. The process has been optimized towards the large scale nanotubes
The catalytic decomposition of acetylene was carried out in a flow reactor at atmospheric pressure. A ceramic boat containing 20-100 mg of the catalyst was placed in a quartz tube (inner diameter 4-10 mm, length 60-100 cm). The reaction mixture of 2.5-10% CzH2 (Alphagaz, 99.6%) in N, (Alphagaz, 99.99%) was passed over the catalyst bed at a rate of 0.15-0.59 mol C2H2g-lh-' for several hours at temperatures in the range 773-1073 K. The catalysts were prepared by the following methods. Graphite supported samples containing 0.5-10 wt% of metal were prepared by impregnation of natural graphite flakes (Johnson-Matthey, 99.5%) with the solutions of the metal salts in the appropriate concentrations: Fe or Co oxalate (Johnson-Matthey), Ni or Cu acetate (Merck). Catalysts deposited on SiO, were obtained by porous impregnation of silica gel (with pores of 9 nm, ,S 600 m2g1, Janssen Chimica) with aqueous solutions of Fe(IJ1) or Co(I1) nitrates in the appropriate amounts to obtain 2.5 wt% of metal or by ion-exchange-precipitation of the same silica gel with 0.015 M solution of Co(I1) nitrate (Merck) following a procedure described in Ref. [ 151. The catalyst prepared by the latter method had 2.1 wt% of Co. All samples were dried overnight at 403 K and then calcined for 2 hours at 173 K in flowing nitrogen and reduced in a flow of 10% H, in Nz at 773 K for 8 hours. Zeolite-supported Co catalyst was synthesized by solid-state ion exchange using the procedure described by Kucherov and SlinkinC16, 171. COO
*To whom all correspondence should be addressed. +Permanent address: Laboratory of Organic Catalysis, Chemistry Department, Moscow State University, 119899, Moscow, Russia. 15
zyxwvutsr zyxwvu zyxwv V.IVANOV et al.
was mixed in an agath morter with HY zeolite. The product was pressed, crushed, dried overnight at 403 K and calcined in air for 1 hour at 793 K, then for 1 hour at 1073 K and after cooling for 30 minutes in flowing nitrogen, the catalyst was reduced in a flow of 10% H2 in N2 for 3 hours at 673K. The concentration of COO was calculated in order to obtain 8 wt% of Co in the zeolite. The list of studied catalysts and some characteristics are given in Table 1. The samples were examined before and after catalysis by SEM (Philips XL 20) and HREM by both a JEOL 200 CX operating at 200 kV and a JEOL 4000 EX operating at 40OkV. The specimens for TEM were either directly glued on copper grids or dispersed in acetone by ultrasound, then dropped on the holey carbon grids. 'H-NMR studies were performed on a Bruker MSL-400 spectrometer operating in the Fourier transform mode, using a static multinuclei probehead operating at 400.13 MHz. A pulse length of 1 ps is used for the IH 90"flip angle and the repetition time used (1 second) is longer than five times T,, ('H) of the analyzed samples.
ite sheets on the latter catalysts. The tubular filaments on Fe- and Co-graphite sometimes possessed wellcrystalline graphite layers. In the same growth batch we also observed a large amount of non-hollow filaments with a structure similar to that observed on Cu and Ni catalysts. In general, encapsulated metal particles were observed . on all graphite-supported catalysts. According to Ref.  it can be the result of a rather weak metal-graphite interaction. We mention the existence of two types of encapsulated metal particles: those enclosed in filaments (Fig. 1) and those encapsulated by graphite. It is interesting to note that graphite layers were parallel to the surface of the encapsulated particles. As was found in Ref. [131, the method of catalytic decomposition of acetylene on graphite-supported catalysts provides the formation of very long (50 pm) tubes. We also observed the formation of filaments up to 60pm length on Fe- and Co-graphite. In all cases these long tubules were rather thick. The thickness varied from 40 to 100 nm. Note that the dispersion of metal particles varied in the same range. Some metal aggregates of around 500 nm in diameter were also found after the procedure of catalyst pretreatment (Fig. 2). Only a very small amount of thin (20-40 nm diameter) tubules was observed. The as-produced filaments were very strongly covered by amorphous carbon produced by thermal pyrolysis of acetylene. The amount of amorphous carbon varied with the reaction conditions. It increased with increasing reaction temperature and with the percentage of acetylene in the reaction mixture. Even in optimal conditions not less than 50% of the carbon was deposited in the form of amorphous carbon in accordance with[ 131. As it was established by Geus et aL[l8, 191 the decrease of the rate of carbon deposition is a positive factor for the growth of fibres on metal catalysts. SiO, is an inhibitor of carbon condensation as was shown in Ref. . This support also provides possibilities for the stabilization of metal dispersion. Co and Fe, i.e. the metals that give the best results for the tubular condensation of carbon on graphite support, were introduced on the surface of silica gel
zyxwv zyxwvutsrq zyxwvu zy
3. RESULTS AND DISCUSSION
3.1 Catalyst support
The influence of the support on the mechanism of filament formation was previously described[1-41. The growth process was shown to be strongly dependent on the catalyst-support interaction. In the first stage of our studies we performed the acetylene decomposition reaction over graphite supported metals. This procedure was reported in Ref. [ 131 as promising to obtain a large amount of long nanotubes. The reaction was carried out in the presence of either Cu, Ni, Fe or Co supported particles. All of these metals showed a remarkable activity in filament formation (Fig. 1).The structure of the filaments was different on the various metals. We have observed the formation of hollow structures on the surface of Co and Fe catalysts. On Cu and Ni, carbon was deposited in the form of irregular fibres. The detailed observation showed fragments of turbostratic graph-
Table 1. Method of preparation and metal content of the catalysts
Sample Co-graphite F-phite Ni-graphite -aphite Co-SiO, CO-HY Co-Si0,-1 Co-Si02-2 Fe-SiO,
Poae 0 (A)
Method of preparation
Impregnation Impregnation Impregnation Impregnation Ion exchange precipitation Solid state ion exchange Pore impregnation Pore impregnation Pore impregnation
90 7.5 40
Metal (wt%) 0.5-10 2.5 2.5 2.5 2.1 8 2.5 2.5 2.5
"Measured by SEM and TEM. %e distribution of the particles was also measured (Fig. 6).
Metal particle diameteP (nm) 1Cb100 2 100 2 loo
2 loo 2-2Ob 1-50 10-100 10-100 10-100
zyxwvu zyxw 17
Catalytic production and purification of nanotubules
Fig. 1. Carbon filaments grown after acetylene decomposition at 973 K for 5 hours on (a) Co(2.5%)-graphite;(b) Fe-graphite; (c) Ni-graphite; (d) Cu-graphite.
by different methods. Both metals showed very similar catalytic behaviour. Carbon was deposited on these catalysts mostly in the form of filaments. TEM images of the tubules obtained on these catalysts are given in Fig. 3. Most of the filaments produced on silicasupported catalysts were tubular, with well-resolved graphite layers. Nevertheless non-tubular filaments also grow in these conditions. We observed that the relative quantity of well-graphitized tubules was higher on Co-silica than on Fe-silica catalyst. As in the case of graphite-supported catalysts, some metal particles were also encapsulated by the deposited carbon (Fig. 4). However, the amount of encapsulated metal was much less. Differences in the nature of encapsulation were observed. Almost all encapsulated metal particles on silica-supported catalysts were found inside the tubules (Fig. 4(a)). The probable mechanism of this encapsulation was precisely described elsewhere[ 213. We supposed that they were catalytic particles that became inactive after introduction into the tubules during the growth process. On the other hand, the formation of graphite layers around the metal in the case of graphitesupported catalysts can be explained on the basis of
models proposed earlier[4,18,22]. The metal outside of the support is saturated by the carbon produced by hydrocarbon decomposition, possibly in the form of “active” carbides. The latter then decomposes on the surface of the metal, producing graphite layers. Such a situation is typical for catalysts with a weak metal-support interaction, as in the case of graphite. The zeolite support was used to create very finely dispersed metal clusters. Metals can be localized in the solid-state exchanged zeolites in the small cages, supercages or intercrystalline spaces. In fact, in accordance with previously observed data [231, hydrogenation of as-made catalysts led to the migration of metal to the outer surface of the zeolite HY. The sizes of metal crystallites varied in our catalyst from 1 to 50 nm. We suppose that because of steric limitations only the metal particles at the outer surface and in supercages could be available for filament growth. The hydrocarbon decomposition over Co-HY provides the formation of different graphite-related structures (it should be noted that only a small amount of amorphous carbon was observed). Similar to the previous catalysts, nanotubules of various radius and metal particles encapsulated by graphite were found
Catalytic production and purification of nanotubules
Fig. 4. Catalytic particles encapsulated in tubules on Co-SO,: (a) low magnification; (b) HREM.
Fig. 5. Acetylene decomposition on Co-HY (973 K, 30 minutes): (a) encapsulated metal particle; (b) carbon filaments (A) and tubules of small diameters (B) on the surface of the catalyst.
silica catalyst synthesized by the ion-exchangeprecipitation method. This method leads to a better dispersion and a sharper size distribution than porous impregnation (Fig. 6). The rate of acetylene was varied from 0.15 to 0.59 mol C,H, g-' h-'. The amount of condensed carbon at 973 K changed as a function of hydrocarbon rate from 20 to 50 wt%
relatively. The optimal C,H, rate was found to be 0.34 mol g-' h-'. At this rate, 40-50 wt% of carbon precipitates on the catalyst surface after 30 minutes of reaction. The increase of acetylene rate leads to an increase of the -amount of amorphous carbon (equal to 2 wt% on the external walls of the tubules, for optimal conditions).
V. IVANOV et al.
ments (Fig. 7). Thus, we suppose that the formation of graphite tubules in these conditions is a very rapid process and the thermal pyrolysis leading to the formation of amorphous carbon does not have a great influence. Hence, carbon nanotubules, quasifree from amorphous carbon, are formed. 3.2.3 Reaction time. Two series of experiments were performed in order to study the influence of the reaction time on the characteristics of surface carbon structures. In the first series, the hydrocarbon deposition was periodically stopped, the catalyst was cooled down under flowing nitrogen and it was removed from the furnace. After taking a small part of the reaction mixture for TEM analysis, the remaining amount of the catalyst was put back into the furnace and the hydrocarbon deposition was further carried out under the same conditions. In the second series, different portions of catalyst were treated by hydrocarbon for different times. The results were similar for both series of catalysts. Typical images of carbon surface structures grown during different times are shown in Fig. 8. In accordance with Ref.  we observed the dependence of the rate of filament formation on the size of the catalytic particles. In the first (1 minute) reaction period, mostly very thin carbon filaments were observed as grown on the smallest metal particles. These filaments were very irregular and the metal particles were generally found at the tips of the fibres. With increasing reaction time the amount of well-graphitized tubules progressively increased. At the same time the average length of the nanotubules increased. We need, however, to note that a relation exists between the lengths of the tubules and their diameters. The longest tubules are also the thickest. For instance, the tubules of 3&60 pm length have diameters of 35-40 nm corre-
zyxwvutsrqp zyxwvutsrqp zyxwvuts 6-9
Fig. 6. Sizedistribution of metal crystallites on the surface of Co-silica made by precipitation-ionexchangemethod.
3.2.2 Reaction temperature. The reaction temperature was vaned in the range 773-1073K. The formation of filament structures was observed at all studied temperatures. As has already been mentioned, the graphitization of carbon into the tubular structures on metal-supported catalysts is generally accompanied by the formation of amorphous carbon. Both processes are temperature dependent. The filaments grown at low temperature (773 K) are relatively free of amorphous carbon. The amount of amorphous carbon increases with increasing temperature and represents about 10% of all carbon condensed on the external surface of the catalyst at 973 K. However, crystallinity of the graphite layers in tubules also strongly depends on the reaction temperature being the lowest at low temperature. The average length of the tubules is not strongly influenced by temperature. However, the amorphous carbon on the outer layers of filaments produced under optimal conditions is often deposited in frag-
Fig.7. Graphite nanotubule on Co-SiO, with the fragments of amorphous carbon (arrowed) at the external surface.
zyxwvutsrqpo zyxwvut V. IVANOVet al.
after cooling and reheating the carbon deposited sample. Metal particles even found near the tips of the tubules were always covered by graphite layers. It supports the model of an “extrusion” of the carbon tubules from the surface of active particles . 3.2.4 Injuence of hydrogen. The influence of the presence of hydrogen in the reaction mixture on the formation of nanofibres has been shown in various papersC1-3, 18, 25, 261. It was postulated that the presence of H2 decreases the rate of hydrocarbon decomposition and as a result favours the process of carbon polycondensation over the production of filaments. However, the addition of hydrogen into the mixture of acetylene and nitrogen did not give major effects on the tubule formation in our case. We suppose that the activity of metal nanoparticles on our Co-SiO, catalyst was high enough to provide filament formation without hydrogen addition. It differs from the previous investigations, which were
performed on metal-supported catalysts with larger and, thus, less active metal aggregates. It is also important to point out that pure cobalt oxide, alone or finely dispersed in SiO, (i.e. Co-SiO,, Co-SO,-1 and Co-Si02-2 in Table l), zeolite HY, fullerene (i.e. C60/C70: 80/20) is at least as effective as the reduced oxides for the production of nanotubules in our experimental conditions. In fact, the catalysts studied in this work are also active if the hydrogenation step is not performed. This important point, is presently being investigated in our laboratory in order to elucidate the nature of the active catalyst (probably a metal carbide) for the production of nanotubules.
3.3 The amount of hydrogen injlaments
As it can be observed from the high resolution images of tubules (Fig. 9(a)) their graphitic structure is generally defective. The defects can be of different
Fig. 9. Carbon nanotubules on Co-SO,: (a) HREM image showing defects in tubules;(b) helical tubules of various pitches between the straight tubules.
zyxwv zyxwv zyxwvutsr zyxwvuts zyxwvu 23
Catalytic production and purification of nanotubules
Table 2. Hydrogen
content measured ‘H-NMR
Coronene (reference) Catalyst Co-SiO, Evacuated catalyst Co-SiO, Carbonated catalyst CoSiO, Evacuated carbonated catalyst Co-SiO,
T,, (‘H)” (ms)
520 20 960 50 160
4.03 1.33 0.26 1.80 1.26b
with the increase of reaction temperature. The free valencies of carbon in such defects can be compensated by the formation of C-H bonds. The carbon layers produced on the surface of silica-supported catalysts after hydrocarbon decomposition always have chemically bonded hydrogen (up to 2 wt% in some cases). We performed a quantitative ‘H-NMR study using coronene (Cz4Hlz) as external standard. The ‘HNMR spectra of the catalyst samples before and after reaction are given in Fig. 10. The static proton spectrum gives a broad band at 6.9ppm similar to that obtained on the reference sample (7.2 ppm). The sharp proton band at 7.9 ppm before the catalysis can be related to the small amount of hydroxyl groups still remaining on the surface of silica after temperature treatment before reaction. This amount was taken into account in the calculations of the hydrogen content in carbon species on the surface (Table 2). The total quantity of hydrogen is approximately 2 wt%. This amount can be sufficient to saturate all free carbon vacancies in sp3 defects of graphitic structure.
”‘H longitudinal relaxation time, measured by the inversion-recovery technique, at 293 K. bAs 50 wt% of hydrocarbons are deposited on the catalyst, the hydrogen content of the hydrocarbons is: 2( 1.26-0.13) ~ 2 . 2 wt%. 6
natures. The most interesting ones are regular defects leading to the formation of helices. The helical tubules are 6-10% of the total amount of filaments as estimated from the microscopy observations (Fig. 9(b)). The mechanism of helices formation was discussed elsewhereC271 and a model based on the regular introduction of pentagon-heptagon pairs was proposed. The presence of stress causes the formation of “kinks” in the graphite layers. This kind of defect was also well describedC211. There are also defects in the graphite layers, which are typical for turbostratic graphite. We already mentioned that the formation of these kinds of defect strongly decreases
3.4 Gas$cation of nanotubes
The carbon deposited catalysts were treated both by oxidation and hydrogenation at temperatures in the range of 873-1173 K for various exposure times. Some results of oxidation treatment are presented in
Fig. 10. ‘H NMR spectra: (a) coronene; (b) Co-SiO, covered by carbon nanotubules; (c) Co-SiO, covered by carbon nanotubules and evacuated to torr for the NMR measurement; (d) Co-SiO, torr for the NMR measurement. evacuated to
zyxwvuts zyxwvut zyxwv
V. IVANOV et al.
Fig. 11. Tips of carbon nanotubules grown on Co- SiO, (acetylene reaction at 973 K, 30 minutes after oxidation in air for 30 minutes at 873, K: (a) low magnification; (b) HREM.
Fig. 11. The loss of carbon rapidly increases with the increase of temperature. Heating of the catalysts in open air for 30 minutes at 973 K leads to the total elimination of carbon from the surface. The gasification of amorphous carbon proceeds more rapidly than that of filaments. The tubules obtained after oxidation of carbon-deposited catalysts during 30 minutes at 873 K are almost free from amorphous carbon. The process of gasification of nanotubules on the surface of the catalyst is easier in comparison with the oxidation of nanotubes containing soot obtained by the arc-discharge method C28, 291. This can be easily explained, in agreement with Ref. , by the surface activation of oxygen of the gaseous phase on Co-SiO, catalyst. The gasification of graphite layers proceeds more easily at the tips of the tubules and at structural defects. Typical images of the tips of catalytically produced tubules after treatment in air are presented in Fig. 11. On graphite tubules grown from Co-SiO, catalyst, two types of tip were usually observed. In the first, the tubules are closed by graphite layers with the metal particle inside the tubules (Fig. 4(a)). In the second type, more generally observed, the tubules are closed with amorphous carbon. The opening of tubules during oxidation could proceed on both types of tip. The gasification of carbon filaments by hightemperature hydrogen treatment was postulated as involving the activation of hydrogen on the metal surfaceC31-331. We observed a very slight effect of catalyst hydrogenation, which was visible only after the treatment of carbon-deposited catalyst for 5 hours at 1173 K. We suppose that the activation of hydrogen in our case could proceed on the noncovered centers of Co or, at very high temperatures, it could be thermal dissociation on the graphite surface layers of tubules. The result was similar to that of oxidation but the process proceeded much slower. We called it “gentle” gasification and we believe that this method of thinning of the nanotu-
bules could be preferable in comparison with oxidation, because of the easier control in the former case.
3.5 Product purijication For the physico-chemical measurements and practical utilisation in some cases the purification of nanotubules is necessary. In our particular case, purification means the separation of filaments from the substrate-silica support and Co particles. The carbon-containing catalyst was treated by ultra-sound (US) in acetone at different conditions. The power of US treatment, and the time and regime (constant or pulsed), were varied. Even the weakest treatments made it possible to extract the nanotubules from the catalyst. With the increase of the time and the power of treatment the amount of extracted carbon increased. However, we noticed limitations of this method of purification. The quantity of carbon species separated from the substrate was no more than 10% from all deposited carbon after the most powerful treatment. Moreover, the increase of power led to the partial destruction of silica grains, which were then extracted with the tubules. As a result, even in the optimal conditions the final product was never completely free of silica (Fig. 12). For better purification, the tubule-containing catalyst was treated by H F (40%) over 72 hours. The resulting extract was purer than that obtained after US treatment. The addition of nitric acid also makes it possible to free the tubules of metal particles on the external surface. The conditions of the acid treatment and tubule extraction have yet to be optimized. 4. CONCLUSIONS
In this study we have shown that the catalytic method-carbon deposition during hydrocarbons conversion-can be widely used for nanotubule production methods. By variation of the catalysts and reaction conditions it is possible to optimize the process towards the preferred formation of hollow
Catalytic production and purification of nanotubules
Fig. 12. Carbon nanotubules after separation from the substrate by ultra-sound treatment. Note the SiO, grains attached to the tubules.
carbon filaments. The deposited carbon in these filaments has a graphitic structure, i.e. the as-made tubules can be assumed to be analogous to the tubules obtained by the arc-discharge fullerene production. By the use of catalysts with very finely dispersed metal or metal oxide particles on the surface, it was possible to produce nanotubules having diameters of the same range as nanotubules obtained by the arc-discharge method. We can thus suppose that the former tubules will possess all the properties predicted for the fullerene tubules. The catalytic method, as was shown in this study, has some advantages over arc-discharge tubule production. First, the yield of nanotubules in the catalytic production is higher than in the arc-discharge. It is possible to optimize the method for the deposition of almost all of the carbon in the form of tubular filaments. In the arc-discharge production the amount of tubules in the soot is usually no more than 25%. Isolation of panotubules is also easier in the case of catalytic production. They can be separated from the substrate by the combination of various methods (ultra-sound treatment, chemical treatment). The high percentage of tubules in the product (only tubules are seen by TEM on the catalyst surface) makes possible their effective purification by gasification, either by oxidation or hydrogenation. The former treatment can also be used for the opening of nanotubules. The characteristics of nanotubules obtained by catalytic reaction are better controlled than in the arc-discharge method. By varying the active particles on the surface of the catalyst the nanotubule diameters can be adjusted. The length of the tubules is
dependent on the reaction time; very long tubules, even up to 60 pm, can be produced. The catalytic method provides the basis for synthesis of carbon tubules of a large variety of forms. Straight tubules, as well as bent and helically wound tubules, were observed. The latter regular helices of fullerene diameter can be of special interest from both theoretical and practical points of view.
Acknowledgements-This text presents research results of the Belgian Programme on Inter University Poles of Attraction initiated by the Belgian State Prime Minister’s Office of Science Policy Programming. The scientific responsibility is assumed by the authors. A. Fonseca and D. Bernaerts acknowledge, respectively, the Rbgion Wallonne and the National Found for Scientific Research, for financial support. Thanks are due to Prof. G. Van Tendeloo and Prof. J. Van Landuyt for useful discussions and for their continued interest in this research.
zy zyxwvutsrq REFERENCES
1. A. Sacco, Jr, F. W. A. H. Geurts, G. A. Jablonski, S. Lee and R. A. Gately, J. Catal 119, 322 (1989). 2. G. A. Jablonski, F. W. Geurts and A. Sacco, Jr, Carbon 30, 87 (1992). 3. P. E. Nolan and D. C. Lynch, Carbon 32,477 (1994). 4. R. T. K. Baker, Carbon 27, 315 (1989). 5. N. M. Rodriguez, J. Mater. Res. 8, 3233 (1993). 6. A. Oberlin, M. Endo and T. Koyama, J. Cryst. Growth 32, 335 (1976). 7. S. Iijima, Nature 354, 56 (1991). 8. R. E. Smalley, Proc. R. A. Welch Found. Conf. Chem. Res. XXXVI, Houston, Texas, 26-27 October 1992, p. 161. 9. M. R. Pederson and J. Q. Broughton, Phys. Rev. Lett. 69,2689 (1992). 10. J. W. Mintmire, B. I. Dunlap and C. T. White, Phys. Rev. Lett. 68, 631 (1992).
zyxwvut zyxwv zyxwvutsr zyxwvutsrq zyxwvz zyxwvuts V. IVANOV et al.
11. N. Hamada, S. Sawada and A. Oshiyama, Phys. Rev. Lett. 68, 1579 (1992). 12. K. Harigaya and M. Fujita, Phys. Ret.. B47, 16563 (1993). 13. M. JosC-Yacaman, M. Miki-Yoshida, L. Rendon and J. G. Santiesteban, PhYs. Lett. 62, 657 (1993). 14. V. Ivanov, J. B. Nagy, P. Lambin, A. Lucas, X. B. Zhang, F. Zhang, D. Bernaerts, G. Van Tendeloo, s. inckx and J. Van Landuyt, Chem. Phys. Lett. 223, 329 (1994). 15. J. C. Lee, D. L. Trimm, M. A. Kohler, M. S. Wainwright and N. W . Cant, Catal. Today 2,643 (1988). 16. A. V. Kucherov and A A. Slinkin, Zeolites 6,175 (1986). 17. A. V. Kucherov and A. A. Slinkin, Zeolites 7,38 (1987). 18. A. J. H.M. KO&, p. K. de Bokx, E. Boellard, W, Klop and J. W. Geus, J. Catal. 96,468 (1985). 19. J. W. Geus, private communication. 20. R. T. K. Baker and J. J. Chludzinski, Jr, J. Catal. 64, 464 (1980). 21. D. Bernaerts, X. B. Zhang X. F. Zhang, G. Van Tendeloo, S . Amelinckx, J. Van Landuyt, V. Ivanov and J. B. Nagy, Phil. Mag. 71, 605 (1995). 22. L. S. Lobo and M. D. Franco, Catal. Today 7, 247 (1990).
23. A. A. Slinkin, M. I. Loktev, I. V. Michin, V. A. Plachotnik, A. L. Klyachko and A. M. Rubinstein, Kinet. Katal. 20, 181 (1979). 24. S. Amelinckx, X. B. Zhang, D. Bernaerts, X. F. Zhang, v. Ivanov and J. B,Nagy, Science, 265, 635 (1995). 25. M. S. Kim, N. M. Rodriguez and R. T. K. Baker, J. Catal. 131,60 (1991). 26. A. Sacco, P. Thacker, T. N. Chang and A. T. S. Chiang, J. catal, 85, 224 (1984). 27. X. B. Zhang, X. F. Zhang, D. Bernaerts, G. Van TendeJ, Van v. Ivanov, J, B. loo, s. Nagy, Ph. Lambin and A. A. Lucas, Europhys. Lett. 27, 141 (1994). 28. p* M. Ajayan, T. w- Ebbesen, T. Ichihashis. Iijim% K. Tanigaki and H. Hiura, Nature 362, 522 (1993). 29. T. W. Ebbesen, P. M. Ajayan, H. Hiura and K. Tanigaki, Nature 367, 519 (1994). 30. R. T. K. Baker and R. D. Sherwood, J. Catal. 70; 198 (1981)31. A. Tomita and y. Tamai, J. Catal. 27,293 (1972). 32. A. Tomita and Y. T a m 6 J. Phys. Chem. 78,2254 (1974). 33. J. L. Figueiredo, C. A. Bernardo, J. J. Chludzinski and R. T. K. Baker, J. Cutal. 110, 127 (1988).
PHYSICS OF CARBON NANOTUBES
M. S . DRESSELHAUS,’ G. DRESSELHAUS,* and R. SAITO~
‘Department of Electrical Engineering and Computer Science and Department of Physics, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, U.S.A. ’Francis Bitter National Magnet Laboratory, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, U.S.A. ‘Department of Electronics-Engineering,University of Electro-Communications, Tokyo 182, Japan
(Received 26 October 1994; accepted 10 February 1995)
Abstract-The fundamental relations governing the geometry of carbon nanotubes are reviewed, and explicit examples are presented. A framework is given for the symmetry properties of carbon nanotubes for both symmorphic and non-symmorphic tubules which have screw-axissymmetry. The implications of symmetry on the vibrational and electronic structure of ID carbon nanotube systems are considered. The corresponding properties of double-wall nanotubes and arrays of nanotubes are also discussed. Key Words-Single-wall, multi-wall, vibrational modes, chiral nanotubes, electronic bands, tubule arrays.
governing these parameters, and list typical numerical values for these parameters. In the theoretical carbon nanotube literature, the focus is on single-wall tubules, cylindrical in shape with caps at each end, such that the two caps can be joined together to form a fullerene. The cylindrical portions of the tubules consist of a single graphene sheet that is shaped to form the cylinder. With the recent discovery of methods to prepare single-walled nanotubes[4,5], it is now possible to test the predictions of the theoretical calculations. It is convenient to specify a general carbon nanotubule in terms of the tubule diameter d, and the chiral angle 0, which are shown in Fig. 1. The chiral vector C h is defined in Table 1 in terms of the integers (n,rn) and the basis vectors a, and a2 of the honeycomb lattice, which are also given in the table in terms of rectangular coordinates. The integers (n,m ) uniquely determine dr and 0. The length L of the chiral vector c, (see Table 1) is directly related to the tubule diameter &. The chiral angle 0 between the Ch direction and the zigzag direction of the honeycomb lattice (n,O) (see Fig. 1) is related in Table 1 to the integers ( n , m ) . We can specify a single-wall C,,-derived carbon nanotube by bisecting a Cm molecule at the equator and joining the two resulting hemispheres with a cylindrical tube having the same diameter as the C60 molecule, and consisting of the honeycomb structure of a single layer of graphite (a graphene layer). If the C6, molecule is bisected normal to a five-fold axis, the “armchair” tubule shown in Fig. 2 (a) is formed, and if the C,, molecule is bisected normal to a 3-fold axis, the “zigzag” tubule in Fig. 2(b) is formed. Armchair and zigzag carbon nanotubules of larger diameter, and having correspondingly larger caps, can likewise be defined, and these nanotubules have the general appearance shown in Figs. 2(a) and (b). In addition, a large number of chiral carbon nanotubes can be formed for 0 < 10 1 < 30°, with a screw axis along
Carbon nanotube research was greatly stimulated by the initial report of observation of carbon tubules of nanometer dimensions[l] and the subsequent report on the observation of conditions for the synthesis of large quantities of nanotubes[2,3]. Since these early reports, much work has been done, and the results show basically that carbon nanotubes behave like rolled-up cylinders of graphene sheets of sp2 bonded carbon atoms, except that the tubule diameters in some cases are small enough to exhibit the effects of one-dimensional(1D) periodicity. In this article, we review simple aspects of the symmetry of carbon nanotubules (both monolayer and multilayer) and comment on the significance of symmetry for the unique properties predicted for carbon nanotubes because of their 1D periodicity. Of particular importance to carbon nanotube physics are the many possible symmetries or geometries that can be realized on a cylindrical surface in carbon nanotubes without the introduction of strain. For 1D systems on a cylindrical surface, translational symmetry with a screw axis could affect the electronic structure and related properties. The exotic electronic properties of 1D carbon nanotubes are seen to arise predominately from intralayer interactions, rather than from interlayer interactions between multilayers within a single carbon nanotube or between two different nanotubes. Since the symmetry of a single nanotube is essential for understanding the basic physics of carbon nanotubes, most of this article focuses on the symmetry properties of single layer nanotubes, with a brief discussion also provided for two-layer nanotubes and an ordered array of similar nanotubes.
zyxwvutsr zyx zy zyxw zyxwv
2. FUNDAMENTAL PARAMETERS AND RELATIONS FOR CARBON NANOTUBES
In this sect.ion, we summarize the fundamental parameters for carbon nanotubes, give the basic relations 27
M. S. DRESSELHAUS ef al.
Fig, 3. The 2D graphene sheet is shown along with the vector which specifies the chiral nanotube. The pairs of integers (n,rn) in the figure specify chiral vectors Ch (see Table 1) for carbon nanotubes, including Zigzag, armchair, and chiral tubules. Below each pair of integers (n,rn)is listed the number of distinct caps that can be joined continuously to the cylindrical carbon tubule denoted by ( n , m ) [ 6 ]The . circled dots denote metallic tubules and the small dots are for semiconducting tubules.
zyxwvutsrqp zyxwvutsrqp zyxwvutsrq zyxwvutsrq zyxwvutsrq
Fig. 1. The 2D graphene sheet is shown along with the vector which specifies the chiral nanotube. The chiral vector OA or C, = nu, ma, is defined on the honeycomb lattice by unit vectors a , and u2 and the chiral angle 6 is defined with respect to the zigzag axis. Along the zigzag axis 6 = 0”. Also shown are the lattice vector OB = T of the 1D tubule unit cell, and the rotation angle $ and the translation T which constitute the basic symmetry operation R = ($1 7 ) . The diagram is constructed for (n,rn) = (4,2).
the axis of the tubule, and with a variety of hemispherical caps. A representative chiral nanotube is shown in Fig. 2(c). The unit cell of the carbon nanotube is shown in Fig. 1 as the rectangle bounded by the vectors Ch and T, where T is the ID translation vector of the nanotube. The vector T is normal to Ch and extends from
Fig. 2. By rolling up a graphene sheet (a single layer of carbon atoms from a 3D graphite crystal) as a cylinder and capping each end of the cylinder with half of a fullerene molecule, a “fullerene-derivedtubule,” one layer in thickness, is formed. Shown here is a schematic theoretical model for a single-wall carbon tubule with the tubule axis OB (see Fig. 1) normal to: (a) the 0 = 30” direction (an “armchair” tubule), (b) the 0 = 0” direction (a “zigzag” tubule), and (c) a general direction B with 0 < 16 I < 30” (a “chiral” tubule). The actual tubules shown in the figure correspond to ( n , m )values of: (a) ( 5 , 5 ) , (b) (9,0),and (c) (10,5).
the origin to the first lattice point B in the honeycomb lattice. It is convenient to express T in terms of the integers ( t ,,f2) given in Table 1, where it is seen that the length of T is &L/dR and dR is either equal to the highest common divisor of (n,rn), denoted by d , or to 3d, depending on whether n - rn = 3dr, r being an integer, or not (see Table 1). The number of carbon atoms per unit cell n, of the 1D tubule is 2N, as given in Table 1, each hexagon (or unit cell) of the honeycomb lattice containing two carbon atoms. Figure 3 shows the number of distinct caps that can be formed theoretically from pentagons and hexagons, such that each cap fits continuously on to the cylinders of the tubule, specified by a given ( n , m ) pair. Figure 3 shows that the hemispheres of C,, are the smallest caps satisfying these requirements, so that the diameter of the smallest carbon nanotube is expected to be 7 A, in good agreement with experiment[4,5]. Figure 3 also shows that the number of possible caps increases rapidly with increasing tubule diameter. Corresponding to selected and representative (n,rn) pairs, we list in Table 2 values for various parameters enumerated in Table 1, including the tubule diameter d,, the highest common divisors d and dR, the length L of the chiral vector Ch in units of a (where a is the length of the 2D lattice vector), the length of the 1D translation vector T of the tubule in units of a, and the number of carbon hexagons per 1D tubule unit cell N . Also given in Table 2 are various symmetry parameters discussed in section 3 . 3. SYMMETRY OF CARBON NANOTUBFS
zyxwvu zyxwvut In discussing the symmetry of the carbon nanotubes, it is assumed that the tubule length is much larger than its diameter, so that the tubule caps can be neglected when discussing the physical properties of the nanotubes. The symmetry groups for carbon nanotubes can be either symmorphic [such as armchair (n,n)and zigzag
zyx zyxw zyx zyxw
Physics of carbon nanotubes
Table 1. Parameters of carbon nanotubes Symbol ___
1.421 *4 (graphite) 2.46 A
carbon-carbon distance length of unit vector
unit vectors reciprocal lattice vectors
Ch = na,
+ ma2 = ( n , m )
n, m : integers
circumference o f nanotube
L = /C,I= u J n ~ + m 2 + n m
diameter of nanotube
+m + m2 + nm
cos 0 =
tan 0 = 2n + m
the highest common divisor of ( n ,m ) the highest common divisor of (2n m,2m n )
translational vector of 1D unit cell
m not a multiple of 3d
m a multiple of 3d.
T = t,a,
+ f2a2 = (11,12) +n
t , , t,: integers
zyxwvutsrq t, =
1, = -~
aL T= -
length of T
+ in2+ nm)
2 N = n,/unit
number of hexagons per 1D unit cell
R = p a , + qa2 = ( n q ) d = m p - nq, 0 5 p s n/d, 0 5 q 5 m/d M = [(2n + m ) p ( 2 m n ) q ] / d , N R = MCh dT
number of 2 n revolutions
p , q : integers? M: integer
basic symmetry operation$ rotation operation
t ( p , q ) are uniquely determined by d = m p - nq, subject to conditions stated in table, except for zigzag tubes for which C, = (n,O), and we definep = 1, q = -1, which gives M = 1. $ R and R refer to the same symmetry operation.
(n,O) tubules], where the translational and rotational symmetry operations can each be executed independently, or the symmetry group can be non-symmorphic (for a general nanotube), where the basic symmetry operations require both a rotation $ and translation r and is written as R = ( $ 1 r). We consider the symmorphic case in some detail in this article, and refer the reader to the paper by Eklund et al. in
this volume for further details regarding the nonsymmorphic space groups for chiral nanotubes. The symmetry operations of the infinitely long armchair tubule ( n = m), or zigzag tubule (rn = 0), are described by the symmetry groups Dnh or Dnd for even or odd n, respectively, since inversion is an element of Dnd only for odd n , and is an element of Dnh only for even n . Character tables for the D, groups
zyxwvutsrqp zyxwvut zyxwv zyxwv zyxwvut zy zyxwvu zyxw zyxwvuts M. S. DRESSELHAUS et ai.
Table 2. Values for characterization parameters for selected carbon nanotubes labeled by (n,rn)
5 9 1 1 1 10
15 9 1 3 1 10 18 5 15 15
6.78 7.05 7.47 1.55 7.72 7.83 8.14 10.36 17.95 31.09
6 5 5
m J93 m 10 m 6175 6525
m fin n
Table 3. Character table for group D(u+l,
1 2 2
1 ... 1 1 1 1 1 ... 2 ~ 0 ~ 2 6~ ~0 ~ 2. . 6. 2~c o ~ j 6 ~ 2 c 0 s 2 + ~ 2 ~ 0 ~ 4. .4. 2~c 0 s 2 j + ~
2cos2j6, . . . 2cos j2c+5j
+ 1) and j is an integer
m m m 43
are given in Table 3 (for odd n = 2 j 1) and in Table 4 (for even n = 2 j ) , wherej is an integer. Useful basis functions are listed in Table 5 for both the symmorphic groups (D2jand DzJ+,)and non-symmorphic groups C,,, discussed by Eklund ef al. . Upon taking the direct product of group D, with the inversion group which contains two elements ( E ,i), we can construct the character tables for Dnd= D , @ i from Table 3 to yield D,,, D,,, . . .for symmorphic tubules with odd numbers of unit cells around the circumference [(5,5), (7,7), . . . armchair tubules and (9,0),(ll,O), . . . zigzag tubules]. Likewise, the character table for Dnh= 0, @ ah can be obtained from Table 4 to yield D6h,Dsh,. . . for even n. Table 4 shows two additional classes for group D, relative to group D ( z J + l )because , rotation by .rr about the main symmetry axis is in a class by itself for groups D 2 j .Also the n two-fold axes nC; form a class and represent two-fold rotations in a plane normal to the main symmetry axis C,, , while the nCi dihedral axes, which are bisectors of the nC; axes, also form a class for group D,, when n is an even integer. Correspondingly, there are two additional one-dimensional representations B, and B2 in DZi corresponding to the two additional classes cited above. The symmetry groups for the chiral tubules are Abelian groups. The corresponding space groups are non-symmorphic and the basic symmetry operations
( 2 j + 1)C; 1 -1 0 0
10 18 182 62 194 20 12 70 70 210
1/10 1/18 149/ 182 11/62 71/194 1/20 1/12 1/14 3/70 1/42
631388 v3/2 1/ 2
1 1 149 17 11 1 1 5
R = ($1 T ) require translations T in addition to rotations $. The irreducible representations for all Abelian groups have a phase factor E , consistent with the requirement that all h symmetry elements of the symmetry group commute. These symmetry elements of the Abelian group are obtained by multiplication of the symmetry element R = ( $ IT) by itself an appropriate number of times, since R h = E , where E is the identity element, and h is the number of elements in the Abelian group. We note that N,the number of hexagons in the 1D unit cell of the nanotube, is not always equal h, particularly when d # 1 and dR # d. To find the symmetry operations for the Abelian group for a carbon nanotube specified by the (n,rn) integer pair, we introduce the basic symmetry vector R = p a , qa,,. shown in Fig. 4, which has a very important physical meaning. The projection of R on the Ch axis specifies the angle of rotation $ in the basic symmetry operation R = ( 3 I T ) , while the projection of R on the T axis specifies the translation 7 . In Fig. 4 the rotation angle $ is shown as x = $L/2n. If we translate R by ( N / d ) times, we reach a lattice point B" (see Fig. 4). This leads to the r e l a t i o n m =MCh + dT where the integer M is interpreted as the integral number of 27r cycles of rotation which occur after N rotations of $. Explicit relations for R, $, and T are contained in Table 1. If d the largest common divisor of (n,rn) is an integer greater than I , than ( N / d )translations of R will translate the origin 0 to a lattice point B", and the projection (N/d)R.T = T 2 .The total rotation angle $then becomes 2.rr(Mld)when ( N / d ) R reaches a lattice point B". Listed in Table 2 are values for several representative carbon nanotubes for the rotation angle $ in units of 27r, and the translation length T in units of lattice constant a for the graphene layer, as well as values for M . From the symmetry operations R = ( 4I T ) for tubules (n,rn), the non-symmorphic symmetry group of the chiral tubule can be determined. Thus, from a symmetry standpoint, a carbon tubule is a onedimensional crystal with a translation vector T along the cylinder axis, and a small number N of carbon
zyxwv zyxwvutsrqpon zyxwvuts zyxwvutsrqpon zyxwvutsrqponmlkji zyx zyx zyxwvutsrqponm zyxwvutsrqp 31
Physics of carbon nanotubes
AI A2 Bl
1 1 1
2 2 2
-1 -1 -2 2
1 1 1 2 cos Gj 2 cos 2Gj
2 c o s ( j - l)bj
1 1 2 cos 24j 2 cos 4+j
... ... ...
2cos(j- l)+j 2COS2(j - l ) + j
1 0 0
2 c o s ( j - l)2+j
where $, = 27r/(2j) and j is an integer.
hexagons associated with the 1D unit cell. The phase factor E for the nanotube Abelian group becomes E = exp(27riM/N for the case where ( n , m )have no common divisors (i-e., d = 1). If M = 1, as for the case of zigzag tubules as in Fig. 2(b) NR reach a lattice point after a 2n rotation. As seen in Table 2, many of the chiral tubules with d = 1 have large values for M ; for example, for the (6J) tubule, M = 149, while for the (7,4) tubule, M = 17. Thus, many 2~ rotations around the tubule axis are needed in some cases to reach a lattice point of the 1D lattice. A more detailed discussion of the symmetry properties of the non-symmorphic chiral groups is given elsewhere in this volume. Because the 1D unit cells for the symmorphic groups are relatively small in area, the number of phonon branches or the number of electronic energy bands associated with the 1D dispersion relations is relatively small. Of course, for the chiral tubules the 1D unit cells are very large, so that the number of phonon branches and electronic energy bands is aIso large. Using the transformation properties of the atoms within the unit cell (xatom ’IfeS ) and the transformation properties of the 1D unit cells that form an Abelian group, the symmetries for the dispersion relations for phonon are obtained[9,10]. In the case of n energy bands, the number and symmetries of the distinct energy bands can be obtained by the decomposition of the equivalence transformation (xatom sites) for the atoms for the ID unit cell using the irreducible representations of the symmetry group.
We illustrate some typical results below for electrons and phonons. Closely related results are given elsewhere in this volume[8,1 I]. The phonon dispersion relations for (n,O)zigzag tubules have 4 x 3 n = 12n degrees of freedom with 60 phonon branches, having the symmetry types (for n odd, and Dndsymmetry):
Of these many modes there are only 7 nonvanishing modes which are infrared-active (2A2, + 5E1,) and 15 modes that are Raman-active. Thus, by increasing the diameter of the zigzag tubules, modes with different symmetries are added, though the number and symmetry of the optically active modes remain the
Table 5 . Basis functions for groups D ( 2 , )and Do,+,,
Fig. 4. The relation between the fundamental symmetry vector R = p a , + qaz and the two vectors of the tubule unit cell for a carbon nanotube specified by ( n , m )which, in turn, determine the chiral vector C , and the translation vector T . The projection of R on the C,, and T axes, respectively, yield (or x) and T (see text). After ( N / d )translations, R reaches a lattice point B”. The dashed vertical lines denote normals to the vector C, at distances of L/d, X / d , 3L/d,. . . ,L from the origin.
zyxwv zyxw zyxwv zyxwvutsrq
zyxwvut zyxwv M. S. DRESSZLHAUS et a/.
same. This is a symmetry-imposed result that is generally valid for all carbon nanotubes. Regarding the electronic structure, the number of energy bands for (n,O)zigzag carbon nanotubes is 2n, the number of carbon atoms per unit cell, with symmetries
search directions. The multi-wall calculations have been predominantly done for double-wall tubules, although some calculations have been done for a fourwalled tubule[16-18] and also for nanotube arrays [ 16,171. The first calculation for a double-wall carbon nanotube[l5] was done using the tight binding technique, which sensitively includes all symmetry constraints in a simplified Hamiltonian. The specific geometrical arrangement that was considered is the most commensurate case possible for a double-layer nanotube, for which the ratio of the chiral vectors for the two layers is 1:2, and in the direction of translational vectors, the ratio of the lengths is 1:1. Because the C60-derivedtubule has a radius of 3.4 A, which is close to the interlayer distance for turbostratic graphite, this geometry corresponds to the minimum diameter for a double-layer tubule. This geometry has many similarities to the AB stacking of graphite. In the double-layer tubule with the diameter ratio 1:2, the interlayer interaction y1 involves only half the number of carbon atoms as in graphite, because of the smaller number of atoms on the inner tubule. Even though the geometry was chosen to give rise to the most commensurate interlayer stacking, the energy dispersion relations are only weakly perturbed by the interlayer interaction. More specifically, the calculated energy band structure showed that two coaxial zigzag nanotubes that would each be metallic as single-wall nanotubes yield a metallic double-wall nanotube when a weak interlayer coupling between the concentric nanotubes is introduced. Similarly, two coaxial semiconducting tubules remain semiconducting when the weak interlayer coupling is introduced[l5]. More interesting is the case of coaxial metal-semiconductor and semiconductormetal nanotubes, which also retain their individual metallic and semiconducting identities when the weak interlayer interaction is turned on. On the basis of this result, we conclude that it might be possible to prepare metal-insulator device structures in the coaxial geometry without introducing any doping impurities, as has already been suggested in the literature[10,20,21]. A second calculation was done for a two-layer tubule using density functional theory in the local density approximation to establish the optimum interlayer distance between an inner ( 5 3 ) armchair tubule and an outer armchair (10,lO) tubule. The result of this calculation yielded a 3.39 A interlayer separation [16,17], with an energy stabilization of 48 meV/carbon atom. The fact that the interlayer separation is about halfway between the graphite value of 3.35 A and the 3.44 A separation expected for turbostratic graphite may be explained by interlayer correlation between the carbon atom sites both along the tubule axis direction and circumferentially. A similar calculation for double-layered hyper-fullerenes has also been carried out, yielding an interlayer spacing of 3.524 A for C60@C240with an energy stabilization of 14 meV/C atom for this case. In the case of the doublelayered hyper-fullerene, there is a greatly reduced pos-
A symmetry-imposed band degeneracy occurs for the and E E ( ~ bands - ~ , ~at ~the~ Fermi level, when n = 3r, r being an integer, thereby giving rise to zero gap tubules with metallic conduction. On the other hand, when n # 3r, a bandgap and semiconducting behavior results. Independent of whether the tubules are conducting or semiconducting, each of the [4 + 2(n -1)J energy bands is expected to show a ( E - Eo)-1’2type singularity in the density of states at its band extremum energy Eo[ 101. The most promising present technique for carrying out sensitive measurements of the electronic properties of individual tubules is scanning tunneling spectroscopy (STS) becaise of the ability of the tunneling tip to probe most sensitively the electronic density of states of either a single-wall nanotube[l2], or the outermost cylinder of a multi-wall tubule or, more generally, a bundle of tubules. With this technique, it is further possible to carry out both STS and scanning tunneling microscopy (STM) measurements at the same location on the same tubule and, therefore, to measure the tubule diameter concurrently with the STS spectrum. Although still preliminary, the study that provides the most detailed test of the theory for the electronic properties of the ID carbon nanotubes, thus far, is the combined STMISTS study by Olk and Heremans[ 131. In this STM/STS study, more than nine individual .multilayer tubules with diameters ranging from 1.7 to 9.5 nm were examined. The I- Vplots provide evidence for both metallic and semiconducting tubules[ 13,141. Plots of dl/dVindicate maxima in the 1D density of states, suggestive of predicted singularities in the 1D density of states for carbon nanotubes. This STM/ STS study further shows that the energy gap for the semiconducting tubules is proportional to the inverse tubule diameter lid,, and is independent of the tubule chirality. Ef+3)/21g
4. MULTI-WALL NANOTUBES AND ARRAYS
Much of the experimental observations on carbon nanotubes thus far have been made on multi-wall tubules[15-19]. This has inspired a number of theoretical calculations to extend the theoretical results initially obtained for single-wall nanotubes to observations in multilayer tubules. These calculations for multi-wall tubules have been informative for the interpretation of experiments, and influential for suggesting new re-
zyxwvuts zyxwvu zyxwvutsrq zy Physics of carbon nanotubes
sibility for interlayer correlations, even if C60 and CZmtake the same I), axes. Further, in the case of C240,the molecule deviates from a spherical shape to an icosahedron shape. Because of the curvature, it is expected that the spherically averaged interlayer spacing between the double-layered hyper-fullerenes is greater than that for turbostratic graphite. In addition, for two coaxial armchair tubules, estimates for the translational and rotational energy barriers (of 0.23 meV/atom and 0.52 meV/atom, respectively) were obtained, suggesting significant translational and rotational interlayer mobility of ideal tubules at room temperature[l6,17]. Of course, constraints associated with the cap structure and with defects on the tubules would be expected to restrict these motions. The detailed band calculations for various interplanar geometries for the two coaxial armchair tubules basically confirm the tight binding results mentioned above[ 16,171. Further calculations are needed to determine whether or not a Peierls distortion might remove the coaxial nesting of carbon nanotubes. Generally 1D metallic bands are unstable against weak perturbations which open an energy gap at EF and consequently lower the total energy, which is known as the Peierls instability. In the case of carbon nanotubes, both in-plane and out-of-plane lattice distortions may couple with the electrons at the Fermi energy. Mintmire and White have discussed the case of in-plane distortion and have concluded that carbon nanotubes are stable against a Peierls distortion in-plane at room temperature, though the in-plane distortion, like a KekulC pattern, will be at least 3 times as large a unit cell as that of graphite. The corresponding chiral vectors satisfy the condition for metallic conduction ( n - m = 3r,r:integer). However, if we consider the direction of the translational vector T, a symmetry-lowering distortion is not always possible, consistent with the boundary conditions for the general tubules. On the other hand, out-of-plane vibrations do not change the size of the unit cell, but result in a different site energy for carbon atoms on A and B sites for carbon nanotube structures. This situation is applicable, too, if the dimerization is of the “quinone” or chain-like type, where out-of-plane distortions lead to a perturbation approaching the limit of 2D graphite. Further, Harigaya and Fujita[27,28] showed that an in-plane alternating double-single bond pattern for the carbon atoms within the 1D unit cell is possible only for several choices of chiral vectors. Solving the self-consistent calculation for these types of distortion, an energy gap is always opened by the Peierls instability. However, the energy gap is very small compared with that of normal 1D cosine energy bands. The reason why the energy gap for 1D tubules is so small is that the energy gain comes from only one of the many 1D energy bands, while the energy loss due to the distortion affects all the 1D energy bands. Thus, the Peierls energy gap decreases exponentially with increasing number of energy bands N[24,26-281. Because the energy change due to the Peierls distor-
tion is zero in the limit of 2D graphite, this result is consistent with the limiting case of N = 00. This very small Peierls gap is, thus, negligible at finite temperatures and in the presence of fluctuations arising from 1D conductors. Very recently, Viet et al. showed that the in-plane and out-of-plane distortions do not occur simultaneously, but their conclusions regarding the Peierls gap for carbon nanotubes are essentially as discussed above. The band structure of four concentric armchair tubules with 10, 20, 30, and 40 carbon atoms around their circumferences (external diameter 27.12 A) was calculated, where the tubules were positioned to minimize the energy for all bilayered pairs[l7]. In this case, the four-layered tubule remains metallic, similar to the behavior of two double-layered armchair nanotubes, except that tiny band splittings form. Inspired by experimental observations on bundles of carbon nanotubes, calculations of the electronic structure have also been carried out on arrays of (6,6) armchair nanotubes to determine the crystalline structure of the arrays, the relative orientation of adjacent nanotubes, and the optimal spacing between them. Figure 5 shows one tetragonal and two hexagonal arrays that were considered, with space group symmetries P4,/mmc (DZh)h), P6/mmm ( D i h ) ,and P6/mcc (D,‘,), respectively[16,17,30]. The calculation shows
zyxwvut zyxwvuts Fig. 5 . Schematic representation of arrays of carbon nanotubes with a common tubule axial direction in the (a) tetragonal, (b) hexagonal I, and (c) hexagonal I1 arrangements. The reference nanotube is generated using a planar ring of twelve carbon atoms arranged in six pairs with the Dsh symmetry [16,17,30].
zyxwvutsrqpo zyxwvuts zyxwvut M. S . DRESSELHAUS et al.
that the hexagonal PG/mcc (D&)space group has the lowest energy, leading to a gain in cohesive energy of 2.4 meV/C atom. The orientational alignment between tubules leads to an even greater gain in cohesive energy (3.4 eV/C atom), The optimal alignment between tubules relates closely to the ABAB stacking of graphite, with an inter-tubule separation of 3.14 A at closest approach, showing that the curvature of the tubules lowers the minimum interplanar distance (as is also found for fullerenes where the corresponding distance is 2.8 A). The importance of the inter-tubule interaction can be seen in the reduction in the intertubule closest approach distance to 3.14 A for the P6/mcc (D,",) structure, from 3.36 A and 3.35 A,respectively, for the tetragonal P42/mmc (D&)and P6/mmm (D&)space groups. A plot of the electron dispersion relations for the most stable case is given in Fig. 6[16,17,30], showing the metallic nature of this tubule array by the degeneracy point between the H and K points in the Brillouin zone between the valence and conduction bands. It is expected that further calculations will consider the interactions between nested nanotubes having different symmetries, which on physical grounds should interact more weakly, because of a lack of correlation between near neighbors. Modifications of the conduction properties of semiconducting carbon nanotubes by B (p-type) and N (n-type) substitutional doping has also been discussed[311 and, in addition, electronic modifications by filling the capillaries of the tubes have also been proposed. Exohedral doping of the space between nanotubes in a tubule bundle could provide yet an-
other mechanism for doping the tubules. Doping of the nanotubes by insertion of an intercalate species between the layers of the tubules seems unfavorable because the interlayer spacing is too small to accommodate an intercalate layer without fracturing the shells within the nanotube. No superconductivity has yet been found in carbon nanotubes or nanotube arrays. Despite the prediction that 1D electronic systems cannot support superconductivity[33,34], it is not clear that such theories are applicable to carbon nanotubes, which are tubular with a hollow core and have several unit cells around the circumference. Doping of nanotube bundles by the insertion of alkali metal dopants between the tubules could lead to superconductivity. The doping of individual tubules may provide another possible approach to superconductivity for carbon nanotube systems.
zyxwvu zyxwvu z
KT AH K M L H r M A L
This journal issue features the many unusual properties of carbon nanotubes. Most of these unusual properties are a direct consequence of their 1D quantum behavior and symmetry properties, including their unique conduction properties[l 11 and their unique vibrational spectra. Regarding electrical conduction, carbon nanotubes show the unique property that the conductivity can be either metallic or semiconducting, depending on the tubule diameter dt and chiral angle 0. For carbon nanotubes, metallic conduction can be achieved without the introduction of doping or defects. Among the tubules that are semiconducting, their band gaps appear to be proportional to l/d[, independent of the tubule chirality. Regarding lattice vibrations, the number of vibrational normal modes increases with increasing diameter, as expected. Nevertheless, following from the 1D symmetry properties of the nanotubes, the number of infrared-active and Raman-active modes remains independent of tubule diameter, though the vibrational frequencies for these optically active modes are sensitive to tubule diameter and chirality. Because of the restrictions on momentum transfer between electrons and phonons in the electron-phonon interaction for carbon nanotubes, it has been predicted that the interaction between electrons and longitudinal phonons gives rise only to intraband scattering and not interband scattering. Correspondingly, the interaction between electrons and transverse phonons gives rise only to interband electron scattering and not to intraband scattering. These properties are illustrative of the unique behavior of 1D systems on a rolled surface and result from the group symmetry outlined in this paper. Observation of ID quantum effects in carbon nanotubes requires study of tubules of sufficiently small diameter to exhibit measurable quantum effects and, ideally, the measurements should be made on single nanotubes, characterized for their diameter and chirality. Interesting effects can be observed in carbon nanotubes for diameters in the range 1-20 nm, depending
Fig. 6 . Self-consistent band structure (48 valence and 5 conduction bands) for the hexagonal I1 arrangement of nanotubes, calculated along different high-symmetry directions in the Brillouin zone. The Fermi Ievel is positioned at the degeneracy point appearing between K-H, indicating metallic behavior for this tubule array[l7].
Physics of carbon nanotubes
on the property under investigation. To see 1D effects, faceting should be avoided, insofar as facets lead to 2D behavior, as in graphite. To emphasize the possibility of semiconducting properties in non-defective carbon nanotubes, and to distinguish between conductors and semiconductors of similar diameter, experiments should be done on nanotubes of the smallest possible diameter, To demonstrate experimentally the high density of electronic states expected for 1D systems, experiments should ideally be carried out on single-walled tubules of small diameter. However, to demonstrate magnetic properties in carbon nanotubes with a magnetic field normal to the tubule axis, the tubule diameter should be large compared with the Landau radius and, in this case, a tubule size of 10 nm would be more desirable, because the magnetic localization within the tubule diameter would otherwise lead to high field graphitic behavior. The ability of experimentalists to study 1D quantum behavior in carbon nanotubes would be greatly enhanced if the purification of carbon tubules in the synthesis process could successfully separate tubules of a given diameter and chirality. A new method for producing mass quantities of carbon nanotubes under controlled conditions would be highly desirable, as is now the case for producing commercial quantities of carbon fibers. It is expected that nano-techniques for manipulating very small quantities of material of nm size[14,36] will be improved through research of carbon nanotubes, including research capabilities involving the STM and AFM techniques. Also of interest will be the bonding of carbon nanotubes to the other surfaces, and the preparation of composite or multilayer systems that involve carbon nanotubes. The unbelievable progress in the last 30 years of semiconducting physics and devices inspires our imagination about future progress in 1D systems, where carbon nanotubes may become a benchmark material for study of 1D systems about a cylindrical surface.
4. D. S. Bethune, C. H. Kiang, M. S. deVries, G. Gorman, R. Savoy, J. Vazquez, and R. Beyers, Nature (London) 363, 605 (1993). 5. S. Iijima and T. Ichihashi, Nature (London) 363, 603 (1993). 6. M. S. Dresselhaus, G. Dresselhaus, and R. Saito, Phys. Rev. B 45, 6234 (1992). 7. R. A. Jishi, M. S. Dresselhaus, and G. Dresselhaus, Phys. Rev. B 47, 16671 (1993). 8. P. C. Eklund, J. M. Holden, and R. A. Jishi, Carbon 33, 959 (1995). 9. R. A. Jishi, L. Venkataraman, M. S. Dresselhaus, and G . Dresselhaus, Chem. Phys. Lett. 209, 77 (1993). 10. Riichiro Saito, Mitsutaka Fujita, G. Dresselhaus, and M. S. Dresselhaus, Mater. Sci. Engin. B19, 185 (1993). 11. J. W. Mintmire and C. T. White, Carbon 33, 893 (1995). 12. S. Wang and D. Zhou, Chem. Phys. Lett. 225, 165 (1994). 13. C. H. Olk and J. P. Heremans, J. Mater. Res. 9, 259 (1994). 14. J. P. Issi et al., Carbon 33, 941 (1995). 15. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, J. Appl. Phys. 73, 494 (1993). 16. J. C. Charlier and J. P. Michenaud, Phys. Rev. Lett. 70, 1858 (1993). 17. J. C. Charlier, Carbon Nunotubes and Fullerenes. PhD thesis, Catholic University of Louvain, Department of Physics, May 1994. 18. Ph. Lambin, L. Philippe, J. C. Charlier, and J. P. Michenaud, Comput. Muter. Sei. 2, 350 (1994). 19. Ph. Lambin, L. Philippe, J. C. Charlier, and J. P. Michenaud, In Proceedings of the Winter School on Fullerenes (Edited by H. Kuzmany, J. Fink, M. Mehring, and S. Roth), Kirchberg Winter School, Singapore, World Scientific Publishing Co., Ltd. (1994). 20. R. Saito, M. Fujita, G . Dresselhaus, and M. S. Dresselhaus, Appl. Phys. Lett. 60, 2204 (1992). 21. M. S. Dresselhaus, G. Dresselhaus, and Riichiro Saito, Mater. Sei. Engin. B19, 122 (1993). 22. Y. Yosida, Fullerene Sci. Tech. I, 55 (1993). 23. R. E. Peierls, In Quantum Theory of Solids. London, Oxford University Press (1955). 24. J. W. Mintmire, Phys. Rev B 43, 14281 (June 1991). 25. Kikuo Harigaya, Chem. Phys. Lett. 189, 79 (1992). 26. R. Saito, M. Fujita, G . Dresselhaus, and M. S. Dresselhaus, In Electrical, Optical and Magnetic Properties of Organic Solid State Materials, MRS Symposia Proceedings, Boston. Edited by L. Y. Chiang, A. F. Garito, and D. J. Sandman, vol. 247, p. 333, Pittsburgh, PA, Materials Research Society Press (1992). 27. K. Harigaya and M. Fujita, Phys. Rev. B 47, 16563 (1 993). 28. K. Harigaya and M: Fujita, Synth. Metals 55, 3196 (1993). 29. N. A. Viet, H . Ajiki, and T. Ando, ISSP Technical Reoorf 2828 (1994). 30. J. C. Charlier, X. Gonze, and J. P. Michenaud, Europhys. Lett. 29, 43 (1994). 31. J. Y.Yi and J. Bernholc, Phys. Rev. B47, 1708 (1993). 32. T. W. Ebbesen, Annu. Rev. Mater. Sei. 24, 235 (1994). 33. H. Frohlich, Phys. Rev. 79, 845 (1950). 34. H. Frohlich, Proc. Roy. SOC. London A215, 291 (1952). 35. R. A. Jishi, M. S. Dresselhaus, and G. Dresselhaus, Phys. Rev. B 48, 11385 (1993). 36. L. Langer, L. Stockman, J. P. Heremans, V. Bayot, C. H. Olk, C . Van Haesendonck, Y. Bruynseraede, and J. P. Issi, J. Mat. Res. 9, 927 (1994).
zyxwv zyx zyxwvu zyxwv zyxwvu zy zyxw -
Acknowledgements-We gratefully acknowledge stimulating discussions with T. W. Ebbesen, M. Endo, and R. A. Jishi. We are also in debt to many colleagues for assistance. The research at MIT is funded by NSF grant DMR-92-01878. One of the authors (RS) acknowledges the Japan Society for the Promotion of Science for supporting part of his joint research with MIT. Part of the work by RS is supported by a Grantin-Aid for Scientific Research in Priority Area “Carbon Cluster” (Area No. 234/05233214) from the Ministry of Education, Science and Culture, Japan.
1. S. Iijima, Nature (London) 354, 56 (1991). 2. T. W. Ebbesen and 2’. M. Ajayan, Nature (London) 358, 220 (1992). 3. T. W. Ebbesen, H. Hiura, J. Fujita, Y. Ochiai, S. Matsui, and K. Tanigaki, Chem. Phys. Lett. 209, 83 (1993).
zyxwvu zyxwvu zyx zyxwvutsr zyxwvut zyxw
ELECTRONIC AND STRUCTURAL PROPERTIES OF CARBON NANOTUBES J. W. MINTMIRE and C . T. WHITE
Chemistry Division, Naval Research Laboratory, Washington, DC 20375-5342, U.S.A. (Received 12 October 1994; accepted in revised form 15 February 1995)
Abstract-Recent developments using synthetic methods typical of fullerene production have been used to generate graphitic nanotubes with diameters on the order of fullerene diameters: “carbon nanotubes.” The individual hollow concentric graphitic nanotubes that comprise these fibers can be visualized as constructed from rolled-up single sheets of graphite. We discuss the use of helical symmetry for the electronic structure of these nanotubes, and the resulting trends we observe in both band gap and strain energy versus nanotube radius, using both empirical and first-principles techniques. With potential electronic and structural applications, these materials appear to be appropriate synthetic targets for the current decade. Key Words-Carbon nanotube, electronic properties, structural properties, strain energy, band gap, band structure, electronic structure.
Less than four years ago Iijima[l] reported the novel synthesis based on the techniques used for fullerene synthesis[2,3] of substantial quantities of multiple-shell graphitic nanotubes with diameters of nanometer dimensions. These nanotube diameters were more than an order of magnitude smaller than those typically obtained using routine synthetic methods for graphite fibers[4,5]. This work has been widely confirmed in the literature, with subsequent work by Ebbesen and Ajayan demonstrating the synthesis of bulk quantities of these materials. More recent work has further demonstrated the synthesis of abundant amounts of single-shell graphitic nanotubes with diameters on the order of one nanometer[7-9]. Concurrent with these experimental studies, there have been many theoretical studies of the mechanical and electronic properties of these novel fibers[lO-30]. Already, theoretical studies of the individual hollow concentric graphitic nanotubes, which comprise these fibers, predict that these nanometer-scale diameter nanotubes will exhibit conducting properties ranging from metals to moderate bandgap semiconductors, depending on their radii and helical structure[lO-221. Other theoretical studies have focused on structural properties and have suggested that these nanotubes could have high strengths and rigidity resulting from their graphitic and tubular structure[23-30]. The metallic nanotubes- termed serpentine -have also been predicted to be stable against a Peierls distortion to temperatures far below room temperaturejl01. The fullerene nanotubes show the promise of an array of all-carbon structures that exhibits a broad range of electronic and structural properties, making these materials an important synthetic target for the current decade. Herein, we summarize some of the basic electronic and structural properties expected of these nanotubes from theoretical grounds. First we will discuss the basic structures of the nanotubes, define the nomencla37
ture used in the rest of the manuscript, and present an analysis of the rotational and helical symmetries of the nanotube. Then, we will discuss the electronic structure of the nanotubes in terms of applying Born-von Karman boundary conditions to the two-dimensional graphene sheet. We will then discuss changes introduced by treating the nanotube realistically as a threedimensional system with helicity, including results both from all-valence empirical tight-binding results and first-principles local-density functional (LDF) results. 2. NANOTUBE STRUCTURE AND SYMMETRY
Each single-walled nanotube can be viewed as a conformal mapping of the two-dimensional lattice of a single sheet of graphite (graphene), depicted as the honeycomb lattice of a single layer of graphite in Fig. 1, onto the surface of a cylinder. As pointed out by Iijima[ 11, the proper boundary conditions around the cylinder can only be satisfied if one of the Bravais lattice vectors of the graphite sheet maps to a circumference around the cylinder. Thus, each real lattice vector of the two-dimensional hexagonal lattice (the Bravais lattice for the honeycomb) defines a different way of rolling up the sheet into a nanotube. Each such lattice vector, E,can be defined in terms of the two primitive lattice vectors R I and R2and a pair of integer indices [n,,nz], such that B = n l R 1 n2R2,with Fig. 2 depicting an example for a [4,3] nanotube. The point group symmetry of the honeycomb lattice will make many of these equivalent, however, so truly unique nanotubes are only generated using a one-twelfth irreducible wedge of the Bravais lattice. Within this wedge, only a finite number of nanotubes can be constructed with a circumference below any given value. The construction of the nanotube from a conformal mapping of the graphite sheet shows that each nanotube can have up to three inequivalent (by point
zyxwvutsrqponml J. W. MINTMIRE and C. T. WHITE
sets, the nanotubes are chiral and have three inequivalent helical operations. Because real lattice vectors can be found that are normal to the primitive real lattice vectors for the graphite sheet, each nanotube thus generated can be shown to be translationally periodic down the nanotube axis[12-14,23]. However, even for relatively small diameter nanotubes, the minimum number of atoms in a translational unit cell can be quite large. For example, for the [4,3] nanotube ( n l = 4 and nz = 3) then the radius of the nanotube is less than 0.3 nm, but the translational unit cell contains 148 carbon atoms as depicted in Fig. 2. The rapid growth in the number of atoms that can occur in the minimum translational unit cell makes recourse to the helical and any higher point group symmetry of these nanotubes practically mandatory in any comprehensive study of their properties as a function of radius and helicity. These symmetries can be used to reduce to two the number of atoms necessary to generate any nanotube[13,14]; for example, reducing the matrices that have to be diagonalized in a calculation of the nanotube’s electronic structure to a size no larger than that encountered in a corresponding electronic structure calculation of two-dimensional graphene. Before we can analyze the electronic structure of a nanotube in terms of its helical symmetry, we need to find an appropriate helical operator S (h, p) , representing a screw operation with a translation h units along the cylinder axis in conjunction with a rotation p radians about this axis. We also wish to find the operator S that requires the minimum unit cell size (Le., the smallest set of carbon atoms needed to generate the entire nanotube using S) to minimize the computational complexity of calculating the electronic structure. We can find this helical operator S( h, p) by first finding the real lattice vector H = m l R , m2R2 in the honeycomb lattice that will transform to S ( h ,p) under conformal mapping, such that h = I H x BI /I BI and p = 2.1r(H.B)/(BIZ.An example of H is depicted in Fig. 2 for the [4,3] nanotube. If we construct the cross product H x B of H and B, the magnitude I H x BI will correspond to the area “swept out” by the helical operator S. Expanding, we find
zyx zyxwvutsrq zyxwvutsr
Fig. 1. Two-dimensional honeycomb lattice of graphene; primitive lattice vectors R, and R, are depicted outlining primitive unit cell.
group symmetry) helical operations derived from the primitive lattice vectors of the graphite sheet. Thus, while all nanotubes have a helical structure, nanotubes constructed by mapping directions equivalent to lattice translation indices of the form [n,O] and [n,n],to the circumference of the nanotube will possess a reflection plane. These high-symmetry nanotubes will, therefore, be achiral[ 12-14,231. For convenience, we have labeled these special structures based on the shapes made by the most direct continuous path of bonds around the circumference of the nanotube. Specifically, the [n,O]-type structures were labeled as sawtooth and the [n,n]-type structures as serpentine. For all other conformations inequivalent to these two
where I R I x Rz I is just the area per two-carbon unit cell of the primitive graphene lattice. Thus ( m l n 2m 2 n 1 )gives the number of carbon pairs required for the unit cell under helical symmetry with a helical operator generated using H and the conformal mapping. Given a choice for n, and n2, then ( m ~ n z- m z n ~ ) must equal some integer value
Fig. 2. Depiction of conformal mapping of graphene lattice to [4,3] nanotube. B denotes [4,3] lattice vector that transforms to circumference of nanotube, and H transforms into the helical operator yielding the minimum unit cell size under helical symmetry. The numerals indicate the ordering of the helical steps necessary to obtain one-dimensional translation periodicity.
Integer arithmetic then shows that the smallest magnitude nonzero value of N will be given by the greatest common divisor of nl and n2. Thus, we can easily determine the helical operator H + S(h, p) that yields
zyxwvu zyxwvutsrqp zyxwvutsrqponmlkjihg zyxwvutsrqp zyxwvutsrq Electronic and structural properties of carbon nanotubes
the minimum unit cell (primitive helical motif) size of 2Natoms, where N is the greatest common divisor of n , and n,. Next, consider the possible rotational symmetry around the helical axis. This operation is of special interest because all the rotation operations around the chain axis will commute with the helical operator S (, h, p) , allowing solutions of any one-electron Hamiltonian model to be block-diagonalized into the irreducible representations of both the helical operation and the rotation operator simultaneously. We observe that the highest order rotational symmetry (and smallest possible rotation angle for such an operator) will be given by a C, rotation operator, where N remains the greatest common divisor of n , and nz. This can be seen straightforwardly by considering the real lattice vector B,,
The conformal mapping will transform this lattice operation B, to a rotation of 2 a / N radians around the nanotube axis, thus generating a C, subgroup. The rotational and helical symmetries of a nanotube defined by B can then be seen by using the corresponding helical and rotational symmetry operators S(h,pp) and C, to generate the nanotube[l3,14]. This is done by first introducing a cylinder of radius
posed by the rolling up of the nanotube. We then continue by analyzing a structurally correct nanotube within a Slater-Koster sp tight-binding model using the helical symmetry of the nanotube. We then finish by discussing results for both geometry optimization and band structure using first-principles local-density functional methods.
3.1 Graphene model
One of the simplest models for the electronic structure of the states near the Fermi level in the nanotubes is that of a single sheet of graphite (graphene) with periodic boundary conditions[lO-161. Let us consider a Slater-Koster tight-binding model and assume that the nearest-neighbor matrix elements are the same as those in the planar graphene (Le., we neglect curvature effects). The electronic structure of the nanotube will then be basically that of graphene, with the additional imposition of Born-von Karman boundary conditions on the electronic states, so that they are periodic under translations of the circumference vector B. The electronic structure of the a-bands near the Fermi level then reduces to a Huckel model with one parameter, the Vppnhopping matrix element. This model can be easily solved, and the one-electron eigenvalues can be given as a function of the twodimensional wavevector k in the standard hexagonal Brillouin zone of graphene in terms of the primitive lattice vectors R1 and R,:
E(k) = I / , , J ~ + ~ c o s ~ .+R~~c o s ~ . R ~ + ~ c o - sR ~ 2 ). ( R ~
The two carbon atoms located at d = (R, R2)/3 and 2d in the [O,O] unit cell of Fig. 1 are then mapped to the surface of this cylinder. The first atom is mapped to an arbitrary point on the cylinder surface, which requires that the position of the second be found by rotating this point by 27r(d.B)/IBI2 radians about the cylinder axis in conjunction with a translation Id x IBI /IBI units along this axis. The positions of these first two atoms can then be used to generate 2 ( N - 1) additional atoms on the cylinder surface by (N-1) successive 2a/N rotations about the cylinder axis. Altogether, these 2 N atoms complete the specification of the helical motif which corresponds to an area on the cylinder surface given by N J R , x Rzl. This helical motif can then be used to tile the remainder of the nanotube by repeated operation of the helical operation defined by S ( h , p) generated by the H defined using eqn (2).
The Born-von Karman boundary conditions then restrict the allowed electronic states to those in the graphene Brillouin zone that satisfy
zyxwvut zyxwv zyxwvuts
3. ELECTRONIC STRUCTURE OF CARBONNANOTUBES
We will now discuss the electronic structure of single-shell carbon nanotubes in a progression of more sophisticated models. We shall begin with perhaps the simplest model for the electronic structure of the nanotubes: a Huckel model for a single graphite sheet with periodic boundary conditions analogous to those im-
that rn an integer[l0,14,15]. In terms of the twodimensional Brillouin zone of graphene, the allowed states will lie along parallel lines separated by a spacing of 2 ~ / BI l , Fig. 3a depicts a set of these lines for the [4,3] nanotube. The reduced dimensionality of these one-electron states is analogous to those found in quantum confinement systems; we might expect that the multiple crossings of the Brillouin zone edge would lead to the creation of multiple gaps in the electronic density-of-states (DOS) as we conceptually transform graphene into a nanotube. However, as depicted in Fig. 3b, these one-electron states are actually continuous in an extended Brillouin zone picture. A direct consequence of our conclusion in the previous section-that the helical unit cell for the [4,3] nanotube would have only two carbons, the same as in graphene itself-is that the a-band in graphene will transform into a single band, rather than several. Initially, we showed that the set of serpentine nanotubes [n,n] are metallic. Soon thereafter, Hamada et al. and Saito et a1.[16,17] pointed out that the periodicity condition in eqn ( 5 ) further groups the remaining nanotubes (those that cannot be constructed
zyxwvut zyxwvutsrqp zyxwvut zyxwvutsrqp zyxwvut J. W. MINTMIREand C. T. WHITE
from the condition n, = n2)into one set that has moderate band gaps and a second set with small band gaps. The graphene model predicts that the second set of nanotubes would have zero band gaps, but the symmetry breaking introduced by curvature effects results in small, but nonzero, band gaps. To demonstrate this point, consider the standard reciprocal lattice vectors K, and K2 for the graphene lattice given by Ki.Rj = 2 ~ 6The ~ ~band . structure given by eqn (4) will have a band crossing (i.e., the occupied band and the unoccupied band will touch at zero energy) at the corners K of the hexagonal Brillouin zone, as depicted in Fig. 3. These six corners K of the central Brillouin zone are given by the vectors kK = f (K, - K2)/3, f (2K1 K2)/3, and k ( K l + 2K2)/3. Given our earlier definition of B, B = n l R l + n2R2, a nanotube will have zero band gap (within the graphene model) if and only if k, satisfies eqn (5), leading to the condition n, - n2 = 3m, where m is an integer. As we shall see later, when we include curvature effects in the electronic Hamiltonian, these "metallic" nanotubes will actually fall into two categories: the serpentine nanotubes that are truly metallic by symmetry[lO, 141, and quasimetallic with small band gaps[15-18]. In addition to the zero band gap condition, we have examined the behavior of the electron states in the vicinity of the gap to estimate the band gap for the moderate band gap nanotubes[l3,14]. Consider a wave vector k in the vicinity of the band crossing point K and define Ak = k - k x , with Ak = IAkl. The function ~ ( kdefined ) in eqn (4) has a cusp in the vicinity of R, but &'(k) is well-behaved and can be expanded in a Taylor expansion in Ak. Expanding ETk), we find
zyxwvuts zyx +
Fig. 3. (a) Depiction of central Brillouin zone and allowed graphene sheet states for a [4,3]nanotu_be conformation. Note Fermi level for graphene occurs at K points at vertices of hexagonal Brillouin zone. (b) Extended Brillouin zone picture of [4,3] nanotube. Note that top left hexagon is equivalent to bottom right hexagon.
graphite sheet with periodic boundary conditions imposed analogous to those in a quantum confinement problem. This level approximation allowed us to analyze the electronic structure in terms of the twodimensional band structure of graphene. Going beyond this level of approximation will require explicit treatment of the helical symmetry of the nanotube for practical computational treatment of the electronic structure problem. We have already discussed the ability to deEZ(Ak) = V;p,azAk2, (6) termine the optimum choice of helical operator S in terms of a graphene lattice translation H. We now exwhere a = lRll = J R 2 is J the lattice spacing of the amine some of the consequences of using helical symhoneycomb lattice. The allowed nanotube states sat- metry and its parallels with standard band structure isfying eqn (5) lie along parallel lines as depicted in theory. Because the symmetry group generated by the Fig. 2 with a spacing of 2a/B, where B = I B I . For the screw operation S is isomorphic with the one-dimennonmetallic case, the smallest band gap for the nano- sional translation group, Bloch's theorem can be generalized so that the one-electron wavefunctions will tube will occur at the nearest allowed point to I?, which will lie one third of the line spacing from K. transform under S according to Thus, using Ak = 2?r/3B, we find that the band gap equals[ 13,141
where rcc is the carbon-carbon bond distance (rcc = a/& 1.4 A) and RT is the nanotube radius (RT= B/2a). Similar results were also obtained by Ajiki and Ando[ 1Sj .
3.2 Using helical symmetry The previous analysis of the electronic structure of the carbon nanotubes assumed that we could neglect curvature effects, treating the nanotube as a single
zyxw The quantity K is a dimensionless quantity which is conventionally restricted to a range of --P < K 5 T ,a central Brillouin zone. For the case cp = 0 (i.e., S a pure translation), K corresponds to a normalized quasimomentum for a system with one-dimensional translational periodicity (i.e., K = kh, where k is the traditional wavevector from Bloch's theorem in solidstate band-structure theory). In the previous analysis of helical symmetry, with H the lattice vector in the graphene sheet defining the helical symmetry generator, K in the graphene model corresponds similarly to the product K = k . H where k is the two-dimensional quasimomentum vector of graphene.
Electronic and structural properties of carbon nanotubes Before we continue our description of electronic structure methods for the carbon nanotubes using helical symmetry, let us reconsider the metallic and quasimetallic cases discussed in the previous section in more detail. The graphene model suggests that a metallic state will occur where two bands cross, and that the Fermi level will be pinned to the band crossing. In terms of band structure theory however, if these two bands belong to the same irreducible representation of a point group of the nuclear lattice that also leaves the point in the Brillouin zone invariant, then rather than touching (and being degenerate in energy) these one-electron eigenfunctions will mix and lead to an avoided crossing. Only if the two eigenfunctions belong to different irreducible representations of the point group can they be degenerate. For graphene, the high symmetry of the honeycomb lattice allows the degeneracy of the highest-occupied and lowest-unoccupied states at the corners K of the hexagonal Brillouin zone in graphene. Rolling up graphene into a nanotube breaks this symmetry, and we must ask what point group symmetries are left that can allow a degeneracy at the band crossing rather than an avoided crossing. For the nanotubes, the appropriate symmetry operations that leave an entire band in the Brillouin zone invariant are the C, rotation operations around the helical axis and reflection planes that contain the helical axis. We see from the graphene model that a reflection plane will generally be necessary to allow a degeneracy at the Fermi level, because the highest-occupied and lowestunoccupied states will share the same irreducible representation of the rotation group. To demonstrate this, consider the irreducible representations of the rotation group. The different irreducible representations transform under 1he generating rotation (of ~ T / N radians) with a phase factor an integer multiple 2am/N, where m = 0, . . . , N - 1. Within the graphene model, each allowed state at quasimomentum k will transform under the rotation by the phase factor given by k.B/N, and by eqn ( 5 ) we see that the phase factor at K i s just 2 ~rn/N.The eigenfunctions predicted using the graphene model are therefore already members of the irreducible representations of the rotation point group. Furthermore, the eigenfunctions at a given Brillouin zone point k in the graphene model must be members of the same irreducible representation of the rotation point group. For the nanotubes, then, the appropriate symmetries for an allowed band crossing are only present for the serpentine ( [ n n, ] ) and the sawtooth ([n,O])conformations, which will both have C,,, point group symmetries that will allow band crossings, and with rotation groups generated by the operations equivalent by conformal mapping to the lattice translations R 1+ R2 and R1,respectively. However, examination of the graphene model shows that only the serpentine nanotubes will have states of the correct symmetry @e., different parities under the reflection operation) at the point where the bands can cross. Consider the K point at (K, - K2)/3. The serpentine case always sat-
and at the points the one-electron isfies eqn (3, wave functions transform under the generator of the rotation group C,,with a phase factor given by kR. (R,+ R2) = 0. This irreducible representation of the C, group is split under reflection into the two irreducible representations a, and a2 of the C,, group that are symmetric and antisymmetric, respectively, under the reflection plane; the states at K will belong to these two separate irreducible representations. Thus, the serpentine nanotubes are always metallic because of symmetry if the Hamiltonian allows sufficient bandwidth for a crossing, as is normally the case[lO]. The sawtooth nanotubes, however, present a different picture. The one-electron wave functions at K transform under the generator of the rotation group for this nanotube with a phase factor given by LR-R,= 2n/3. This phase factor will belong to one of the e representations of the C,,, group, and the states at If in the graphene Brillouin zone will therefore belong to the same symmetry group. This will lead to an avoided crossing. Therefore, the band gaps of the nonserpentine nanotubes that satisfy eqn ( 5 ) are not truly metallic but only small band gap systems, with band gaps we estimate from empirical and first-principles calculation to be of the order of 0.1 eV or less. Now, let us return to our discussion of carrying out an electronic structure calculation for a nanotube using helical symmetry. The one-electron wavefunctions II;- can be constructed from a linear combination of Bloch functions ‘pi, which are in turn constructed from a linear combination of nuclear-centered functions x j ( r ) ,
zyxwvu zyxwvuts zyxwvu
zyxwv zyxwvuts zyxwvutsr zy zyxwvutsrq zyxwvu As the next step in including curvature effects beyond the graphene model, we have used a Slater-Koster parameterizationof the carbon valence states- which we have parameterized[32,33] to earlier LDF band structure calculations on polyacetylene-in the empirical tight-binding calculations. Within the notation in ref.  our tight-binding parameters are given by V,,= -4.76 eV, V,,= 4.33 eV, Vpp,= 4.37 eV, and Vppa= -2.77 eV. We choose the diagonal term for the carbon p orbital, = 0 which results in the s diagonal term of E, = -6.0 eV. This tight-binding model reproduces first-principlesband structures qualitatively quite well. As an example, Fig. 4 depicts both §later-Koster tight-binding results and first-principles LDF results[l0,12] for the band structure of the [5,5] serpentine nanotube within helical symmetry. AI1 bands have been labeled for the LDF results according to the four irreducible representations of the C,, point group: the rotationally invariant a, and a, representations, and the doubly-degenerate el and e2 representation. As noted in our discussion for the ser-
zyxwvut zyxwvu zyxwv
J. W. MINTMIRE and C . T. WHITE
zyxwvutsrq zyxwvu zyxwvutsrqponm zyxwvutsr zyxwvutsr t
Fig. 4. (a) Slater-Koster valence tight-binding and (b) firstprinciples LDF band structures for [5,5] nanotube. Band structure runs from left at helical phase factor K = 0 to right at K = n. Fermi level E~ for Slater-Koster results has been shifted to align with LDF results.
pentine nanotubes, this band structure is metallic with a band crossing of the a, and a2 bands. Within the Slater-Koster approximation, we can easily test the validity of the approximations made in eqn (7) based on the graphene model. In Fig. 5 we depict the band gaps using the empirical tight-binding method for nanotube radii less than 1.5 nm. The nonmetallic nanotubes (nl - n2 # 3 rn) are shown in the upper curve where we have also depicted a solid line showing the estimated band gap for the nonmetallic nanotubes using I GpX) rcc/Rr, with V,, as given above and rcc = 1.44 A. We see excellent agreement between the estimate based on the graphene sheet and the exact calculations for the tight-binding model with curvature introduced, with the disagreement increasing with increasing curvature at the smaller radii.
Nanotube radius (nm)
Fig. 5 . Band gap as a function of nanotube radius calculated using empirical tight-binding Hamiltonian. Solid line gives estimate using Taylor expansion of graphene sheet results in eqn. (7).
where ni(K)are the occupation numbers of the oneelectron states, xj” denotes Srnxj(r),and Pf are the coefficients of the real lattice expansion of the density matrix given by
zyxwvutsrq zyxwvu The total energy for the nanotube is then given by
3.3 First-principles methods We have extended the linear combination of Gaussian-type orbitals local-density functional approach to calculate the total energies and electronic structures of helical chain polymers. This method was originally developed for molecular systems[36401, and extended to two-dimensionally periodic systems[41,42] and chain polymers. The one-electron wavefunctions here J.i are constructed from a linear combination of Bloch functions pj, which are in turn constructed from a linear combination of nuclearcentered Gaussian-type orbitals xj (r) (in this case, products of Gaussians and the real solid spherical harmonics). The one-electron density matrix is given by
where Z,, and R, denote the nuclear charges and coordinates within a single unit cell, Rr denotes the nuclear coordinates in unit cell rn (RZ= SmR,), and [p1 Ip2] denotes an electrostatic interaction integral,
Rather than solve for the total energy directly as expressed in eqn (13), we follow the suggestion of ear-
Electronic and structural properties of carbon nanotubes
lier workers to fit the exchange-correlation 'potential and the charge density (in the Coulomb potential) to a linear combination of Gaussian-type functions. We have carried out a series of geometry optimizations on nanotubes with diameters less than 2 nm. We will present some results for a selected subset of the moderate band gap nanotubes, and then focus on results for an example chiral systems: the chiral [9,2] nanotube with a diameter of 0.8 nm. This nanotube has been chosen because its diameter corresponds to those found in relatively large amounts by Iijima after the synthesis of single-walled nanotubes. How the structural properties of the fullerene nanotubes change with conformation is one of the most important questions to be answered about these new materials. In particular, two properties are most apt for study with the LDF approach: how does the band gap change with nanotube diameter, and how does the strain energy change with nanotube diameter? We have studied these questions extensively using empirical methods[ 10-14,23], and are currently working on a comprehensive study of the band gaps, strain energies, and other properties using the LDF approach. We expect from eqn (7) and the previous analysis of the graphene sheet model that the moderate band gap nanotubes should have band gaps that vary roughly inversely proportional to the nanotube radius. In Fig. 6 we depict representative results for some moderate band gap nanotubes. In the figure, we see that not only do our first-principles band gaps decrease in an inverse relationship to the nanotube radius, but that the band gaps are well described with a reasonable value of V,, - -2.5 eV. Second, we expect that the strain energy per carbon should increase inversely proportional to the square of the nanotube radius. Based on a continuum elastic model, Tibbetts derived a strain energy for a thin graphitic nanotube of the general form:
where E is the elastic modulus, R is the radius of curvature, L is the length of the cylinder, and a is a representative thickness of the order of the graphite interplanar spacing (3.35 A). Assuming that the total number of carbons is given by N = 23rRL/hl, where hl is the area per carbon, we find that the strain energy per carbon is expected to be
In earlier work, we found this relationship was well observed, using empirical bond-order potentials for all nanotubes with radii less than 0.9 nm, and for a range of serpentine nanotubes using the LDF method. As part of our studies, we have carried out first-principles LDF calculations on a representative sample of chiral nanotubes. Iijima and Ichihashi have recently reported the synthesis of single-shell fullerene nanotubes with diameters of about 1 nm, using the gas-phase product of a carbon-arc synthesis with iron vapor present. After plotting the frequency of single-shell nanotubes they observed versus nanotube diameter, they found enhanced abundances for diameters of roughly 0.8 nm and 1.1 nm. For first-principles simulations then to be useful, they should be capable of calculations for nanotubes with diameters from about 0.6-2.0 nm. In Fig. 7 we depict the calculated total energy per carbon, shifted relative to an extrapolated value for an infinite radius nanotube, for a representative sample of nanotubes over this range using the LDF approach. In this figure, the open squares denote results for unoptimized nanotubes, where the nano-
zyxwvutsrq zyxwvuts zyxwvu zyxwv 0.4
zyxwvutsrqpo zyxwvutsrqpo 0
Nanotube radius (nm)
Nanotube radius (nm)
Fig. 6 . Band gap as a function of nanotube radius using firstprinciples LDF method. Solid line shows estimates using V = -2.5 eV. graphene sheet model with ,
Fig. 7 . Strain energy per carbon (total energy minus total energy extrapolated for the graphite sheet) as a function of nanotube radius calculated for unoptimized nanotube structures (open squares) and optimized nanotube structures (solid circles). Solid line depicts inverse square relationship drawn through point at smallest radius.
zyxwvutsrqp zyxwvuts zyxwvu zyxwv zyxwvut zyxwvutsr
zyx I " " l " " l " " l " " I
Table I . Relaxation energy per carbon (eV) obtained by geometry optimization of nanotubes relative to extrapolated value for graphene
Nanotube t12SI tm21 11~41
Unrelaxed energy (ev)
Relaxed energy (eV)
0.6050 0.5630 0.5370 0.4170 0.4060 0.2460
0.067 0.071 0.076 0.133 0.140 0.366
0.073 0.130 0.137 0.354
tube has been directly constructed from a conformal mapping of graphene with a carbon-carbon nearest-
Electronic and structural properties of carbon nanotubes
graphene sheet, and on the other hand the small band gap and truly metallic serpentine conformation nanotubes that do satisfy this condition. We have earlier demonstrated[ 10-121 for the serpentine nanotubes that, for diameters under a nanometer, we expect that the density of states at the Fermi level is comparable to metallic densities and that the nanotubes should not Peierls-distort at normal temperatures. Independent of helicity, we find that the larger-diameter moderate band gap members of the family of moderate band gap nanotubes (nl- n2 # 3 m ) have bandgaps given approximately by Eg = I V,,I ( rcc/RT) and hence do not have bandgaps approaching kBT at room temperature until their diameters exceed approximately about 30 nm[lO]. We have also examined the energetics and elastic properties of small-diameter graphitic nanotubes using both first-principles and empirical potentials[W] . We find that the strain energy per carbon relative to an unstrained graphite sheet goes as 1/R$ (where RT is the nanotube radius) and is insensitive to other aspects of the lattice structure, indicating that relationships derivable from continuum elastic theory persist well into the small radius limit. In general, we find that the elastic properties are those expected by directly extrapolating the behavior of larger graphitic fibers to a small cross-section. The recent advances in synthesis of single-shell nanotubes should stimulate a wealth of new experimental and theoretical studies of these promising materials aimed at determining their structural, electronic, and mechanical properties. Many questions remain to be further investigated. How can they be terminated[29,43] and can they be connected? What are their electrical properties? For those that are semiconductors, can they be successfully doped[#]? What are the mechanical properties of these nanotubes? How will they respond under compression and stressI2328]? Do they have the high strengths and rigidity that their graphitic and tubular structure implies? How are these nanotubes formed[43,45,46]? Can techniques be devised that optimize the growth and allow the extraction of macroscopic amounts of selected nanotubes[7,8]? These questions all deserve immediate attention, and the promise of these noveI all-carbon materials justify this as a major research area for the current decade.
4. G . G. Tibbetts, J. Crystal Growth 66, 632 (1983). 5. J. S. Speck, M. Endo, and M. S. Dresselhaus, J. Crystal Growth 94, 834 (1989). 6. T . W. Ebbesen and P. M. Ajayan, Nature (London) 358, 220 (1992). 7. S. Iijima and T . Ichihashi, Nature (London) 363, 603 (1993). 8. D. S. Bethune, C. H. Klang, M. S. DeVries, G . Gorman, R. Savoy, J. Vazquez, and R. Beyers, Nature (London) 363, 605 (1993). 9. M. Endo, K. Takeuchi, S. Igarashi, K. Kobori, M. Shiraishi, and H. W. Kroto, J. Phys. Chem. SoNds 54, 1841 (1993). 10. J. W. Mintmire, B. I. Dunlap, and C. T. White, Phys. Rev. Lett. 68, 631 (1992). 11. C. T. White, J. W. Mintmire, R. C. Mowrey, D. W. Brenner, D. H. Robertson, J. A. Harrison, and B. I. Dunlap, In Buckminsferfullerenes(Edited by W. E. Billups and M. A. Ciufolini) pp. 125-184. VCH, New York, (1993). 12. J. W. Mintmire, D. H. Robertson, B. I. Dunlap, R. C. Mowrey, D. W. Brenner, and C. T . White, Electrical, Optical, and Magnetic Properties of Organic Solid State Materials (Edited by L. Y. Chiang, A. E Garito, and D. J. Sandman) p. 339. MRS Symposia Proceedings No. 247. Materials Research Society, Pittsburgh (1992). 13. C. T. White, D. H. Robertson, and J. W. Mintmire, Phys. Rev. B 47, 5485 (1993). 14. J. W. Mintmire, D. H. Robertson, and C. T. White, J. Phys. Chem. Solids 54, 1835 (1993). 15. N. Hamada, S. Sawada, and A. Oshiyamu, Phys. Rev. Lett. 68, 1579 (1992). 96. R. Saito, M. Fujita, G. Dresselhaus, M. S. Dresselhaus, Phys. Rev. B 46, 1804 (1992). Mater. Res. SOC. Sym. Proc. 247,333 (1992); Appl. Phys. Lett. 60,2204 (1992). 47. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, J. Appl. Phys. 73, 494 (1993). 18. H. Ajiki and T. Ando, J. Phys. Soc. Japan 62, 1255 (1993). J. Phys. Soc. Japan 62, 2470 (1993). 19. P.-J. Lin-Chung and A. K. Rajagopal, J: Phyx C6,3697 (1994). Phys. Rev. B 49, 8454 (1994). 20. X. Blase, L. X. Benedict, E. L. Shirley, and S. G . Louie, Phys. Rev. Lett. 72, 1878 (1994). 21. D. J. Klein, W. A. Seitz, and T. G. Schmalz, J. Phys. Chem. 97, 1231 (1993). 22. K. Harigaya, Phys. Rev. B 45, 12071 (1992). 23. D. H. Robertson, D. W. Brenner, and J. W. Mintmire, Phys. Rev. B 45, 12592 (1992). 24. A. A. Lucas, P. H. Lambin, and R. E. Smalley, J. Phys. Chem. Solids 54, 581 (1993). 25. J.-C. Charlier and J.-P. Michenaud, Phys. Rev. Lett. 70, 1858 (1993). 26. G. Overney, W. Zhong, and D. Tomanek, Z . Phys. D 27, 93 (1993). 21. R. S. Ruoff, J. Tersoff, D. C. Lorents, S. Subramoney, and B. Chan, Nature 364, 514 (1993). 28. J. Tersoff and R. S . Ruoff, Phys. Rev. Lett. 73, 676 (1994). 29. M. Fujita, R. Saito, G . Dresselhaus, M. S. Dresselhaus, Phys. Rev. B 45, 13834 (1992). 30.. B.i. Dunlap, Phys. Rev. B 46, 1933 (1992). 31. J. C. Slater and G. E Koster, Phys. Rev. 94, 1498 (1954). 32. M. L. Elert, J. W. Mintmire, and C. T. White, J. Phys. (Paris), Colloq. 44, C3-451 (1983). 33. M. L. Elert, C. T. White, and J. W. Mintmire, Mol. Cryst. Liq. Cryst. 125, 329 (1985). C. T. White, D. H. Robertson, and J. W. Mintmire, unpublished. 34. J. W. Mintmire and C . T. White, Phys. Rev. Lett. 50, 101 (1983). Phys. Rev. B 28, 3283 (1983). 35. J. W. Mintmire, In Density Functional Methods in Chemistry (Edited by J. Labanowski and 3. Andzelm) p. 125. Springer-Verlag, New York (1991). 36. B. I. Dunlap, J. W. D. Connolly, and J. R. Sabin, J.
zyxwvuts zyxwvutsrqp zyxwvutsr zyxwvutsrq zyxwvutsrqpon zyxwvu
Acknowledgements-This work was supported by the Office of Naval Research (ONR) through the Naval Research Laboratory and directly through the ONR (Chemistry-Physics and Materials Divisions. We thank D. H. Robertson, D. W. Brenner, and E. I. Dunlap for many useful discussions.
REFERENCES 1. S. Iijima, Nature (London) 354, 56 (1991). 2. W. Kratschmer, L. D. Lamb, K. Fostiropoulos, and D. R. Huffman, Chem. Phys. Lett. 170, 167 (1990). Nature 347, 354 (1990). 3. W. E. Billups and M. A. Ciufolini, eds. Buckminsterfullerenes. VCH, New York (1993).
37. 38. 39.
zyxwv zyxwvu zyxwvu zy z zyxwvu zyxwvu
J . W. MINTMIRE and C. T. WHITE Chem. Phys. 71,3396 (1979). J. Chem. Phys. 71,4993 (1979). J. W. Mintmire, Int. J. Quantum Chem. Symp. 13, 163 (1979). J. W. Mintmire and J. R. Sabin, Chem. Phys. 50, 91 (1980). J. W. Mintmire and B. I. Dunlap, Phys. Rev. A 25, 88 (1982). J. W. Mintmire, Int. J. Quantum Chem. Symp. 24, 851 (1990).
41. J. W. Mintmire and J. R. Sabin, Int. J. Quantum Chem. Symp. 14, 707 (1980). 42. J. W. Mintmire, J. R. Sabin, and S. B. Trickey, Phys. Rev. B 26, 1743 (1982). 43. S. Iijima, Mater. Sci. Eng. B19, 172 (1993). 44. J.-Y. Yi and J. Bernholc, Phys. Rev. B 47, 1703 (1993). 45. M. Endo and H. W. Kroto, J. Phys. Chem. 96, 6941 (1992). 46. S. Iijima, P. M. Ajayan, and T. Ichihashi, Phys. Rev. Left. 69, 3100 (1992).
CARBON NANOTUBES WITH SINGLE-LAYER WALLS CHING-HWAKIANG,^^' WILLIAM A. GODDARD111: ROBERTBEYERS,’ and DONALDS. BETHUNE’
‘IBM Research Division, Almaden Research Center, 650 Harry Road, San Jose, California 95120-6099, U.S.A. ’Materials and Molecular Simulation Center, Beckman Institute, Division of Chemistry and Chemical Engineering, California Institute of Technology, Pasadena, California 91 125, U.S.A. (Received 1 November 1994; accepted 10 February 1995)
Abstract-Macroscopic quantities of single-layer carbon nanotubes have recently been synthesized by cocondensing atomic carbon and iron roup or lanthanide metal vapors in an inert gas atmosphere. The nanotubes consist solely of carbon, sp -bonded as in graphene strips rolled to form closed cylinders. The structure of the nanotubes has been studied using high-resolution transmission electron microscopy. Iron group catalysts, such as Co, Fe, and Ni, produce single-layer nanotubes with diameters typically between 1 and 2 nm and lengths on the order of micrometers. Groups of shorter nanotubes with similar diameters can grow radially from the surfaces of lanthanide carbide nanoparticles that condense from the gas phase. If the elements S, Bi, or Pb (which by themselves do not catalyze nanotube production) are used together with Co, the yield of nanotubes is greatly increased and tubules with diameters as large as 6 nm are produced. Single-layer nanotubes are anticipated to have novel mechanical and electrical properties, including very high tensile strength and one-dimensional conductivity. Theoretical calculations indicate that the properties of single-layer tubes will depend sensitively on their detailed structure. Other novel structures, including metallic crystallites encapsulated in graphitic polyhedra, are produced under the conditions that lead to nanotube growth.
nanotubes, fiber, cobalt, catalysis, fullerenes, TEM.
The discovery of carbon nanotubes by Iijima in 1991[I] created much excitement and stimulated extensive research into the properties of nanometer-scale cylindrical carbon networks. These multilayered nanotubes were found in the cathode tip deposits that form when a DC arc is sustained between the graphite electrodes of a fullerene generator. They are typically composed of 2 to 50 concentric cylindrical shells, with outer diameters typically a few tens of nm and lengths on the order of pm. Each shell has the structure of a rolled up graphene sheet-with the sp2 carbons forming a hexagonal lattice. Theoretical studies of nanotubes have predicted that they will have unusual mechanical, electrical, and magnetic properties of fundamental scientific interest and possibly of technological importance. Potential applications for them as onedimensional conductors, reinforcing fibers in superstrong carbon composite materials, and sorption material for gases such as hydrogen have been suggested. Much of the theoretical work has focussed on single-layer carbon tubules as model systems. Methods to experimentally synthesize single-layer nanotubes were first discovered in 1993, when two groups independently found ways to produce them in macroscopic quantities[2,3]. These methods both involved covaporizing carbon and a transition metal catalyst and produced single-layer nanotubes approximately 1 nm in diameter and up to several microns long. In one case, Iijima and Ichihashi produced single-layer nanotubes by vaporizing graphite and Fe in an Ar/CH4 atmosphere. The tubes were found in the deposited soot. 47
Bethune et al., on the other hand, vaporized Co and graphite under helium buffer gas, and found singlelayer nanotubes in both the soot and in web-like material attached to the chamber walls. 2. SYNTHESIS OF SINGLELAYER CARBON NANOTUBES
In a typical experiment to produce single-layer nanotubes, an electric arc is used to vaporize a hollow graphite anode packed with a mixture of metal or metal compound and graphite powder. Two families of metals have been tried most extensively to date: transition metals such as Fe, Co, Ni, and Cu, and lanthanides, notably Gd, Nd, La, and Y.While these two metal groups both catalyze the formation of singlelayer nanotubes, the results differ in significant ways. The iron group metals have been found to produce high yields of single-layer nanotubes in the gas phase, with length-to-diameter ratios as high as several thousand[2-11]. To date, no association between the nanotubes and metal-containing particles has been clearly demonstrated. In contrast, the tubes formed with lanthanide catalysts, such as Gd, Nd, and Y, are shorter and grow radially from the surface of 10-100 nm diameter particles of metal carbide[8,10,12-15], giving rise to what have been dubbed “sea urchin” particles[121. These particles are generally found in the soot deposited on the chamber walls. Some other results fall in between or outside these main groups. In the case of nickel, in addition to long, straight nanotubes in the soot, shorter single-layer
C.-H. KIANGet al.
tubes growing radially (urchin style) for fcc-Ni or NiC3 particles in the rubbery collar that forms around the cathode have also been found[16,17]. Second despite the fact that copper reportedly does not catalyze single-layer tube growth in the gas phase[1I], Lin et ai. found that numerous short, single-layer tube structures form on the cathode tip when a Cu-containing anode is used[lS]. Finally, the growth of single-layer tubules on a graphite substrate by pyrolyzing a hydrogedbenzene mixture in a gas-phase flow-reactor at 1000°C was recently reported[l9]. That experimental result is unique among those described here, in that no metal atoms are involved. An overview of some of the experimental results on single-layer nanotubes is presented in Table 1. In the arc-production of nanotubes, experiments to date have been carried out in generally similar fashion. An arc is typically run with a supply voltage of 20-30 V and a DC current of 50-200 A (depending on the electrode diameters, which range from 5-20 mm). Usually He buffer gas is used, at a pressure in the range 50-600 Torr and flowing at 0-15 ml/min. The anode is hollowed out and packed with a mixture of a metal and powdered graphite. In addition to pure iron group metals, mixtures of these rnetals[7,S,lO] and metal compounds (oxides, carbides, and sulfides)  have been successfully used as source materials for the catalytic metals in nanotube synthesis. The ratio of metal to graphite is set to achieve the desired metal concentration, typically a few atomic percent. Parameter studies have shown that single-layer nanotubes can be produced by the arc method under a wide range of conditions, with large variations in variables such as the buffer gas pressure (100-500 Torr), gas flow rate, and metal concentration in the
anode[4,5]. These parameters are found to change the yield of nanotubes, but not the tube characteristics such as the diameter distribution. In contrast, the presence of certain additional elements, although they do not catalyze nanotube growth when used alone, can greatly modify both the amount of nanotube production and the characteristics of the nanotubes. For example, sulfur, bismuth, and lead all increase the yield and produce single-layer nanotubes with diameters as large as 6 nm, much larger than those formed with Co catalyst alone. Sulfur also appears to promote the encapsulation of Co-containing crystallites into graphitic polyhedra. Lambert et al. recently reported that a platinum/cobalt 1: 1 mixture also significantly increased the yield of nanotubes[ 111, even though Pt alone also has not produced nanotubes[9,11]. Different product morphologies have been found in different regions of the arc-reactor chamber. On the cold walls, a primary soot is deposited. In normal fullerene production, this soot has a crumbly, flocculent character. However, under conditions that lead to abundant nanotube growth, the density of tubes in this soot can be high enough to give it a rubbery character, allowing it to be peeled off the chamber wall in sheets. This rubbery character may be caused by either chemical or physical cross-linking between the nanotubes and the soot. We note that fullerenes in amounts comparable to those obtained without a metal present can be extracted from the rubbery soots using the normal solvents. Second, a hard slag is deposited on the cathode tip. This cathode tip contains high densities of multilayer nanotubes and polyhedral particles[20,21]. The fact that the transition-metal-catalyzed singlelayer nanotubes are distributed throughout the soot and rarely in the slag deposit leads to the conclusion
zyxwvuts zy Table 1. Results on single-layer nanotubes*
co co co Ni Ni Fe+Ni Fe+Ni Co+Ni co+s Co+Bi Co+Pb Co+Pt Y cu no metal
0.7-1.6 0.6-1.3 0.9-2.4 1-2 0.6-1.8 1.2-1.5 0.6-1.3 0.9-3.1 >0.6 10.6 1.0-6.0 0.8-5 0.7-4 =2
0.80, 1.05 0.7-0.8 1.3, 1.5 1.2-1.3
Fe,C fcc-co Co wrapped with graphene layers fcc-Ni in polyhedra in cathode deposit
zyxwvutsrq zyxwvutsr zyxwvut
1.1-1.7 1-4 >2
0.7-0.8 1.7 1.3-1.8 1.2-1.3 1.3, 1.5 1.2, 1.5
Co(C) in polyhedra and fcc-Co
CoPt YC2 in polyhedra Cu in polyhedra graphite substrate
*Unless specified, samples were from soot deposited on the chamber wall and the buffer gas was helium. Elements are those incorporated in the graphite anode, D is the nanotube diameter range, D , is the most abundant nanotube diameter, and Crystallites refers to metal-containing particles generated by the arc process and found in the soot. ‘Statistics from 60 tubes; bfrom 40 tubes; ‘from over 100 tubes; dfrom 70 tubes; ‘from over 300 tubes; ‘Nanotubes grew radially out of YC, crystals, 15-100 nm long; gNanotubes found in the cathode deposit, 3-40 nm long; hNanotubes formed by C6Hs pyrolysis on graphite substrate.
Carbon nanotubes with single-layer walls
that, in that case, the nanotubes form in the gas phase. Third, a soft rubbery blanket or collar builds up around the cathode when iron group metals are used. This material has been found to contain graphitic polyhedral particles, metals or metal carbides encapsulated in polyhedral particles, string of beads structures[8,16], and single-layer nanotubes[4,8,16]. Finally, with some catalysts, notably Co, mixtures of Co with Fe, Ni, Pt, S, Bi, and Pb, and Fe/Ni mixtures, web-like materials form inside the chamber when the arc is running [3,6,8,111. Figure 1 is a scanning electron micrograph (SEM) of a sample of the web-like material obtained by vaporizing Co and C under 400 Torr He. The threads and bundles of carbon nanotubes, often partly clad with a layer of non-crystalline carbon and fullerenes. The threads connect rounded particles with typical diameters of a few tens of nanometers. Figure 2a is a transmission electron microscope (TEM) image of the nanotube bundles. The sample was prepared by sonicating some soot in ethanol for a few minutes and placing a drop of the liquid on a holey-carbon-coated copper TEM grid. Shown in the micrograph is a region where a gap in the holey-carbon film was formed after the soot was put on the grid. Bundled and individual nanotubes bridge the = 0.25 pm gap. The soot particles themselves consist of non-crystalline carbon containing dark spots that have been identified by Energy Dispersive X-ray Spectroscopy (EDS) and electron diffraction to befcc-Co particles. Figure 2b, taken at higher magnification, shows a region where a high density of tubes span a gap in the soot. The process of
zyxwv zy 49
pulling the tubules out of the soot mass has aligned them to a striking degree. A high resolution TEM (HRTEM) image of a group of nanotubes (Fig. 2c) demonstrates their tendency to aggregate into bundles. The aggregation process is presumably driven by van der Waals attraction, which has been shown experimentally to give rise to significant forces between adjacent multilayer nanotubes, and is predicted to give rise to ordering of bundled single-layer nanotubes into crystalline arrays. A micrograph showing a bundle of Ni-catalyzed nanotubes end-on lends some support to this idea[ 171. The metals Y and Gd have been found to facilitate the growth of urchin particles - consisting of bundles of relatively short single-layer nanotubes rooted on and extending radially outward from metal carbide particles, such as Gd,C,[12,15] and YC2[8,14,17]. These tubules have diameters of 1 to 2 nm, similar to the longer tubules produced by the iron group metals, but have lengths of only 10 to 100 nm. These structures have been found in the primary soot, suggesting that they form in the gas phase. However, the similar structures reported for the case of Ni were found in the rubbery blanket surrounding the cathode[ 16,171. In that case, the nanotubes radiated from metal particles that were identified by electron diffraction to be crystalline fcc-Ni or Ni3C. The Ni-containing particles were typically encased in several graphitic carbon layers, and the free ends of the short, radial singlewalled tubes were generally observed to be capped. In the experiment of Lin et ai., Cu was used in the anode and single-layer nanotubes formed in the center region of the cathode deposit[l8]. These tubes had lengths of a few tens of nanometers and diameters of 1-4 nm. Unlike tubes produced using transition metals or lanthanides, these nanotubes usually had irregular shapes, with diameters varying along the tube axes. From this Lin et al. infer that the nanotube structures contain relatively high densities of pentagonal and heptagonal defects. The tubes were not found to be associated with Cu-containing particles. Copper crystallites loosely wrapped in graphitic carbon were occasionally found in the cathode deposit. Recently, a non-arc method leading to single-layer nanotube production was reported. Endo et al. demonstrated that sections of single-layer nanotubes form at early times when a benzene/hydrogen mixture is pyrolyzed at 1000°C over a graphite substrate[l9]. In this work, primary nanotubes quite similar to arcproduced carbon nanotubes form, in some cases with only single-layer graphene walls and diameters as small as 2-3 nm. At later times, these primary pyrolytic carbon nanotubes (or PCNTs) accrete additional amorphous pyrolytic carbon and grow into fibers with pm diameters and cm lengths. High-temperature annealing can then be used to increase the crystallinity of the fibers. The process to make PCNTs is distinguished from that used to make vapor-grown carbon fibers (VCGCF)[24,25] by the fact that VGCF is produced by thermally decomposing hydrocarbon vapor in the presence of a transition metal catalyst.
Fig. 1. Scanning electron micrograph of the soot taken from the chamber wall; the threads are nanotube bundles.
zyxwvutsrqpon zyxwvuts zyxwv C.-H. KIANG et af.
Fig. 2a. Bundles and individual single-layer carbon nanotubes bridge across a gap in a carbon film.
3. STRUCTURE OF SINGLE-LAYER CARBONNANOTUBES
The structure of an ideal straight, infinitely long, single-layer nanotube can be specified by only two parameters: its diameter, D,and its helicity angle, a, which take on discrete values with small increments[2,26]. These atomic scale structural parameters can in principle be determined from selected area diffraction patterns taken from a single tubule. Although for multilayer tubes numerous electron diffraction studies confirming their graphitic structure have been published, the very weak scattering from nm diameter single-layer tubes and their susceptibilityto damage by a 100-200 keV electron beam make it very difficult to make such measurements. Iijima was able to show by diffraction that a single-layer tube indeed had a cylindrical graphene sheet structure. Saito reported a similar conclusion based on diffraction from a bundle of several single-layer tubes[l7].
On the molecular scale, single-layer carbon nanotubes can be viewed either as one-dimensional crystals or as all-carbon semi-flexible polymers. Alternatively, one can think of capped nanotubes as extended fullerenes. For example, one can take a Csomolecule and add a belt of carbon to form a C,o. By repeating the process, one can make a long tubule of 0.7 nm diameter with zero helicity. Likewise, joining belts of 75 edge-sharing benzene rings generates a nanotube of about 6 nm diameter. Nanotubes typically have diameters smaller than multilayer tubes. TEM micrographs show that single-layer tubules with diameters smaller than 2 nm are quite flexible, and often are seen to be bent, as in Fig. 3a. Bends with radii of curvature as small as ten nm can be observed. Tubes with diameters larger than 2 nm usually exhibit defects, kinks, and twists. This is illustrated in the TEM image of several relatively large nanotubes shown in Fig. 3b. The diameter of the tubes seems to vary slightly along the tube axis due to radial defor-
Fig. 2b. Nanotubes aligned when a portion of soot was pulled apart.
zyxwvutsrqponm zyxwvu zyxwvuts C.-H. KIANG et al.
Fig. 2c. Aggregated single-layer nanotubes from soot produced by co-vaporizing Co and Bi.
mation. Classical mechanical calculations show that the tubes with diameters greater than 2 nm will deform radially when packed into a crystal, as indicated by TEM images presented by Ruoff et al.. The stability of nanotubes is predicted to be lowered by the defects. This may account for the observation that smaller tubes often appear to be more perfect because, with their higher degree of intrinsic strain, smaller tubes may not survive if defective. The most likely defects involve the occurrence of 5- and 7-fold rings. These defects have discrete, specific effects on the tube morphology, and can give changes in tube diameter, bends at specific angles, or tube closure, for example[29,30,3 11. By deliberately placing such defects in specific locations, it would be possible in principle to create various branches and joints, and thus to connect nanotubes together into elaborate 3-D networks[32,33]. Despite a wealth of theoretical work on the electronic structure [26,34-411, and vibrational properties
[38,42,43] of single-layer nanotubes, very little characterization beyond TEM microscopy and diffraction has been possible to date, due to the difficulty in separating them from the myriad of other carbon structures and metal particles produced by the relatively primitive synthetic methods so far employed. Recently, it was reported that the Raman spectrum of a sample containing Co-catalyzed nanotubes showed striking features that could be correlated with theoretical predictions of the vibrational properties of single-layer tubules. Kuzuo et al.  were able to use transmission electron energy loss spectroscopy to study the electronic structure of a bundle of single-layer nanotubes selected by focusing the electron beam to a 100nm diameter circular area. Features of the spectra obtained were shifted and broadened compared to the corresponding features for graphite and multilayer nanotubes. These changes were tentatively interpreted to be effects of the strong curvature of the nanotube wall.
Carbon nanotubes with single-layer walls P
4. THE METAL PARTICLES
The encapsulated ferromagnetic particles produced by this process may eventually be of technological interest, for example, in the field of magnetic storage media. Some work characterizing the magnetic properties of the encapsulated Co particles produced by arc co-evaporation with carbon has been recently reported. The phase and composition of the metalcontaining particles may also provide information on the growth conditions in the reactor. The temporal and spatial profiles of temperature, metal and carbon densities, and reaction rates all affect the growth of both these particles and the nanotubes. The composition of the metal-containing particles in the soot deposited at regions away from the electrode is not the same as for those found in the cathode deposit. For iron group metals, pure metallic particle as well as cementite phase (Fe,C, Co3C, and Ni,C) exist in the outer surface of the cathode deposit[ 161. These particles appear spher-
Fig. 3a. Small-diameter tubes are often bent and curled.
ical and are wrapped with layers of graphene sheet with no gaps. The low-temperature phases, a-Fe and a-hcp Co, form abundantly, whereas the high-temperature phases, P-Fe and 0-fcc Co, comprise less than 10% of the metal particle. In contrast, the metal particles found in the soot on the chamber wall contain mostly hightemperature phases, such as Fe,C, fcc-C0[3,47], and fcc-Ni[l6], and not all of the particles are wrapped in graphitic layers. These findings show that as the particles move away from the arc their temperature is rapidly quenched. The relatively fast time scale for reaction that this implies may be crucial for the growth of single-layer carbon nanotubes and, in particular, it may preclude the growth of additional layers of carbon on the single-layer tubules. The presence of sulfur is found to enhance the formation of graphitic carbon shells around cobaltcontaining particles, so that cobalt or cobalt carbide particles encapsulated in graphitic polyhedra are found throughout the soot along with the single-layer nano-
zyxwvutsrqponm zyxwvu zyxwvuts zyxwv C.-H. KIANG et a/.
Fig. 3b. Large-diameter tubes produced with Co and S present; the tubes shown have approximate diameters of 5.7, 3.1, and 2.6 nm.
tubes. Figure 4 is a high-resolution image of some encapsulated Co particles, which have structures reminiscent of those observed for Lac2 and YC2 particles found in cathode deposits[16,48-501. Crystallites en-
capsulated in graphitic polyhedra constitute about 30% of the total Co-containing particles. The role of sulfur in the formation of these filled polyhedra is not clear. Sulfur is known to assist the graphitization of
Fig. 4. Filled graphite polyhedra found in soot produced with an anode containing sulfur and cobalt.
zyxwvuts zyxwv zyxwvuts
C.-H. KIANGet ai.
vapor-grown carbon fibers, but the detailed process is not yet understood. 5. GROWTH OF SINGLE-LAYER CARBON NANOTUBES
There remains a major puzzle as to what controls the growth of these nanotubes, and how it precludes the formation of additional layers. The reaction conditions in the electric arc environment used for nanotube production to date are not ideal for mechanistic studies, since the plasma composition near the arc is very complex and inhomogeneous, making individual variables impossible to isolate. So far, we can only examine the product composition to extract clues about the growth mechanism. One feature that can be analyzed is the diameter distribution of single-layer carbon nanotubes formed. Table 1 summarizes the data available. This should be considered to be only a qualitative description, given the non-systematic sampling procedures, statistical uncertainties, and wide variations in the growth conditions used in various laboratories. The nanotube diameters were obtained from high-resolution TEM images. At a gross level, the most interesting aspect of the accumulated data is the consistency of the production of 1-2 nm diameter tubes by the various metals and combinations of metals. The exceptional cases are the combinations of Co with S, Pb, or Bi, which produce considerably large tubes. Even in those cases, the main peak in the distribution occurs between 1 and 2 nm. Figure 5 presents detailed histograms of the abundance of different di-
ameter nanotubes produced with Fe, Co, and Co/S, adapted from earlier reports[2,5]. In comparing the diameter distributions produced using Co and Co/S, there is striking correlation of both the overall maxima and even the fine structures exhibited by the distributions (Figs. 5b and 5c, respectively). For the cases where large diameter tubes (> 3 nm) are produced by adding S, Pb, or Bi to the cobalt, the tubes are still exclusively single-layered. We observed only one double-layer nanotube out of over a thousand tubes observed. This suggests that nucleation of additional layers must be strongly inhibited. The stability of nanotubes as a function of their diameter has been investigated theoretically via classical mechanical calculations[52,53]. The tube energies vary smoothly with diameter, with larger diameter tubes more stable than smaller ones. The narrow diameter distributions and occurrence of only single-layer tubes both point to the importance of growth kinetics rather than energetic considerations in the nanotube formation process. S, Pb, and Bi affect the Co-catalyzed production of single-layer nanotubes by greatly increasing the yield and the maximum size of the nanotubes. The formation of web-like material in the chamber is very dramatically enhanced. As noted above, these elements do not produce nanotubes without a transition metal present. How these effects arise and whether they involve a common mechanism is not known. In the production of VGCF, sulfur was found to be an effective scavenger for removing blocking groups at graphite basal edges. The added elements may assist the transport of carbon species crucial for the growth of nanotubes in the vicinity of the arc. Or they could act as co-catalysts interacting with Co to catalyze the reaction, or as promoters helping to stabilize the reactants, or simply as scavengers that remove blocking groups that inhibit tube growth. Growth models for vapor-grown carbon fibers (VGCF) have been proposed[24,25]. Those fibers, produced by hydrocarbon decomposition at temperatures around 12OO0C,are believed to grow from the surface of a catalyst particle, with carbon deposited on the particle by decomposition of the hydrocarbon migrating by diffusion through the particle, or over its surface, to the site where the fiber is growing. The fiber size is comparable to the size of the catalytic particle, but can thicken if additional pyrolytic carbon is deposited onto the fiber surface. It is tempting to think that single-wall nanotubes may also grow at the surfaces of transition metal particles, but particles much smaller than those typical in VGCF production. To date however, the long single-layer nanotubes found in the soot have not been definitely associated with metal particles. Thus, how the metal exerts its catalytic influence, and even what the catalytic species are, remain open questions. The urchin particles produced by lanthanide or Ni catalysts do show an association between the single-layer nanotubes and catalyst particles. In this case, the particles are 10 to 100 times larger than the tube diameters. In the case of singlelayer tubes produced by Cu in the cathode deposit,
zyxwvut zyxwv zyxwvu
L c1 0
Nanotube dlameter (nm)
Fig. 5. Diameter distributionsof nanotubes produced via different methods: (a) Fe catalyst in an Ar/CH, atmosphere, adapted from Ref. 2; (b) Co catalyst in He atmosphere, adapted from Ref. 5 ; (c) Cocatalyst with sulfur, about 4 at.% each, adapted from Ref. 5 .
zyxw zyxwvuts zyxw Carbon nanotubes with single-layer walls
growth occurs under extreme conditions of temperature and carbon density. The nanotubes produced also have very different characteristics. Therefore, we expect that their formation mechanism will be quite different. It is possible that instead of growth occurring at a metal particle interface, as has been proposed for VOCF, urchin particles[& 171, and long single-walled nanotubes, a mechanism more akin to those proposed for the growth of multilayer nanotubes on the cathode tip in an all-carbon environment may be involved[21,26,29,54]. In that case, it has been suggested that growth occurs at the free end of the nanotube, which protrudes out into the carbon plasma. Some features of the arc process are known and are relevant to growth models for single-layer nanotubes. Earlier isotope labelling analyses of fullerene formation shows that fullerenes formed in the arc are built up from atomic carbon[55-57]. Also, the production of nanotubes does not seem to depend on whether metal oxide or pure metal is used in the graphite anode. These results imply that both the metal and the carbon are completely atomized under the arc conditions, and that both the catalytic species and nanotubes must be built up from atoms or atomic ions. This fact, together with the consistency of the diameters of the single-layer nanotubes produced in the gas phase by transition metal catalysts, suggests a model where small catalytic particles rapidly assemble in a region of high carbon density. Single-layer tubules nucleate and grow very rapidly on these particles as soon as they reach a critical size, leading to the relatively narrow diameter distributions observed. If nucleation of additional layers is slow, the rapid drops in temperature and carbon density as the tubes move away from the arc could turn off the growth processes before multilayers can form. 6. FUTURE DIRECTIONS
Experimental research on single-layer nanotubes is still in a very early stage. Understanding the growth mechanism of these nanotubes remains a great challenge for scientists working in this area. Not even the nature of the catalytically active species has been established to date. Developing better controlled systems than standard arc reactors will be necessary to allow the dependence of tube growth on the various important parameters to be isolated. The temperature and the carbon and metal densities are obvious examples of such parameters. In the arc plasma, they are highly coupled and extremely inhomogeneous. Knowledge of the growth mechanism will possibly allow us to optimize the fabrication scheme and the characteristics of the nanotubes. A second key problem is to devise means to separate the tubes from the soot and metal particles, either chemically or mechanically. This is an essential step towards manipulation and thorough characterization of these materials. Recently, it was reported that a significant fraction of the metal particles could be removed from the sample by vacuum annealing it at
high (1600°C) temperature[ll]. The amorphous carbon soot particles, however, are difficult to remove, and the oxidative approach used with some success to isolate multilayer tubes seems to destroy the singlelayer tubes. Measurement of the mechanical, optical, electrical, and magnetic properties requires a clean sample to interpret the data unambiguously. Tests of the dependence of electrical conductivity and mechanical strength on the tube diameter should be done, and may soon be feasible with the availability of nanotubes with a wide range of diameters. The unique properties of single-layer carbon nanotubes will continue to inspire scientists in diverse fields to explore their properties and possible applications. Defect-free nanotubes are predicted to have very high tensile strength. A theoretical calculatior, of the elastic constant for single-layer nanotubes gives a result consistent with a simple estimate based on the c, elastic constant of graphite (cI1= 1.06 TPa). Using this constant, one finds a force constant of 350 Nt/(m of edge) for graphene sheet. Multiplying this value by the circumference of a 1.3 nm diameter nanotube gives Nt for such a tube. an elastic constant of 1.45 x Macroscopically, a bundle of these tubes 25 pms in diameter would support a 1-kg weight at a strain of 3%. In comparison, a steel wire of that diameter would break under a load of about 50 gm. When nanotubes are assembled into crystalline bundles, the elastic modulus does not decrease linearly with tube diameter but, rather, it remains constant for tube diameters between 3 and 6 nm, suggesting the strength-to-weight ratio of the crystal increases as the tube diameter increases . The anisotropy inherent in the extreme aspect ratios characteristic of these fibers is an important feature, particularly if they can be aligned. Ab initio calculations show that these nanotubes could be onedimensional electric conductors or semiconductors, depending on their diameter and helicity[36,39,59]. Other applications of carbon nanotubes have been proposed in areas that range widely, from physics, chemistry, and materials to biology. Examples, such as hydrogen storage media, nanowire templates, scanning tunneling microscopy tips, catalyst supports, seeds for growing carbon fibers, batteries materials, reinforcing fillings in concrete, etc. provide ample motivation for further research on this pseudo-one-dimensional form of carbon.
Acknowledgement-This research is partially supported by the NSF (ASC-9217368) and by the Materials and Molecular Simulation Center. We thank J. Vazquez for help with the SEM imaging of nanotubes, G . Gorman and R. Savoy for X-ray analysis, and M. S. de Vries for mass spectrometry. REFERENCES
1. S. Iijima, Nature 354, 56 (1991). 2. S. Iijima and T. Ichihashi, Nature 363, 603 (1993). 3. D. S. Bethune, C. H. Kiang, M. S. deVries, G. Gorman, R. Savoy, J. Vazquez and R. Beyers, Nature 363, 605 (1993). 4. P. M. Ajayan, J. M Lambert, P. Bernier, L. Barbedette,
zyxwvutsrq zyxwvutsrq zyxwvutsr zyxwvut zyxwvu zyxwvutsrq zyxw zyxwvutsr C.-H. KIANG et al.
C. Colliex, and J. M. Planeix, Chern. Phys. Lett. 215, 509 (1993). 5. C.-H. Kiang, W. A. Goddard 111, R. Beyers, J. R. Salem, and D. S. Bethune, J. Phys. chem. 98,6612 (1994). 6. C.-H. Kiang, P. H. M. van Loosdrecht, R. Beyers, J. R. Salem, D. S. Bethune, W. A. Goddard 111, H. C . Dorn, P. Burbank, and S. Stevenson, Proceedings of the Seventh Internutional Symposium on Small Particles und Inorganic Clusters, Kobe, Japan, Surf. Rev. Lett. (in press). 7. S. Seraphin and D. Zhou, Appl. Phys. Lett. 64, 2087 (1994). 8. S. Seraphin, J. Electrochem. SOC. (USA) 142,290 (1995). 9. S. Seraphin, D. Zhou, J. Jiao, M. S. Minke, S. Wang, T. Yadav, and J. C . Withers, Chem. Phys. Lett. 217, 191 (1994). 10. Y. Tapesh, J. C. Withers, S. Seraphin, S. Wang, and D. Zhou, In NovelForms of Carbon, MRS Proc. 349, pp. 275-281. Mat. Res. SOC.,Pittsburgh (1994). 11. J. M. Lambert, P. M. Ajayan, P. Bernier, J. M. Planeix, V. Brotons, B. Cog, and J. Castaing, Chem. Phys. Lett. 226, 364 (1994). 12. S. Subramoney, R. S. Ruoff, D. C. Lorents, and R. Malhotra, Nature 366, 637 (1994). 13. S. Wang and D. Zhou, Chem. Phys. Lett. 225, 165 (1994). 14. D. Zhou, S. Seraphin, and S. Wang, Appl. Phys. Lett. 65, 1593 (1994). 15. S. Subramoney, P. van Kavelaar, R. S. Ruoff, D. C. Lorents, and A. J. Kazmer, In Recent Advances in the Chemistry and Physics of Fullerenes and Related Materials (Edited by K. M. Kadish and R. S. Ruoff). The Electrochemical Society, Pennington, NJ (1994). 16. Y. Saito, T. Yoshikawa, M. Okuda, N. Fujirnoto, K. Sumiyama, K. Suzuki, A. Kasuya, and Y. Nishina, J. Phys. Chern. Solids 54, 1849 (1993). 17. Y. Saito, M. Okuda, N. Fujimoto, T. Yoshikawa, MI. Tomita, and T. Hayashi, Jpn. J. Appl. Phys. 2 Lett. (Japan) 33, L526 (1994). 18. X. Lin, X. K. Wang, V. P. Dravid, R. P. H. Chang, and 5. B. Ketterson, Appl. Phys. Lett. 64, 181 (1994). 19. M. Endo, K. Takeuchi, S. Igarashi, K. Kobori, M. Shiraishi, and H. W. Kroto, J. Phys. Chem. Solids 54, 1841 (1993). 20. D. Ugarte, Nature 359, 707 (1992). 21. Y. Saito, T. Yoshikawa, M. Inagaki, M. Tomita, andT. Hayashi, Chem. Phys. Lett. 204, 277 (1993). 22. R. S. Ruoff, J. Tersoff, D. C. Lorents, S. Subramoney, and B. Chan, Nature 364, 514 (1994). 23. J. Tersoff and R. S. Ruoff, Phys. Rev. Lett. 73, 676 (1994). 24. M. Endo, Chemtech 18, 568 (1988). 25. N. M. Rodriguez, J. Mater. Res. 8, 3233 (1993). 26. R. Saito, M. Fujita, G. Dresselhaus, and M. S . Dresselhaus, Matls. Sci. Eng. B19, 185 (1993). 27. P. W. Fowler, J. Phys. Chem. Solids (UK) 54, 1825 (1993). 28. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, Chern. Phys. Lett. 195, 537 (1992). 29. S. Iijima, Mutls. Sci. Engin. B19, 172 (1993). 30. B. I. Dunlap, Phys. Rev. B 49, 5643 (1994). 31. B. I. Dunlap, Phys. Rev. B 50, 8134 (1994). 32. B. I. Dunlap, Phys. Rev. B 4 6 , 1933 (1992).
33. L. A. Chernozatonskii, Physics Lett. A (Netherlands) 172, 173 (1992). 34. J. W. Mintmire, D. H. Robertson, and C. T. White, J. Phys. Chern. Solids 54, 1835 (1993). 35. R. Saito, M. Fujita, G. Dresselhaus, and M. S. Dresselhaus, Phys. Rev. B46, 1804 (1992). 36. R. A. Jishi, M. S. Dresselhaus, and G . Dresselhaus, Phys. Rev. 848, 11385 (1993). 37. M. S. Dresselhaus, G. Dresselhaus, and R. Saito, Solid State Commun. (USA) 84, 201 (1992). 38. R. A. Jishi, D. Inomata, K. Nakao, M. S. Dresselhaus, and G. Dresselhaus, J. Phys. Soc. Jpn. (Japan) 63,2252 (1994). 39. N. Hamada, S. I. Sawada, and A. Oshiyama, Phys. Rev. Lett. 68, 1579 (1992). 40. C. J. Mei and V. H. Smith Jr., Physicu C 213, 157 (1993). 41. M. Springborg and S. Satpathy, Chem. Phys. Lett. 225, 454 (1994). 42. R. A. Jishi and M. S. Dresselhaus, Phys. Rev. B45, 11305 (1992). 43. R. A Jishi, L. Venkataraman, M. S. Dresselhaus, and G. Dresselhaus, Chem. Phys. Lett. 209,77 (1993). 44. J. M. Holden, P. Zhou, X-x Bi, P. C. Eklund, S. Bandow, R. A. Jishi, K. Das Chowdhury, G. Dresselhaus, and M. S. Dresselhaus, Chem. Phys. Lett. 220, 186 (1994). 45. R. Kuzuo, M. Terauchi, M. Tanaka, and Y. Saito, Jpn. J. Appl. Phys. 2, Lett. 33, L1316 (1994). 46. M. E. McHenry, S. A. Majetich, J. 0. Artman, M. DeGraef, and S. W. Staley, Phys. Rev. B 49, 11358 (1994). 47. S. A. Majetich, J. 0. Artman, M. E. McHenry, N. T. Nuhfer, and S. W Staley, Phys. Rev. B48, 16845 (1993). 48. R. S. Ruoff, D. C. Lorents, B. Chan, R. Malhotra, and S. Subramoney, Science 259, 346 (1993). 49. Y. Saito, T. Yoshikawa, M. Okuda, M. Ohkohchi, M. Inagaki, Y. Ando, A. Kasuya, and Y. Nishina, Chern. Phys. Lett. 209, 72 (1993). 50. S. Seraphin, D. Zhou, J. Jiao, J. C. Withers and R. Loutfy, Appl. Phys. Lett. (USA) 63, 2073 (1993). 51. H. Katsuki, K. Matsunaga, M. Egashira, and S. Kawasumi, Carbon 19, 148 (1981). 52. D. H. Robertson, D. W. Brenner, and J. W. Mintmire, Phys. Rev. B 45, 12592 (1992). 53. A. A. Lucas, Ph. Lambin, and R. E. Smalley, J. Phys. Chem. Solids 54, 587 (1993). 54. M. Endo and H. W. Kroto, J. Phys. Chem. 96, 6941 (1992). 55. G. Meijer and D. S. Bethune, J. Chern. Phys. 93, 7800 (1990). 56. R. D. Johnson, C. S. Yannoni, J. R. Salem, andD. S. Bethune, In Clusters and Cluster-Assembled Materials, MRS Proc. 26 (Edited by R. S. Averbach, J. Bernholc, and D. L. Nelson), pp. 715-720. Materials Research Society, Pittsburgh, PA (1991). 57. T. W. Ebbesen, J. Tabuchi, and K. Tanagaki, Chern. Phys. Lett. 191, 336 (1992). 58. T. W. Ebbesen, P. M Ajayan, H. Hiura, and K. Tanigaki, Nature 367, 519 (1994). 59. R. Saito, M. Fujita, G. Dresselhaus, and M. S . Dresselhaus, Appl. Phys. Lett. 60,2204 (1992).
CARBON NANOTUBES: I. GEOMETRICAL CONSIDERATIONS R. SETTON
Centre de Recherche sur la Matiere DivisCe, CNRS, 1 B rue de la Ftrollerie, F 45071 OrlCans Cedex 2, France (Received 22 August 1994; accepted 15 September 1994)
Abstrdct-The geometrical conditions pertaining to closure, helicity, and interlayer distance between successive layers with circular cross-sections in carbon tubules (nanotubes) have been examined. Both the intralayer length of the C-C bonds and the interlayer distance between successive layers must vary with the radius of the layers. The division into groups of the sheets in nanotubes is found to be due to the reciprocal interaction of the interlayer distance variations and of the conditions required to maintain constancy of the pitch angle. Key Words-Carbon
zyxw zyxw zyxw
nanotubes, pitch angIe, helix angle, interlayer distance, carbon-carbon intralayer
folds. The sign of 8 determines the helicity of the scroll, counterclockwise (e> 0) or clockwise (e< 0). The consequence of the presence of scroll helicity in a tubule is expected to be that any increase (decrease) of the intralayer C-C distance G will increase (decrease) the local length of the spiral, but not necessarily the mean interlayer distance, since the scroll can easily adapt its radius of curvature to minimize, if necessary, any energetic strain due to a stress in the local bond lengths.
Carbon tubules (or nanotubes) are a new form of elemental carbon recently isolated from the soot obtained during the arc-discharge synthesis of fullerenes[11. High-resolution electron micrographs do not favor a scroll-like helical structure, but rather concentric tubular shells of 2 to 50 layers, with tips closed by curved, cone-shaped, or even polygonal caps. Later work has shown the possibility of obtaining singleshell seamless nanotubes. Recently, the structure of some helical carbon nanotubes was examined, and the present work is an attempt at completing the geometrical approach to the structural problems encountered in the case of tubules with circular cross-sections. However, most of the conclusions in the present work are applicable to nanotubes with polygonal cross-sections that have also been shown to exist.
2.2 Screw helicity The second type of helicity can affect both scrolls and individual cylinders. It will be present when neither the a nor the b unit vector of the basic twodimensional graphite lattice of the unfolded scroll or cylinder is at an angle of 0" or at a multiple of 30" with the direction of the cylinder axis (Fig. 2). The situation is complicated by the fact that whenever screw helicity affects a seamless cylindrical layer, any change in the value of G must necessarily affect the radius r of the cylinder. It is therefore highly likely that the interlayer distance d between two successive cylinders is not strictly constant in any multilayered tubule with a circular cross-section, since the adverse effect of the elastic strain on the sp2 orbitals and the resulting distribution of charges- which undoubtedly affect the intralayer C-C distance-progressively decreases as the circumference and the radius of curvature of the cylinders increase. As justified later, one is therefore led to introduce a parameter 6d or 6r to characterize the smalI variations of r with respect to a hypothetical nominal value likely to be encountered even if, strictly speaking, the variation 6G should also be taken into account.
zyxwvut zyxwvutsr zyxwvuts zyxwvutsr 2. THEORY
Leaving aside the complications engendered by the presence of end-caps and considering, therefore, only the cylindrical part of the tubules, one must differentiate between two types of helicity.
2.1 Scroll helicity The presence of scroll helicity replaces a set of concentric cylinders by a single sheet rolled upon itself (Fig. 1). Assuming that the distance between the successive rolls of the scroll is constant, its cross-section can be conveniently represented in polar coordinates by the Archimedean spiral:
2.3 Symmetric non-helical tubules and cylinders
In the absence of both types of helicity, the nonhelical or symmetric tubule consists-of a set of cylin-
where a, is the initial radius of the innermost fold and d is the (constant) distance between successive
zyxwvutsrq zyxwvu zyxwvuts R. SETTON
z y x w v u t s r q p o n m l k zyxw zyxwvu Fig. 3. The two possible orientations of the hexagons in nonhelical sheets, relative to the cylinder axis (broken line); (a) case I; (b) case I1 (see text).
Fig. 1. Approximate cross section of a tubule with scroll helicity. The distance d between successive rolls of the spiral is assumed to be constant, and no is the initial radius of the innermost fold.
dius ri of the cylinder can conveniently be described in terms of two orthogonal vectors, Pi and Qi (Fig. 4), respectively integral multiples of the unit vectors x and 7 with moduli I = (3/2)G and I y I = (&/2)G. For the ith layer, we can write:
drical sheets which, for simplicity, will be assumed to have a common axis and a circular cross-section. The hexagons of the unrolled cylinders all have one of their three sets of parallel opposite sides respectively perpendicular (case I) or parallel (case 11) to the common axis of the cylinders (Fig. 3). The orientation of the hexagons with respect to the tube axis of the unrolled ith cylinder as well as the ra-
or, for the scalars R i , Pi, Qi,
where Pi, Qi are integers of identical parity, and Ri = 27rri.
The pitch angle ai characteristic of this orientation of the hexagons is: ai = arctan(Qi/fiPi),
but one can also distinguish an apparent angle of pitch
pi between the helical rows of unbroken hexagons and the plane perpendicular to the cylinder axis, with
Although the limits of
this angle can be limited to 30", since every ( P i ,Qi) doublet is associated with a corresponding doublet (Pi,-Qi), symmetric of (Pi,Qi) with respect to a = O", yielding the same value of the radius (Fig. 5 ) and characterizing the stereoisomer of the chiral ith cylindrical sheet, The doublet (Pi,Qi) is also equivalent to the doublet (Pi, Qj), with Pi= ( P , + Q,)/2 and Qi = (3P, - 2Qi)/2, with the pitch angle ai = 60" - ai. which also yields the same value of ri.
Fig. 2. A portion of an unrolled cylinder with screw helicity. The broken line is parallel to the cylinder axis, and the cylindrical sheet has been cut along a generatrix (full line parallel t o the cylinder axis). a and b are the unit vectors of the two-dimensional carbon layer in sp2 hybridization.
Carbon nanotubes: I. Geometrical considerations
zyxwvutsr zyxwvuts zyxwvu zyxwvutsrqp zy zy
Fig. 4. Screw helicity: the system of (P, Q) coordinates used to describe the orientation of the twodimensional sp2 carbon layer in an unrolled cylindrical sheet whose edges are shown by the slanted unlabelled full lines. Closure of the cylinder is obtained by rolling the sheet around the direction of the cylinder axis given by the dotted line and superimposing hexagons A and B. The slanted dashed lines correspond to a continuous line of unbroken hexagons of the cylinder, and indicate the apparent angle of pitch 0.
zyxwvutsrqponmlkj zyxwvuts zyxwv hence, assuming that writing d for dj,j + L ,
l.t is therefore possible to impose the limits:
is practically constant and
2 ~ =d nj,j+l (I)3G/2
= integral part of)
ni,j+l(I) = 10
0 IQj IPi
in which Qi = 0 and Qi = Pi correspond to cases I and I1 respectively, and for which eqn (4) becomes:
27rri(I) = Pi3G/2
and 2Tri(11) = P,&G.
Referring now to the symmetric tubule, the interlayer distance dj,j+n between two layers of radii ri and rj;-+n IS: di,i+n
and, for two consecutive layers, d f , j + = l 0.339 nm. For the configuration of hexagons in case I, the inFig. 5 . Screw helicity: the three vectors corresponding to crease in length of the circumference of the (i 1)th ( R /= Gd26, with P, = 5 , Q , = 3 and P, = 4, Q, = 6 (see laver with reswct to the circumference of the ith layer text). The vector (Pi,-Qi) characterizes the optical isomer must be equal to an integral and even multiple of I x I ; of (Pi,Qd.
zyxwvuts zyxwvu zyxwvutsr zyxwvutsrqpo zyxwvu zy zyxwvu zyxw
if d = 0.339 nm and G = to better than 1 x 0.142 nm. This is well illustrated by the sequence formed from the values rl = 0.678 nm, G = 0.142 nm, d = 0.339 nm, and 6r/r = 51.5%, which give more than 30 consecutive non-helical (a! = 0") symmetric cylinders, with characteristics ri (nm) = 0.678 + ( i - 1)d and Pi = ( i 1)lO.
2.4 Symmetrical helical cylinders with a = 30" For the configuration of hexagons in case 11, ni,i+l(II) should now be an integral and even multiple of Iy1 or, using eqn (11), = ni,i+,(II)d?G.
(ri+l/G)' = ( 3 / 1 6 ~ ~ ) ( 3 P f + ~ Qi",,)
[(ri+ d)/G]' = (3/16.rr2)[3(Pi +p)'
+ ( Q i + q)']
This equality is not even approximately satisfied for small integral values of ni,i+l(II).There is, however, a possibility offered by the distance di,i+3,that is, for 1.02 nm, namely: ni,i+3(11) = 2 ~ d , , ~ + ~ / & C
sible to find long series of successive cylindrical sheets with 01 = O", it is clear that one should have, for two successive cylinders with identical helicity:
in which p and q are, respectively, integral increments of Pi and Qi. For the pitch angles of the two cylinders to be equal, we must have:
(16) and it can be shown that
= 26 to better than 0.2%. In other words, if a ( P i , Q i ) doublet yields a = 30", which is the pitch angle corresponding to case 11, the chances are high that this angle will be repeated for the (i 3)th cylinder. A good example of this is given by the series described by the values rl = 0.71 nm, G = 0.1421 nm, d = 0.339 nm, and 6d/d = 2%, which yield CY = 30" for i = 1,4, 10, 19, 22, 27, 30, 33, 36, 39, . . ., with most differences between successive values of i either equal to 3 or to a multiple of 3, and the values P, = Qi = I&, 44, 96, 174, 200, 243, 269, 295, 321, 347,. . ., which show the expected differences.
2.5 Symmetric helical tubes and cylinder with a different from 0" or 30" Equality (4) can be rewritten as:
( r i / G ) 2= (3/l6a2)(3Pf
Since the first bracket on the right-hand side is a constant and the second is an integer, it is evident that, for any particular i, some leeway must exist in the value of the ratio ri/G for the equality to be satisfied. Here too, the presence of screw helicity must affect either ri, or G , or both. In view of the fairly small variations of G allowed if the hybridization of the C atoms is to remain sp', and since the deformation of the C orbitals decreases as the radius of the cylindrical sheets increases, the distance between successive cylinders must decrease and probably tend towards a value characteristic of turbostratic graphite. The second problem associated with helical symmetric cylindrical sheets addresses the possibility of finding the same helix angle or pitch in two neighbouring sheets. Apart from cases similar to the one described above (case I, section 2.3) in which it is pos-
In view of the remarks in Q 2.3, it is legitimate to substitute the value 15 for the round bracket in the r.h.s. of eqn (22). Taking then into account the fact that the maximum and minimum possible values of p are obtained when q = 0 and q = p , respectively, eqn (22) yields: 8.66 ~p
The only doublets consistent with this inequality, with the necessity of identical parity for p and q , and with values of r , close to 0.34 nm, are given in Table 1 (from which the doublet (10,O) can be excluded since it is characteristic of a symmetrical, non-helical sheet). Hence, if 6r = 0, the necessary conditionsfor two successive helical cylindrical sheets to have strictly identical pitch angles are:
q : p = 7 : 9 , or 2:10, or 4:10,
since all other values would give either d < 0.334 nm (which is already less than d of graphite and, there-
Table 1. ( p , q ) increments for obtaining identical successive pitch angles
Interlayer distance d (nm)
Pitch angle CY'
(9,7) (10,O) (103 (10~4)
0.334 0.339 0.341 0.348
zyxw zyxwvuts zyxwvutsr zyxwvu 63
Carbon nanotubes: I. Geometrical considerations
zyxwvutsrq zyxwvutsr zyxwvuts
fore, highly unlikely) or d > 0.348 nm (Le., at least 4% Table 3. Computed characteristics of a 28-sheet tubule showing the division into groups of sheets above the value of graphite and also unlikely). If both conditions are met, the pitch angle is 24.18",or 6.59", i (pi,Qi) ri (nm) cyo or 13.00". If only condition (25) above is operative, the successive values of a will be nearly but not strictly 0.475 1 0 (14~0) 2 0.814 0 (24,O) equai, and will be different from these three values. Two examples illustrate these points: 3 1.153 1.94 (34,2)
(b) the five successive cylindrical sheets with r, = 10.22nm, G =0.142 nm, d =0.34 nm, 6d/d = f I S % , and the characteristics shown in Table 2. A "singlehelix angle of about 3"" was observed in the selected area electron diffraction pattern of a four-sheet symmetric helical tube, but the small variations of a shown in Table 2 would obviously not have been visible in the diffractogram shown in the reference.
2.6 Sheet groups It has also been stated that "the helix angle (of a multiple-sheet helical tube) changes about every three to five sheets" so that the gross structure of the tube is constituted by successive groups of cylindrical sheets, with the helix angles increasing by a constant value from each group to the next. In light of the arguments developed in the preceding paragraphs, and except for the specific cases a = O", 6.59", 13.00", 24.18", the pitch angle of the sheets within a group is more likely to be nearly constant rather than strictly constant. This is illustrated by the values in Table 3 showing the characteristics of the 28 sheets in a tube whose inner and outer radii are, respectively, equal to 0.475 and 9.66 nm, calculated on the basis of rl = 0.476 nm, d = 0.34 nm, G = 0.142 nm, 6d/d = +0.8%. Since a is not strictly constant within each group, it is more appropriate to consider a mean value ( a ) of the pitch angle for each group, as shown in Table 4. Only in the first group of sheets (i = 1 to 2) is a truly constant ( a = 0"). For all the other groups, the increments ( p 9q ) of the (Pi, Q,) doublets are constant and equal to (10,2). In fact, it is because these increments are identical that the group pitch angles are nearly constant when the values of Piand Qiare sufficiently Iarge, which is not yet the case in the second group. The above series also illustrates an experimentally established fact: Except for the change of mean vd-
(44,4) (54,6) (64,8) (74,101 (84,121
1.494 1.834 2.175 2.516 2.857
3 .oo 3.67 4.13 4.46 4.72
9 10 11
(94,12) (104~4) (1 14,16)
3.195 3.566 3.877
4.22 4.44 4.63
12 13 14
(123,31) (133,33) (143,35) (1S3,37) (163,39)
4.214 4.555 4.896 5.237 5.578
8.28 8.15 8.04 7.95 7.87
17 18 19
(171,61) (18 1,63) (191,65)
5.919 6.259 6.599
11.64 11.36 11.12
20 21 22 23
(202,56) (212,SS) (222,60) (232,62)
6.935 7.276 7.617 7.958
24 25 26 27 28
(239,9 1) (249,93) (259,95) (269,97) (279,99)
8.296 8.635 8.975 9.315 9.655
12.40 12.17 11.96 11.76 11.56
4 5 6 7 8
(a) the unbroken series of 21 cylinders with a = 6.59", r, = 0.6825 nm, G = 0.142 nm, d = 0.341 nm, 6d/d = &1.5%, with Qi:Pi = 2:10, PI = 20, Pz,= 220, and q : p = 2:10 in all cases;
8.98 8.87 8.77
ues between groups 2 and 3 , and 5 and 6, the successive values of ( a ) increase by a nearly constant amount, namely, about 3 to 4". The question then arises as to the reason causing the modification of Q! between two successive groups, such as the one occurring between i = 11 and i = 12. If (P12, Q12)had been (124,18) instead of (123,31), r I 2 would have been 4.218 nm with a = 4.78" (Le., within 6d/d = +1.0% instead of kO.8% imposed for the values in Table 3). Hence, during the actual synthesis of the tube, the end of each group must be determined by the tolerance in the G values accepted by the spz orbitals compatible with the need to close the cylindrical sheet. Although the physical growth mechanism of the cylindrical sheets is not yet fully known, the fact that
Table 4. Group characteristics of the 28-sheet nanotube described in Table 3
Table 2. Computed characteristics of a five-sheet symmetric tubule with a nearly constant pitch angle I
1 2 3
10.22 10.56 10.90 11.24 11.58
(301,29) (31 1,31) (321,31) (33 1,33) (341,33)
3.18 3.29 3.19 3.29 3.20
1 2 3 4 5 6
Range of i
1 to 2 3 to 8 9 to 1 1 12 to 16 17 to 19 20 to 23 24 to 28
10,o 10,2 10,2 10,2 10,2 10,2 10,2
0 3.65 4.43 8.06 11.37 8.93 11.97
zyxwv zyxwvuts zyxwvuts zyxwvu R. SETTON
successive sheets have nearly constant helicity suggests the following mechanism: once the ith (topmost) sheet is formed, C, species in the gas phase (n = 3,1,2. . . , in order of decreasing abundance) condense onto the outer surface of the tube, probably at a distance slightly larger than 0.34 nm, in registry with the underlying substrate and in sp2 hybridization, since this configuration is the one that best minimizes the energy of the system. The ith sheet thus constitutes the template for the construction of the ( i + 1)th sheet, and the helicity of the as-yet-unclosed cylinder during its formation is the same as that of the underlying substrate. This process continues until the C atoms on either side of the cut form the C-C bonds that close the cylinder. If the geometric characteristics of these bonds are too different from 120" and G = 0.142 nm, the pitch angle will change to the immediately higher or lower value, thus ensuring closure. Once the cylinder is closed, and even if closure only involved a single row of hexagons, the following rows of the cylindrical sheet will necessarily have the same pitch angle, at least as long as the sheet is growing over an existing substrate.
2.8 Influence of the innermost cylinder If the template effect of Endo and Kroto does indeed exist and the growth of the tubule occurs outwards, a knowledge of the Characteristics of the innermost tube is then of paramount importance in any attempt at modelizing the structure of a symmetric nanotube[111. By reversing eqn (17), possible values for P1and Q , can be obtained from
zyxwvuts zyxwvuts 3P;
+ (212 = (16a2/3) [ ( r l / G ) 2* W r ] ,
and the inequalities (8) and (9), provided rl has been determined (say, by HRTEM -high resolution transmission electron microscopy), and G is arbitrarily fixed, say, at G = 0.142 nm. Although the task may become formidable if r1 and/or 6r/r are large, the number of possibilities is strictly limited, especially since selected area electron diffraction (SAED) can provide narrower limits by giving a first approximation of the pitch angle. 3. CONCLUSION
It is clear that a large number of parameters influence the formation of the sheets in a tubule and that 2.7 Smallest inner tube diameter their relative importance is still unknown, as is also the Liu and Cowley have reported the observation of innermost cylinders with diameters as small as 0.7 cause of the occurrence of the defects responsible for or 1.3 nm. The first value is only slightly larger than the eventual polygonization of the sheets. Although the model presented here highlights the necessity of in0.68 nm, the well known diameter of the Cs0 mol6r ecule[lO], while the second is in fair agreement with cluding, as one of the parameters, the uncertainty or 6d on the separation of successive cylindrical sheets, 1.36 nm, the calculated diameter Cm. As shown in Table 5 , there are 5 (PI,Q1)doublets which, with G = it is impossibIe to predict with absolute certainty the 0.142 nm, give rl = 0.35 nm +3%, and 14 (P1,Q1) final characteristics of any of these sheets, symmetric doublets (not all are given in Table 4) for the larger or not, on the basis of the characteristics of thepreof the two values within k5%. It is interesting to find vious one. Nevertheless, a number of features of their structure, such as the presence or absence of helicity, that there is, in both cases, the possibility of forming and the presence of groups of sheets with nearly the a non-helical cylindrical sheet with or = Oo, namely same angle of pitch, can be explained and quantified. ( P , , Q , ) = (10,0), rl = 0.339 nm, and (Pl,QI)=
(20,0), rl = 0.678 nm, with the first row of C atoms
corresponding to one of the equatorial cuts of C60or of C240;but ignorance of the actual mechanism of formation of the first cylindrical sheet forbids an objective choice among the various possibilities.
Table 5 . Some possible characteristics of symmetric sheets with the smallest observed radii
0.339 0.341 0.348 0.352 0.359 0.626 0.644 0.665 0.678 0.679
0 6.59 13.00 30 19.11
30 1.74 30 0 3.30
1. S. Iijima, Nature 354, 56 (1991). 2. X. Lin, X. K. Wang, V. P. Dravid, R. P. H. Chang, and
J. B. Ketterson, Appl. Phys. Letters 64, 181 (1994). 3. M. Liu and J. M. Cowley, Carbon 32, 393 (1994). 4. A. Setton and R. Setton, Synth. Met. 4, 59 (1981). 5 . T. W. Ebbessen and P. M. Ajayan, Nature 358, 220 (1992). 6 . D. R. Stull and G . C. Sinke, Thermodynamicproperties of the elements (No. 18, Advances in Chemistry Series), pp. 66-69. American Chemical Society, Washington (1956). 7. L. A. Girifalco and R. A. Lad, J. Chem. Phys. 25,693 (1956). 8. J.-C. Charlier and J.-P. Michenaud, Phys. Rev.Lett. 70, 1858 (1993). 9. M. Endo and H. W. Kroto, J. Phys. Chem. 96, 6941 (1992). 10. P. A . Heiney, J. E. Fischer, A. R. McGhie, W. J. Romanow, A. M. Denenstein, J. P. McCauley, Jr., A. P. Smith 111, and D. E. Cox, Phys. Rev.Lett. 66,291 (199 1). 11. V. A. Drits and C. Tchoubar, X-Ray diffraction by disordered lamellar structures. Springer-Verlag, Berlin (1 990).
SCANNING TUNNELING MICROSCOPY OF CARBON NANOTUBES AND NANOCONES KLAUSSATTLER
University of Hawaii, Department of Physics and Astronomy, 2505 Correa Road, Honolulu, HI 96822, U.S.A.
(Received 18 July 1994; accepted 10 February 1995)
Abstract-Tubular and conical carbon shell structures can be synthesized in the vapor phase. Very hot carbon vapor, after being deposited onto highly oriented pyrolytic graphite (HOPG), forms a variety of nanostructures, in particular single-shell tubes, multishell tubes, bundles of tubes, and cones. The structures were analyzed by scanning tunneling microscopy (STM) in UHV. Atomic resolution images show directly the surface atomic structures of the tubes and their helicities. A growth pathway is proposed for fuilerenes, tubes, and cones. Hey Words-Carbon
nanotubes, fullerenes, STM, fibers, nanostructures, vapor growth.
yielding quite realistic three-dimensional images from tube terminations. Also, besides a difference in rnorphology, open and closed ends show a difference in electronic structure. Open ends appear with ‘highlighted’ edges in STM images, which is due to an enhanced dangling bond electron state density. Closed ends do not have such highlighted edges. The growth pathway of various fullerene- and graphene-type nano-objects may be related. They are synthesized in the vapor phase and often appear simultaneously on the same sample. A common growth mechanism with similar nucleation seeds may, therefore, lead to these different structures.
Hollow carbon nanostructures are exciting new systems for research and for the design of potential nanoelectronic devices. Their atomic structures are closely related to their oute: shapes and are described by hexagonal/penitagonal network configurations. The surfaces of such structures are atomically smooth and perfect. The most prominent of these objects are fullerenes and nanotubes[l]. Other such novel structures are carbon onions and nanocones. Various techniques have been used to image nanotubes: scanning electron microscopy (SEM)[ 11, scanning tunneling microscopy (STM)[4-71, and atomic force microscopy (AFM)[S]. Scanning probe microscopes are proximity probes. They can provide threedimensional topographic images and, in addition, can give the atomic structure of the surface net. They can also be used to measure the electronic (STM) and elastic (AFMJ properties of small structures. STM is restricted to electrically conducting objects, but AFM does not have this constraint. STM and AFM images give directly the threedimensional morphology of tubes and are consistent with the structures inferred from SEM. In addition, atomically resolved STM images make direct helicity determinations possible. They give information about the nature of stacking of concentric carbon layers within the nanotubes via modifications of their surface density of states. STM is sensitive to such small lateral local density of states variations. Contours taken from the ends of the tubes show that some of them are open and others are closed. Many images indicate that the closed tubes have hemispherical caps. Such terminations can be modeled by fullerene hemispheres with 5 / 6 networks. ICis not easy to determine detailed properties of the tube terminations using STM or AFM. These microscopes cannot image undercut surfaces and the tip shape is convoluted with the cap shape of the nanotube. However, the tips may have very sharp edges
Graphite was used as substrate for the deposition of carbon vapor. Prior to the tube and cone studies, this substrate was studied by us carefully by STM because it may exhibit anomalous behavior with unusual periodic surface structures[9,10]. In particular, the cluster-substrate interaction was investigated[l 11. At low submonolayer coverages, small clusters and islands are observed. These tend to have linear structures[l2]. Much higher coverages are required for the synthesis of nanotubes and nanocones. In addition, the carbon vapor has to be very hot, typically >3O0O0C. We note that the production of nanotubes by arc discharge occurs also at an intense heat (of the plasma in the arc) of >30OO0C. The graphite (grade-A HOPG) was freshly cleaved in UHV and carefully examined by STM before the deposition. The HOPC surface was determined to be atomically flat and defect-free over micrometer dimensions. Any defect or adatom would have easily been detected. The graphite was cooled to -30°C during evaporation. The carbon vapor was produced by resistively heating a 99.99% purity carbon foil (0.5 mrri thick) in UHV (base pressure 2 x lo-’ Torr). The deposition rate of 0.5 A/s was controlled by a quartz crystal film thickness monitor. After deposition, the 65
zyxwvutsrqpo zyxwvu zyxwvu K. SATTLER
samples were transferred to a STM operated at 2 x lo-'' Torr, without breaking vacuum. Our evaporation and condensation process leads to the formation of various nanostructures, with 70% nanotubes on the average, of the overall products. In some areas, which may be as large as one square micron, we find 100% nanotubes. The yield for single-wall tubes varied from experiment to experiment from a few percent to 8090%. Bundles of multiwall tubes were found in some areas, but were usually less abundant than isolated tubes. Individual nanocones were observed together with tubes, but were quite seldom. The microscope was operated in the constant current and in the constant height mode. Atomic resolution images were recorded in the constant current mode, in which the tip-tosample distance is kept constant by means of an electronic feedback control. Bias voltages of 100 to 800 mV (both positive and negative) and tunneling currents of 0.5 to 3.0 nA were applied. A mechanically shaped Pt/lr tip was used. We did not observe any voltage dependent variation of the tube images. Also, the measured heights of the tubes were comparable with their diameters. Both of these observations indicate that the tubes have rather metallic than semiconducting properties. The tubes were stable over long periods of time. After several months of being stored in UHV we still observed the same features as shortly after their preparation. Some of the samples were transferred to an STM operated in air. Again, we observed similar structures as seen in UHV. This shows the high stability of the tubes. It appears that the vapor-phase growth technique produces defect-free tubes, with dangling bonds at the tube edges often being saturated by cap terminations.
being equally distributed. We note that most of the nanotubes that we analyzed showed hemispherical terminations. Therefore, we might assume that the tubes start to grow from an incomplete fullerene cap and that the C,, hemisphere is the nucleation seed for the growth of the 10 A tube. After the C6' hemisphere is formed, growth may continue as an all-hexagon network, forming a tube, rather than continuing as an alternating hexagodpentagon network leading to the C6, sphere. The two caps, on both sides of the 10 A zigzag tube (C60+18j)[17,1S]are identical, with a total number of 12 pentagons, following Euler's theorem. The two caps for the 10 A armchair tube (C60+10j) are 36" rotated relative to each other. It is interesting that we find the zigzag configuration for the tube network. The zigzag tube (Fig. 2) is the only nonhelical one among all the possible tube configurations. A cut normal to the C60+18j tube axis leaves 18 dangling bonds, compared to 10 dangling tube. For the armchair tube, it bonds for the C60+10j may be easy to incorporate pentagonal defects leading to an early closure because only one additional atom is required to form a pentagon at the growth periphery. For the zigzag tube, however, two atoms are required to form a pentagon and the structure might rather continue as a hexagonal network. Therefore, the zigzag 10 A single-shell tubes might have a higher probability for growth.
3. SINGLESHELL TUBES
Single-shell tubes are formed from a single layer of graphite. The surface of the cylinders has a honeycomblattice pattern, just as in a two-dimensional graphite plane. From a theoretical point of view they are interesting as the embodiment of a one-dimensional (1-D) periodic structure along the tube axis. In the circumferential direction, periodic boundary conditions apply to the enlarged unit cell. In addition to the chiral structures, there exist two nonchiral configurations, zigzag and armchair [131. Part of a 15-nm long, 10A tube, is given in Fig. 1. Its surface atomic structure is displayedIl41. A periodic lattice is clearly seen. The cross-sectional profile was also taken, showing the atomically resolved curved surface of the tube (inset in Fig. 1). Asymmetry variations in the unit cell and other distortions in the image are attributed to electronic or mechanical tip-surface interactions[l5,16]. From the helical arrangement of the tube, we find that it has zigzag configuration. The zigzag and armchair tubes can be closed by hemispherical C6' caps, with 3-fold and 5-fold symmetry, respectively. Both caps contain six pentagons
4. MULTI-SHELL TUBES
There is an infinite number of possible atomic structures of graphene tubules. Each structure is characterized by its diameter and the helical arrangement of the carbon hexagons. Presumably, only single-shell tubes with small diameters of about 10 A are formed and tubes with larger diameters are multishell tubes. We produced multilayer tubes with diameters between 20 A and 70 A and up to 2000 A in length. An STM image of such tubes is shown in Fig. 3. The cylindrical shapes are well displayed. We observed in some cases coaxial arrangement of the outermost and an inner tube. The outer tube may be terminated and the adjacent inner one is imaged simultaneously. We measure an interlayer spacing of 3.4 A,which is about the graphite interlayer distance (3.35 A). We find that the tubes are placed almost horizontally on the substrate. Irregular nanostructures were also formed, as displayed in the images. However, the high occurrence of tubes clearly shows that carbon prefers to condense to tubular structures, as opposed to other nanostructures, under our preparation conditions. In Fig. 4 we show an atomic resolution image of a carbon tube. The structure imaged at the upper right corner of the picture comes from another tube. Both of them were -1000 A long. A perfect honeycomb surface structure is observed. By taking into account the curvature of the tube surface and the STM imaging profile, we find the same lattice parameter as that of .graphite (1.42 A). This directly proves that the tubu-
STM of carbon nanotubes and nanocones
Fig. 1. Atomic resolution STM image of a 10 A nanotube of carbon with cross-sectional plot.
lar surface is a graphitic network. The honeycomb surface net is arranged in a helical way, with a chiral angle of 5.0 f 0.5". In a common method for the production of tubular carbon fibers, the growth is initiated by submicrometer size catalytic metal particles[ 191. Tube growth out of a graphite rod during arc-discharge might also be related to nanoparticle-like seeds present
at the substrate. In vapor-phase growth without a catalyst, the tubes may grow out of a hollow fullerene cap instead of a compact spherical particle. This view is supported by our observation of hemispherically capped single-wall and multi-wall tubes on the same samples. It suggests that the C,,-derived tube could be the core of possible multilayer concentric graphitic tubes. After the single-shelltube has been
Fig. 2. Model of the Cm-based 10 A tube with zigzag configuration (C,,+,,j).
K . SATTLER
zyxwvutsrqponm zyxwvutsrq zyxwvutsrq 2.00
Fig. 3. STM images of fullerene tubes on a graphite substrate.
formed, further concentric shells can be added by graphitic cylindrical layer growth. The c60+10i (j = 1,2,3, . . . ) tube has an outer diameter of 9.6 A. In its armchair configuration, the hexagonal rings are arranged in a helical fashion with a chiral angle of 30 degrees. In this case, the tube axis is the five-fold symmetric axis of the C60-cap. The single-shell tube can be treated as a rolled-up graphite sheet that matches perfectly at the closure line. Choosing the cylinder joint in different directions leads to different helicities. One single helicity gives a set of discrete diameters. To obtain the diameter that matches exactly the required interlayer spacing, the tube layers need to adjust their helicities. Therefore, in general, different helicities for different layers in a multilayer tube are expected. In fact, this is confirmed by our experiment. In Fig. 4 we observe, in addition to the atomic lattice, a zigzag superpattern along the axis at the surface of the tube. The zigzag angle is 120" and the period is about 16 A. Such superstructure (giant lattice) was found earlier for plane graphite[lO]. It is a Moire electron state density lattice produced by different helicities of top shell and second shell of a tube. The measured period of 16 A reveals that the second layer of the tube is rotated relative to the first layer by 9". The first and the second cylindrical layers, therefore, have chiral angles of 5" and -4", respectively. This proves that the tubes are, indeed, composed of at least two coaxial graphitic cylinders with different helicities.
Fig. 4. Atomic resolution STM image of a carbon tube, 35 A in diameter. In addition to the atomic structure, a zigzag superpattern along the tube axis can be seen.
fect graphitic cylinders. The bundle is disturbed in a small region in the upper left part of the image. In the closer view in Fig. 6, we recognize six tubes at the bundle surface. The outer shell of each tube is broken, and an inner tube is exposed. We measure again an intertube spacing of -3.4 A.This shows that the exposed inner tube is the adjacent concentric graphene shell. The fact that all the outer shells of the tubes in the bundles are broken suggests that the tubes are strongly coupled through the outer shells. The inner tubes, however, were not disturbed, which indicates that the
zyxwvuts 5. BUNDLES
In some regions of the samples the tubes are found to be closely packed in bundles. Fig. 5 shows a -200 A broad bundle of tubes. Its total length is 2000 A,as determined from a larger scale image. The diameters of the individual tubes range from 20-40 A. They are perfectly aligned and closely packed over the whole length of the bundle. Our atomic-resolution studies[ 101 did not reveal any steps or edges, which shows that the tubes are per-
Fig. 5. STM image of a long bundle of carbon nanotubes. The bundle is partially broken in a small area in the upper left part of the image. Single tubes on the flat graphite surface are also displayed.
STM of carbon nanotubes and nanocones
zyxwvutsrqpo zyxwvutsrqpo zyxwvutsrqp
Fig. 6 . A closer view of the disturbed area of the bundle in Fig. 5 ; the concentric nature of the tubes is shown. The outermost tubes are broken and the adjacent inner tubes are complete.
intertube interaction is weaker than the intratube interaction. This might be the reason for bundle formation in the vapor phase. After a certain diameter is reached for a single tube, growth of adjacent tubes might be energetically favorable over the addition of further concentric graphene shells, leading to the generation of bundles. 6 . CONES
Fig. 7 . A (244 A) STM image of two fullerene cones.
is a hexagon network, while the apex contains five pentagons. The 19.2" cone has mirror symmetry through a plane which bisects the 'armchair' and 'zigzag' hexagon rows. It is interesting that both carbon tubules and cones have graphene networks. A honeycomb lattice without inclusion of pentagons forms both structures. However, their surface nets are configured differently. The graphitic tubule is characterized by its diameter and its helicity, and the graphitic cone is entirely characterized by its cone angle. Helicity is not defined for the graphitic cone. The hexagon rows are rather arranged in helical-like fashion locally. Such 'local helicity' varies monotonously along the axis direction of the cone, as the curvature gradually changes. One can
Nanocones of carbon are found in some areas on the substrate together with tubes and other mesoscopic structures. In Fig. 7 two carbon cones are displayed. For both cones we measure opening angles of 19.0 f 0.5". The cones are 240 and 130 A long. Strikingly, all the observed cones (as many as 10 in a (800 A)2 area) have nearly identical cone angles - 19". At the cone bases, flat or rounded terminations were found. The large cone in Fig. 7 shows a sharp edge at the base, which suggests that it is open. The small cone in this image appears closed by a sphericalshaped cap. We can model a cone by rolling a sector of a sheet around its apex and joining the two open sides. If the sheet is periodically textured, matching the structure at the closure line is required to form a complete network, leading to a set of discrete opening angles. The higher the symmetry of the network, the larger the set. In the case of a honeycomb structure, the sectors with angles of n x (2p/6) (n = 1,2,3,4,5) can satisfy perfect matching. Each cone angle is determined by the corresponding sector. The possible cone angles are 19.2", 38.9", 60", 86.6", and 123.6", as illustrated in Fig. 8. Only the 19.2" angle was observed for all the cones in our experiment. A ball-and-stick model of the 19.2" fullerene cone is shown in Fig. 9. The body part
zyxwvuts Fig. 8. The five possible graphitic cones, with cone angles of 19.2", 38.9", 60", 86.6", and 123.6".
zyxwv zyxwvutsrqpo zyxwvuts K . SATTLER
shapes) to match their corresponding cones and are unlikely to form. This explains why only the 19.2" cones have been observed in our experiment. Carbon cones are peculiar mesoscopic objects. They are characterized by a continuous transition from fullerene to graphite through a tubular-like intermedium. The dimensionality changes gradually as the cone opens. It resembles a 0-D cluster at the apex, then proceeds to a 1-D 'pipe' and finally approaches a 2-D layer. The cabon cones may have complex band structures and fascinating charge transport properties, from insulating at the apex to metallic at the base. They might be used as building units in future nanoscale electronics devices.
Fig. 9. Ball-and-stick model for a 19.2" fullerene cone. The back part of the cone is identical to the front part displayed in the figure, due to the mirror symmetry. The network is in 'armchair' and 'zigzag' configurations, at the upper and lower sides, respectively. The apex of the cone is a fullerene-type cap containing five pentagons.
easily show that moving a 'pitch' (the distance between two equivalent sites in the network) along any closure line of the network leads to another identical cone. For the 19.2"cone, a hexagon row changes its 'local helical' direction at half a turn around the cone axis and comes back after a full turn, due to its mirror symmetry in respect to its axis. The other four cones, with larger opening angles, have Dnd(n = 2,3,4,5) symmetry along the axis. The 'local helicity' changes its direction at each of their symmetry planes. As fullerenes, tubes, and cones are produced in the vapor phase we consider all three structures being originated by a similar-type nucleation seed, a small curved carbon sheet composed .of hexagons and pentagons. The number of pentagons (m) in this fullerenetype (m-P) seed determines its shape. Continuing growth of an alternating pentagodhexagon (516) network leads to the formation of C60(and higher fullerenes). If however, after the Cb0 hemisphere is completed, growth continues rather as a graphitic ( 6 / 6 ) network, a tubule is formed. If graphitic growth progresses from seeds containing one to five pentagons, fullerene cones can be formed. The shape of the 5-P seed is closest to spherical among the five possible seeds. Also, its opening angle matches well with the 19.2"graphitic cone. Therefore, continuing growth of a graphitic network can proceed from the 5-P seed, without considerable strain in the transition region. The 2-P, 3-P, and 4-P seeds would induce higher strain (due to their nonspherical
Acknowledgements-Financial support from the National Science Foundation, Grant No. DMR-9106374,is gratefully acknowledged.
REFERENCES 1 . S. Iijima, Nature 354, 56 (1991). T. W. Ebbesen and P. M. Ajayan, Nature 358, 220 (1992). 2. D. Ugarte, Nature 359, 707 (1992). 3. M. Ge and K. Sattler, Chem. Phys. Lett. 220, 192 (1994). 4. M. Ge and K. Sattler, Science 260, 515 (1993). 5. T. W. Ebbesen, H. Hiura, J. Fijita, Y. Ochiai, S. Matsui, and K. Tanigaki, Chem. Phys. Lett. 209,83 (1993). 6. M. J. Gallagher, D. Chen, B. P. Jakobsen, D. Sand, L. D. Lamb, E A. Tinker, J. Jiao, D. R. Huffman, S. Seraphin, and D. Zhou, Surf. Sci. Lett. 281, L335 (1993). 7. Z. Zhang and Ch. M. Lieber, Appl. Phys. Lett. 62,2792 (1993). 8. R. Hoeper, R. K. Workman, D. Chen, D. Sarid, T. Yadav, J. C . Withers, and R. 0. Loutfy, Surf. Sci. 311, L371 (1994). 9. K. Sattler, Znt. J. Mod. Phys. B 6, 3603 (1992). 10. J. Xhie, K. Sattler, N. Venkateswaran, and M. Ge, Phys. Rev. B 47, 15835 (1993). 1 1 . J. Xhie, K. Sattler, U. Mueller, G. Raina, and N. Venkateswaran, Phys. Rev. B 43, 8917 (1991). 12. M . Ge, K. Sattler, J. Xhie, and N. Venkateswaran, In Novel forms of carbon (Edited by C. L. Renschler, J. Pouch, and D. Cox) Mat. Res. SOC.Proc. 270, 109 (1992). 13. R. Saito, M. Fujita, G. Dresselhaus, and M. S. Dresselhaus, Appl. Phys. Lett. 60, 2204 (1992). 14. M. Ge and K. Sattler, Appl. Phys. Lett. 65, 2284 (1994). 15. D. Tomanek, S. G. Louie, H. J. Mamin, D. W. Abraham, R. E. Thomson, E. Ganz, and J. Clarke, Phys. Rev. B 35, 7790 (1987). 16. J. M. Soler, A. M. Baro, N. Garcia, and H. Rohrer, Phys. Rev. Lett. 57, 444 (1986). 17. N. Hamada, S. Samada, and A. Oshiyama, Phys. Rev. Lett. 68, 1579 (1992). 18. M. S. Dresselhaus, G. Dresselhaus, and R. Saito, Phys. Rev. B 45, 6234 (1992). 19. G. Tibbetts, J. Cryst. Growth 66, 632 (1984). 20. M. Ge and K. Sattler, Appl. Phys. Lett. 64, 710 (1994).
zyxwvu zyxwvu zyxwvuts
zyxwvu zyxwvu zyx
TOPOLOGICAL AND SP3 DEFECT STRUCTURES IN NANOTUBES T. W. EBBESEN' and T. TAKADA~
'NEC Research Institute, 4 Independence Way, Princeton, NJ 08540, U.S.A. 2Fundamental Research Laboratories, NEC Corporation, 34 Miyukigaoka, Tsukuba 305, Japan
(Received 25 November 1994; accepted 10 February 1995)
Abstract-Evidence is accumulating that carbon nanotubes are rarely as perfect as they were once thought to be. Possible defect structures can be classified into three groups: topological, rehybridization, and incomplete bonding defects. The presence and significance of these defects in carbon nanotubes are discussed. It is clear that some nanotube properties, such as their conductivity and band gap, will be strongly affected by such defects and that the interpretation of experimental data must be done with great caution.
Key Words-Defects, topology, nanotubes, rehybridization.
2. CLASSES OF DEFECTS
Figure 1 show examples of nanotubes that are far from perfect upon close inspection. They reveal some of the types of defects that can occur, and will be discussed below. Having defined a perfect nanotube as a cylindrical sheet of graphene with the minimum number of pentagons at each tip to form a seamless structure, we can classify the defects into three groups: 1) topological defects, 2) rehybridization defects and 3) incomplete bonding and other defects. Some defects will belong to more than one of these groups, as will be indicated.
Carbon nanotubes were first thought of as perfect seamless cylindrical graphene sheets -a defect-free structure. However, with time and as more studies have been undertaken, it is clear that nanotubes are not necessarily that perfect; this issue is not simple because of a variety of seemingly contradictory observations. The issue is further complicated by the fact that the quality of a nanotube sample depends very much on the type of machine used to prepare it[l]. Although nanotubes have been available in large quantities since 1992, it is only recently that a purification method was found. So, it is now possible to undertakevarious accurate property measurements of nanotubes. However, for those measurements to be meaningful, the presence and role of defects must be clearly understood. The question which then arises is: What do we call a defect in a nanotube? To answer this question, we need to define what would be a perfect nanotube. Nanotubes are microcrystals whose properties are mainly defined by the hexagonal network that forms the central cylindrical part of the tube. After all, with an aspect rat.io (length over diameter) of 100 to 1000, the tip structure will be a small perturbation except near the ends. This is clear from Raman studies and is also the basis for calculations on nanotube properties[5-71. So, a perfect nanotube would be a cylindrical graphene sheet composed only of hexagons having a minimum of defects at the tips to form a closed seamless structure. Needless to say, the issue of defects in nanotubes is strongly related to the issue of defects in graphene. Akhough earlier studies of graphite help us understand nanotubes, the concepts derived from fullerenes has given us a new insight into traditional carbon materials. So, the discussion that follows, although aimed at nanotubes, is relevant to all graphitic materials. First, different types of possible defects are described. Then, recent evidences for defects in nanotubes and their implications are discussed.
2.1 Topological defects
The introduction of ring sizes other than hexagons, such as pentagons and heptagons, in the graphene sheet creates topological changes that can be treated as local defects. Examples of the effect of pentagons and heptagons on the nanotube structure is shown in Fig. 1 (a). The resulting three dimensional topology follows Euler's theorem in the approximation that we assume that all the individual rings in the sheet are flat. In other words, it is assumed that all the atoms of a given cycle form a plane, although there might be angles between the planes formed in each cycle. In reality, the strain induced by the three-dimensional geometry on the graphitic sheet can lead to deformation of the rings, complicating the ideal picture, as we shall see below. From Euler's theorem, one can derive the following simple relation between the number and type of cycles nj (where the subscript i stands for the number of sides to the ring) necessary to close the hexagonal network of a graphene sheet:
3n, + 2n,
+ n5 - n7 - 2n8 - 372, = 12
where 12 corresponds to a total disclination of 4n (i.e., a sphere). For example, in the absence of other cycles one needs 12 pentagons (ns)in the hexagonal net71
zyxwvutsrqponm zyxwvut T. W. EBBESEN and T. TAKADA
Fig. 1. Five examples of nanotubes showing evidence of defects in their structure (p: pentagon, h: heptagon, d: dislocation); see text (the scale bars equal 10 nm).
work to close the structure. The addition of one heptagon (n7)to the nanotube will require the presence of 13 pentagons to close the structure (and so forth) because they induce opposite 60" disclinations in the surface. Although the presence of pentagons (ns)and heptagons (n,) in nanotubes[9,10] is clear from the disclinations observed in their structures (Fig. la), we are not aware of any evidence for larger or smaller cycles (probably because the strain would be too great). A single heptagon or pentagon can be thought of as point defects and their properties have been calculated[l I]. Typical nanotubes don't have large numbers of these defects, except close to the tips. However, the point defects polygonize the tip of the nanotubes, as shown in Fig. 2. This might also favor the polygonalization of the entire length of the nanotube as illustrated by the dotted lines in Fig. 2. Liu and Cowley have shown that a large fraction of nanotubes are polygonized in the core[12,131. This will undoubtedly have significant effects on their properties due to local rehybridization, as will be discussed in the next section. The nanotube in Fig. 1 (e) appears to be polygonized
(notice the different spacing between the layers on the left and right-hand side of the nanotube). Another common defect appears to be the aniline structure that is formed by attaching a pentagon and a heptagon to each other. Their presence is hard to detect directly because they create only a small local deformation in the width of the nanotube. However, from time to time, when a very large number of them are accidentally aligned, the nanotube becomes gradually thicker and thicker, as shown in Fig. 1 (b). The existence of such tubes indicates that such pairs are probably much more common in nanotubes, but that they normally go undetected because they cancel each other out (random alignment). The frequency of occurrence of these aligned 5/7 pairs can be estimated to be about 1 per 3 nm from the change in the diameter of the tube. Randomly aligned 5/7 pairs should be present at even higher frequencies, seriously affecting the nanotube properties. Various aspects of such pairs have been discussed from a theoretical point of view in the literature[l4,15]. In particular, it has been pointed out by Saito et a1. that such defect pairs
Topological and sp3 defect structures in nanotubes
Fig. 1 continued.
can annihilate, which would be relevant to the annealing away of such defects at high temperature as discussed in the next section. It is not possible to exclude the presence of other unusual ring defects, such as those observed in graphitic sheets[16,171. For example, there might be heptagontriangle pairs in which there is one sp3 carbon atom bonded to 4 neighboring atoms, as shown in Fig. 3. Although there must be strong local structural distortions, the graphene sheet remains flat overa11[16,17]. This is a case where Euler’s theorem does not apply. The possibility of sp3 carbons in the graphene sheet brings us to the subject of rehybridization.
2.2 Rehybridization defects
ter or, to put it more accurately, it will have s p Z f L V character. The size of CY will depend on the degree of curvature of the bend. The complete folding of the graphene sheet will result in the formation of a defect line having strong sp3 character in the fold. We have shown elsewhere that line defects having sp3 character form preferentially along the symmetry axes of the graphite sheet[lb]. This is best understood by remembering that the change from sp2 to sp3 must naturally involve a pair of carbon atoms because a double bond is perturbed. In the hexagonal network of graphite shown in Fig. 4, it can be seen that there are 4 different pairs of carbon atoms along which the sp3 type line defect can form. Two pairs each are found along the [loo] and  symmetry axes. Furthermore, there are 2 possible conformations, “boat” and “chair,” for three of these distinct line defects and a single conformation of one of them. These are illustrated in Fig. 5 . In the polygonized nanotubes observed by Liu and Cowley[12,13], the edges of the polygon must have more sp3 character than the flat faces in between. These are defect lines in the sp2 network. Nanotubes mechanically deformed appear to be rippled, indicat-
The root of the versatility of carbon is its ability to rehybridize between sp, s p 2 , and sp3. While diamond and graphite are examples of pure sp3 and sp2 hybridized states of carbon, it must not be forgotten that many intermediate degrees of hybridization are possible. This allows for the out-of-plane flexibility of graphene, in contrast to its extreme in-plane rigidity. As the graphene sheet is bent out-of-plane, it must lose some of its sp2 character and gain some sp3 charac-
zyxwvutsrqpo T. W. EBBESEN and T. TAKADA
,/ / /
Fig. 2. Nanotube tip structure seen from the top; the presence of pentagons can clearly polygonize the tip.
2.3 Incomplete bonding and other defects Defects traditionally associated with graphite might also be present in nanotubes, although there is not yet much evidence for their presence. For instance, point defects such as vacancies in the graphene sheet might be present in the nanotubes. Dislocations are occasionally observed, as can be seen in Fig. 1 (c) and (d), but they appear to be quite rare for the nanotubes formed at the high temperatures of the carbon arc. It might be quite different for catalytically grown nanotubes. In general, edges of graphitic domains and vacancies should be chemically very reactive as will be discussed below. 3. DISCUSSION
There are now clear experimental indications that nanotubes are not perfect in the sense defined in the introduction[l2,13,19,20].The first full paper dedicated to this issue was by Zhou et al., where both pressure and intercalation experiments indicated that the particles in the sample (including nanotubes) could not be perfectly closed graphitic structures. It was pro-
zyxwvuts zyxwvuts I
Fig. 1 continued.
ing the presence of ridges with sp3 character[l8]. Because the symmetry axes of graphene and the long axis of the nanotubes are not always aligned, any defect line will be discontinuous on the atomic scale as it traverses the entire length of the tube. Furthermore, in the multi-layered nanotubes, where each shell has a different helicity, the discontinuity will not be superimposable. In other words, in view of the turbostratic nature of the multi-shelled nanotubes, an edge along the tube will result in slightly different defect lines in each shell.
zyxwvutsrq Fig. 3. Schematic diagram of heptagon-triangle defects [ 16,171.
Topological and sp3 defect structures in nanotubes
inwards, layer by layer[21,22]. If there were smaller domains along the cylindrical part, their edges would be expected to react very fast to oxidation, contrary to observation. Second, ESR studies do not reveal any strong signal from dangling bonds and other defects, which would be expected from the numerous edges in the paper-machk model. To try to clarify this issue, we recently analyzed crude nanotube samples and purified nanotubes before and after annealing them at high temperature. It is well known that defects can be annealed away at high temperatures (ca. 285OOC). The annealing effect was very significant on the ESR properties, indicating clearly the presence of defects in the nanotubes. However, our nanotubes do not fit the defect structure proposed in the paper-machi model for the reason discussed in the previous paragraph. Considering the types of possible defects (see part 2), the presence of either a large number of pentagon/heptagon pairs in the nanotubes and/or polygonal nanotubes, as observed by Liu and Cowley[12,13], could possibly account for these results. Both the 5/7 pairs and the edges of the polygon would significantly perturb the electronic properties of the nanotubes and could be annealed away at very high temperatures. The sensitivity of these defects to oxidation is unknown. In attempting to reconcile these results with those of other studies, one is limited by the variation in sample quality from one study to another. For instance, IESR measurements undertaken on bulk samples in three different laboratories shoq7 very different results[19,23,24]. As we have pointed out elsewhere, the quantity of nanotubes (and their quality) varies from a few percent to over 60% of the crude samples, depending on the current control and the extent of cooling in the carbon arc apparatus[l]. The type and distribution of defects might also be strongly affected by the conditions during nanotube production. The effect of pressure on the spacing between the graphene sheets observed by Zhou et al. argues most strongly in favor of the particles in the sample having a nonclosed structure[l9]. Harris et af. actually observe that nanoparticles in these samples sometimes do not form closed structures. It would be interesting to repeat the pressure study on purified nanotubes before and after annealing with samples of various origins. This should give significant information on the nature of the defects. The results taken before annealing will, no doubt, vary depending on where and how the sample was prepared. The results after sufficient annealing should be consistent and independent of sample origin.
Fig. 4. Hexagonal network of graphite and the 4 different pairs of carbon atoms across which the sp3-likedefect line
posed that nanotubes were composed of pieces of graphitic sheets stuck together in a paper-machi model. The problem with this model is that it is not consistent with two other observations. First, when nanotubes are oxidized they are consumed from the tip
Fig. 5 . Conformations of the 4 types of defect lines that can occur in the graphene sheet[l8].
The issue of defects in nanotubes is very important in interpreting the observed properties of nanotubes. For instance, electronic and magnetic properties will be significantly altered as is already clear from observation of the conduction electron spin resonance[20,23].
T. W. EBBESEN and T. TAKADA
It would be worthwhile making- theoretical calculations to evaluate the effect of defects on the nanotube properties. The chemistry might be affected, although to a lesser degree because nanotubes, like graphite, are chemically quite inert. If at all possible, nanotubes should be annealed (if not also purified) before physical measurements are made. Only then are the results likely to be consistent and unambiguous. REFERENCES 1. T. W. Ebbesen, Annu. Rev. Mater. Sci. 24, 235 (1994). 2. T. W. Ebbesen and P. M. Ajayan, Nature 358, 220 (1992). 3. T. W. Ebbesen, P. M. Ajayan, H . Hiura, and K. Tanigaki, Nature 367, 519 (1994). 4. H. Hiura, T. W. Ebbesen, K. Tanigaki, and H. Takahashi, Chem. Phys. Lett. 202, 509 (1993). 5. J. W. Mintmire, B. I. Dunlap, and C. T. White, Phys. Rev. Lett. 68, 631 (1992). 6. N. Hamada, S. Sawada, and A. Oshiyama, Phys. Rev. Lett. 68, 1579 (1992). 7. R. Saito, M. Fujita, G. Dresselhaus, and M. S. Dresselhaus, Appl. Phys. Lett. 60, 2204 (1992). 8. H. Terrones and A. L. Mackay, Carbon 30, 1251 (1992). 9. P. M. Ajayan, T. Ichihashi, and S. Iijima, Chem. Phys. Lett. 202, 384 (1993). IO. S. Iijima, T. Ichihashi, and Y. Ando, Nature 356, 776 (1992).
zyxw zyx zyx zy
11. R. Tamura and M. Tsukada.. Phvs. - Rev. B 49. 7697 (1994). 12. M. Liu and J. M. Cowley, Carbon 32, 393 (1994). 13. M. Liu and J. M. Cowley, Ultramicroscopy 53, 333 (1994). 14. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, Chem. Phys. Lett. 195, 537 (1992). 15. C. J. Brabec, A. Maiti, and J. Bernholc, Chem. Phys. Lett. 219, 473 (1994). 16. J. C. Roux, S. Flandrois, C. Daulan, H. Saadaoui, and 0. Gonzalez, Ann. Chim. Fr. 17, 251 (1992). 17. B. Nysten, J. C. Roux, S. Flandrois, C. Daulan, and H . Saadaoui, Phys. Rev. B 48, 12527 (1993). 18. H. Hiura, T. W. Ebbesen, J. Fujita, K. Tanigaki, and 7 . Takada, Nature 367, 148 (1994). 19. 0. Zhou, R. M. Fleming, D. W. Murphy, C. H . Chen, R. C. Haddon, A. P. Ramirez, and S. H. Glarum, Science 263, 1744 (1994). 20. M. Kosaka, T. W. Ebbesen, H. Hiura, and K. Tanigaki, Chem. Phys. Lett. 233, 47 (1995). 21. S. C. Tsang, P. J. F. Harris, and M. L. H. Green, Nature 362, 520 (1993). 22. P. M. Ajayan, T. W. Ebbesen, T. Ichihashi, S. Iijima, K. Tanigaki, and H. Hiura, Nature 362, 522 (1993). 23. M. Kosaka, T. W. Ebbesen, H. Hiura, and K. Tanigaki, Chem. Phys. Lett. 225, 161 (1994). 24. K. Tanaka, T. Sato, T. Yamabe, K. Okahara, et ai., Chem. Phys. Lett. 223, 65 (1994). 25. P. J. F. Harris, M. L. H. Green, and S. C. Tsang, J. Chem. SOC.Faraday Trans. 89, 1189 (1993).
zyxw zyxw zyxw zyxwv
HELICALLY COILED AND TOROIDAL CAGE FORMS OF GRAPHITIC CARBON SIGEOIHARA and SATOSHI ITOH
Central Research Laboratory, Hitachi Ltd., Kokubunji, Tokyo 185, Japan (Received 22 August 1994; accepted in revised form 10 February 1995)
Abstract-Toroidal forms for graphitic carbon are classified into five possible prototypes by the ratios of their inner and outer diameters, and the height of the torus. Present status of research of helical and toroidal forms, which contain pentagons, hexagons, and heptagons of carbon atoms, are reviewed. By molecular-dynamics simulations, we studied the length and width dependence of the stability of the elongated toroidal structures derived from torus C240and discuss their relation to nanotubes. The atomic arrangements of the structures of the helically coiled forms of the carbon cage for the single layer, which are found to be thermodynamically stable, are compared to those of the experimental helically coiled forms of single- and multi-layered graphitic forms that have recently been experimentally observed.
molecular dynamics, torus, helix, graphitic forms.
The toroidal and helical forms that we consider here are created as such examples; these forms have quite interesting geometrical properties that may lead to interesting electrical and magnetic properties, as well as nonlinear optical properties. Although the method of the simulations through which we evaluate the reality of the structure we have imagined is omitted, the construction of toroidal forms and their properties, especially their thermodynamic stability, are discussed in detail. Recent experimental results on toroidal and helically coiled forms are compared with theoretical predictions.
Due, in part, to the geometrical uniqueness of their cage structure and, in part, to their potentially technological use in various fields, fullerenes have been the focus of very intense research[l]. Recently, higher numbers of fullerenes with spherical forms have been available. It is generally recognized that in the fullerene, C60, which consists of pentagons and hexagons formed by carbon atoms, pentagons play an essential role in creating the convex plane. This fact was used in the architecture of the geodesic dome invented by Robert Buckminster Fuller, and in traditional bamboo art (‘toke-zaiku’,# for example). By wrapping a cylinder with a sheet of graphite, we can obtain a carbon nanotube, as experimentally observed by Iijima[S]. Tight binding calculations indicate that if the wrapping is charged (i.e., the chirality of the surface changes), the electrical conductivity changes: the material can behave as a semiconductor or metal depending on tube diameter and chirality. In the study of the growth of the tubes, Iijima found that heptagons, seven-fold rings of carbon atoms, appear in the negatively curved surface. Theoretically, it is possible to construct a crystal with only a negatively curved surface, which is called a minimal surface. However, such surfaces of carbon atoms are yet to be synthesized. The positively curved surface is created by insertion of pentagons into a hexagonal sheet, and a negatively curved surface is created by heptagons. Combining these surfaces, one could, in principle, put forward a new form of carbon, having new features of considerable technological interest by solving the problem of tiling the surface with pentagons, heptagons, and hexagons.
zyxwvutsrq 2. TOPOLOGY OF TOROIDAL AND HELICAL FORMS
2.1 Tiling rule for cage structure
of graphitic carbon Because of the sp2 bonding nature of carbon atoms, the atoms on a graphite sheet should be connected by the three bonds. Therefore, we consider how to tile the hexagons created by carbon atoms on the toroidal surfaces. Of the various bonding lengths that can be taken by carbon atoms, we can tile the toroidal surface using only hexagons. Such examples are provided by Heilbonner and Miyazakif91.However, the side lengths of the hexagons vary substantially. If we restrict the side length to be almost constant as in graphite, we must introduce, at least, pentagons and heptagons. Assuming that the surface consists of pentagons, hexagons, and heptagons, we apply Euler’s theorem. Because the number of hexagons is eliminated by a kind of cancellation, the relation thus obtained contains only the number of pentagons and heptagons: fs- f, = 12(1-g), where fsstands for the number of pentagons, f, the number of heptagons, and g is the genius (the number of topological holes) of the surface.
#At the Ooishi shrine of Ako in Japan, a geodesic dome made of bamboo with three golden balls, which was the symbol called “Umajirushi” used by a general named Mori Misaemon’nojyo Yoshinari at the battle of Okehazama in 1560, has been kept in custody. (See ref. 141). 77
zyxwvuts zyxwvut zyxwvu zyxwvu zyxwvu zyxw zyxwvutsrq S. IHARA and S. ITOH
In the spherical forms (Le., g = 0), fs=f7 12. In C60,for example, there are no heptagons (f,= 0), so that fs = 12. If the torus whose genius ( 8 ) is one, fs=f7. As we mentioned in the introduction, pentagons and heptagons provide Gaussian positive and negative curvatures, respectively. Therefore, pentagons should be located at the outermost region of the torus and heptagons at the innermost.
2.2 Classifications of tori
Fig. 2. Optimized toroidal structures of Dunlap’s tori: (a) torus C540and (b) torus C576;pentagons and heptagons are shaded.
Here, the topological nature of the tori will be discussed briefly. Figure 1 shows the five possible prototypes of toroidal forms that are considered to be related to fullerenes. These structures are classified by created by the torus in our case, the properties of the the ratios of the inner and outer diameters rj and r, , helix strongly depend on the types of the torus. and the height of the torus, h. (Note that r, is larger than Ti). As depicted in Fig. 1, if ri = r,, and h and the magnetic field (-tesla) is a small perturbation on the particle motion, the magneric susceptibility would be due to small quantum corrections to the energy of the system. For this quasiclassical case., the quantizing action of the geometry is not important; the response of the system to the perturbation may be considered as a sum over small plaquettes of the size I , . (This additivity is hidden by the effect of a non-gauge-invariant formalism; nevertheless, it is a general physical property, and the inelastic mean free path is the correlation radius of a local magnetization.) Therefore, at high temperatures a buckytube with R > I, may be considered as a rolied-up graphitic sheet (or concentric tubes). We use this model to calculate the susceptibility, for the field perpendicular to the buckybundle axis. We write the susceptibility tensor of single crystal graphite as
The above discussion ignores all paramagnetic effects including band paramagnetism. Evidence for a Curie-like contribution is seen at low temperatures in some of the curves displayed in Fig. 5 and could arise, in part, from paramagnetic impurities (see below). The anisotropic susceptibility of buckytubes is governed by various geometrical and structural factors (such as the aspect ratio and degree of perfection of its structure). In the direction perpendicular to the buckybundle axis, we d o not expect xi to be larger than 0.5 x.: However, in the direction parallel to the buckybundle axis x: might be much larger for a highquality sample of buckytubes, as discussed above. The measured anisotropy factor in this work (approximately 1.1 at room temperature and increasing with falling temperature) likely represents a value smaller than that achievable with a highly ordered structure. The small value may be caused by imperfectly aligned buckytubes in the buckybundle. The magnetic susceptibility data for buckytubes, amorphous graphite, crystalline graphite, the grayshell material, and C,, as a function of temperatures are shown in Fig. 5. Paramagnetic upturns were observed (for all of the curves) at temperatures lower than 10 K. Amorphous graphite and C,, show no observable temperature dependence at temperatures ranging from 10 K to 300 K, whereas the buckytube sample exhibits a large increase in diamagnetic susceptibility with falling temperature. A plot of xpl vs T for C6, was used to estimate a Curie constant of 8.6 x lO-’/mole, which corresponds to 1.7 x lo-* electron spins per carbon atom in C,,. It is possible that the paramagnetic upturn is caused by a small amount of 0, within the sample. To examine this point, we sealed a Cs0 sample under a vacuum of 2 x lo-’ Torr in a chamber located at
zyxwvu zyxw zyxw xk,
To obtain the magnetic susceptibility of a buckytube for the magnetic field perpendicular to the buckybundle axis, we have to average the magnetic energy E = 0.5 xjJH, Hj over the cylindrical geometry of the buckytube (over a plane containing the a and c axes):
dE = 0 . 5 [ ~H&2 cos2 a or E = O.5H2[x&cos2 a
+ (6H 2 sin2 a ]da
+ x& sin2 a ]d a
x& = 41x&, this argument
zyxwvu Temperature (K)
This is consistent with our experimental results, which strongly Suggest the existence of delocalized Discussion of (L can be found in reference.
Fig. 5 . Temperature dependence of the magnetic susceptibilities measured in a magnetic field of 2 T: (a) C,, powder, (b) polycrystalline graphite anode, (c) gray-shell material, (d) buckybundle: axis perpendicular to H , and (e) buckybundle: axis parallel to H .
zyxwvut zyxwvu zyxwvutsrqp zyxwvu zyxwvutsr zyxwvu X. K. WANCet al.
the center of a quartz tube (holder). No susceptibility difference between the c60 sealed in vacuum and unsealed samples was observed. Cm is a large bandgap (1.4 eV) semiconductor[29,37], and the paramagnetic upturn at very low temperature is probably due to a very small concentration of foreign paramagnetic impurities. We conclude this section stating that buckytubes in a bundle have a large diamagnetic susceptibility for H both parallel to and perpendicular to the buckybundle axis. We attribute the large susceptibility of the buckytubes to delocalized electrons in the graphite sheet. The increase in the diamagnetism at low temperature is attributed to an increasing mean free path. C70, which is formed by 12 pentagons and 25 hexagons, exhibits a larger diamagnetic susceptibility than that of c60, which consists of 12 pentagons and 20 hexagons. This suggests that the diamagnetic susceptibility of fullerenes may increase with an increasing fraction of hexagons. The susceptibility of the buckytubes is likely the largest in this family.
3.3 Transport properties Theory predicts that buckytubes can either be metals, semimetals, or semiconductors, depending on diameter and degree of helicacy. The purpose of our study is to give a preliminary answer to this question. A detailed analysis has been published elsewheret391. In this section, we present mainly experimental results. The transverse magnetoresistance data, p/po ( A p = p ( B ) - p o ) , measured at different temperatures, are shown in Fig. 6. It is seen that, at low temperatures,
the MR is negative at low fields followed by an upturn at another characteristic field that depends on temperature. Our low-temperature MR data has two striking features. First, at low temperatures and low fields A p / p o depends logarithmically on temperature and Bright’s model predicts a VTdependence at low fields. Clearly, the data cannot be described by 1D WL theory. Second, from Fig. 6 (b), we see that the characteristic magnetic field at which the MR exhibits an upturn is smaller for lower temperatures. On the contrary, the transverse MR at different temperatures for the pyrocarbon exhibits quite a different behavior: the upturn field decreases with temperature. With increasing temperature, the Ap/po vs B curves shift upward regularly and there is no crossover between the curves measured at different temperatures. All these facts indicate that the buckytubes show 2D WL behavior at low temperatures. It is also seen that above 60 K the MR is positive; it increases with temperature and tends to saturate at a characteristic magnetic field that is smaller at lower temperatures. Based on a simple two-band model, this means that unequal numbers of electrons and holes are present and that the difference in electron and hole concentrations decreases with increasing temperature. The temperature dependence of the conductance (shown by the right scale in Fig. 7) cannot be described by thermal excitation (over an energy gap) or variable range hopping. Instead, above 60 K conductance, u ( T ) ,increases approximately linearly with temperature. The absence of an exponential or a variable range-hopping-type temperature dependence in the conductivity indicates that the system is semimetallic and that the hopping between the tubes within the bundle is not the dominant transport mechanism. From our transport measurements, we can conclude that at low temperatures, the conductivity of the bundle of buckytubes shows two-dimensional weak localization behavior and the MR is negative; above 60 K the MR is positive and increases approximately
. 8 v
E 2 0.80
0 Fig. 6 . The magnetic field dependence of the high- and lowtemperature MR, respectively; the solid lines are calculated. The inset shows a schematic of the contact configuration for the transport measurements.
100 150 200 250 300
T (K) Fig. 7. The Hall coefficient (left scale) and conductance (right scale) vs temperature. R, was determined using the measured sample dimensions without any correction.
Properties of buckytubes and derivatives
zyxwvutsrqp zyxwvu zyxwvu
linearly with temperate, which is mainly due to an increase in the carrier concentration. The results show that the bundle of buckytubes may best be described as a semimetal.
3.4 The use of a stable glow discharge for the synthesis of carbon nanotubes
Although the generation of carbon nanotubes by vapor-phase growth, catalytic growth[43,44], and corona discharge has been reported, to our knowledge carbon nanotubes in macroscopic quantities are produced only by a carbon-arc discharge in a helium gas atmosphere. Unfortunately, carbon nanotubes synthesized by the conventional arc discharge always coexist with carbonaceous nanoparticles, possess undefined morphologies, and have a variety of defects. One of the serious problems associated with this technique is that the conventional arc discharge is a discontinuous, inhomogeneous, and unstable process. An inhomogeneity of the eIectric field distribution or a discontinuity of the current flow may correlate with the incorporation of pentagons and other defects during growth. A natural question is whether the plasma and current flow can be stabilized to grow high-quality buckytubes. Here, we iintroduce the use of a stable glow discharge for synthesis o f carbon nanotubes. It greatly overcomes many of the problems mentioned above and allows the synthesis of high-quality carbon nanotubes. The fullerene generator used in this study is basically the same chamber we employed for the production of buckyballs and buckytubes described earlier. However, a modification was made with incorporating a high-voltage feedthrough and a tungsten wire. The wire acted as an extension of the Tesla coil, with its free end pointing toward the arc region. Two graphite rods, with the same diameter of inches, were employed as electrodes. The two electrodes with wellpolished ends were positioned very close to each other initially. The glow discharge was stimulated by a corona discharge triggered by the Tesla coil rather than by striking the anode against the cathode to generate a conventional arc discharge. After a plasma was generated gently over the smooth ends of two electrodes, the spacing between the electrodes was slowly in-
creased. Under an appropriate dc current at a He gas pressure of 500 Torr, the glow discharge was selfsustained without the necessity of feeding in the graphite anode. In practice, the rate at which the anode was consumed was equal to the growth rate of the deposited rod, thus keeping the electrode spacing and the discharge characteristics constant. The time dependence of the current across the gap for both the arc discharge and the glow discharge were measured during the deposition of buckytubes. The current of the discharge as a function of time was recorded using a Hewlett-Packard 7090A Measurement Plotting System. The resultant spectrum for the glow discharge, shown in Fig. 8 (a), shows no observable current fluctuation, which demonstrates that the glow discharge is a continuous process. However, the resultant plot for the conventional arc discharge, shown in Fig. 8 (b), indicates that the arc current fluctuates with time. An average arc-jump frequency of about 8 Hz was observed. These results unambiguously demonstrate that the conventional arc discharge is a transient process. Photographs of the cross-section o f two deposited rods produced by consuming graphite rods with the same diameter ( $ inches) at the same dc current (100 A, 20 V) in a He atmosphere at the same pressure (500 Torr) are shown in Fig. 9. Photos (a) and (b) were taken from deposited rods synthesized in the glow mode and the arc mode, respectively. The two photos clearly indicate that the deposited rod produced in the glow mode has a more homogeneous black core, consisting of an array of bundles of buckytubes, and only a thin cladding. The glow mode produced a higher yield of buckytubes than the conventional arc mode. Figure 10 shows scanning electron microscopy (SEM) micrographs of a cross-section of the deposited rod synthesized in the glow mode. In Fig. 10 the upper left corner of the micrographs corresponds to the center of the cross-section of the deposited rod. The micrograph shows an evenly distributed array of parallel bundles of buckytubes from the black region of the deposited rod. The thickest bundles with diameters up to 200 pm were observed for the first time at the central region of the deposited rod. It is interesting to
zyxwvutsr zyxwvuts zyxwv m
Time (sec) Fig. 8. (a) The current of the glow discharge as a function of time; (b) the current of the arc discharge as a function of time.
zyxwvut zyxwv zyxwvutsrqponm X. K. WANGet al.
Fig. 9. Photographs of the cross-section of the deposited rods; photos (a) and (b) were taken from deposited rods produced by the glow discharge and by the conventional arc discharge, respectively.
note that the average diameter of the bundles decreases towards the perimeter of the deposited rod. The cladding shell around the rod is composed of fused graphitic flakes. The geometry and the distribution of the bundles in the deposited rod may be interpreted as follows. In the glow mode, the highest temperature occurs
at the center of the deposited rod and the temperature decreases towards the perimeter because the heat is transported by both radiation and conduction via the He gas. In the cladding shell area, the temperature may not be high enough to form the bundles but is sufficient to form fused graphitic materials. Although several groups have speculated on the effect of the electric field in the formation of buckytubes[ 1316,471, the influence of the temperature on the yield and distribution of the bundles has not been discussed. From our results, we may conclude that the temperature is one of the key factors in the formation of buckybundles. Figure 11 shows two typical TEM images for the deposited rods synthesized in the glow mode and the conventional arc mode, respectively. Two samples for TEM observation were prepared in an identical way. The figures show the dramatic improvement in the yield and quality of buckytubes synthesized in the glow mode. The buckytubes and their bundles shown in Fig. 11 (a) are thicker and longer than that shown in Fig. 11 (b). The length of the tubes shown here is larger than the field of view of HREM used in this study. Our systematic studies indicated that the yield of the tubes made by the glow discharge is at least 20 times larger than that of the tubes made by the arc discharge. In the arc mode, the jumping of the arc causes an instability of the electric field which leads to a closure of the tube tips, so as to minimize dangling bonds and lower the total energy. Therefore, the conventional arc discharge produces a low yield of lowquality buckytubes. Note also that a large number of the tube tips, shown in Fig. 11 (b), are closed by caps that are polygonal or cone-shaped. Iijima has found that the
Fig. 10. A SEM micrograph of the cross-section of the deposited rod synthesized by the glow discharge shows an image of 1/4 of the cross-section of the deposited rod; upper left corner of the image corresponds to the center of the end of the deposited rod.
Properties of buckytubes and derivatives
Fig. 11. (a) and (b) are HREM images of the deposited rods produced by the glow discharge and by the conventional arc discharge, respectively.
polygonal and cone-shaped caps are formed by incorporating pentagons into the hexagonal network. H e speculated that the formation of the pentagons may result from a depletion of carbon in plasma near the end of cathode. Our experimental results offer evidence for the above speculation. Fluctuations of carbon species caused by a discontinuous arc discharge may be responsible for the formation of short tubes with the caps, consisting of pentagons and other defects. Based on these experimental results, one can speculate on the influence of the arc mode on the yield and distribution of the bundles. For the glow discharge, the plasma is continuous, homogeneous, and stable. In other words, the temperature distribution, the electric field which keeps growing tube tips open, and the availability of carbon species (atoms, ions, and radicals) are continuous, homogeneous, and stable over the entire central region of the cathode. Accordingly, a high yield and better quality buckytubes should occur over the entire central region of the cathode. These are consistent with what we observed in Fig. 9 (a), Fig. 10, and Fig. 11 (a). For the conventional arc discharge, we can speculate that the arc starts at a sharp edge near the point of closest approach, and after vaporizing this region it jumps to what then becomes the next point of closest approach (usually within about a radius of the arc area), and so on. The arc wanders around on the surface of the end of the anode, leading, on the average, t o a discontinuous evaporation process and an instability of the electric field. This kind of violent, randomly jumping arc discharge is responsible for the low yield and the low quality of the deposited buckytubes. This is, again, consistent with what we showed in Fig. 9 ( b ) and Fig. 11 (b). Note also from Fig. 11 that carbon nanotubes and nanoparticles coexist in both samples. The coexistence of these two carbonaceous products may suggest that some formation conditions, such as the temperature and the density of the various carbon species, are almost the same for the nanotubes and the
nanoparticles. An effort to promote the growth of carbon nanotubes and eliminate the formation of carbon nanoparticles is presently underway. 4. CONCLUSIONS
In this article, we have reported the structural, magnetic, and transport properties of bundles of buckytubes produced by an arc discharge. By adjusting the arc mode into a stable glow discharge, evenly spaced and parallel buckybundles with diameters up to 200 pm have been synthesized. The magnetic susceptibility of a bulk sample of buckybundles is -10.75 x emu/g for the magnetic field parallel to the bundle axes, which is approximately 1.1 times the perpendicular value and 30 times larger than that of c60. The magnetoresistance (MR) and Hall coefficient measurements on the buckybundles show a negative MR at low temperature, a positive MR at a temperature above 6 0 K , and a conductivity which increases approximately linearly with temperature. Our results show that a buckybundle may best be described as a semimetal.
Acknowledgements-We are grateful to A. Patashinski for useful discussions. This work was performed under the support of NSF grant #9320520 and DMR-9357513 (NYI award for VPD). The use of MRC central facilities supported by NSF is gratefully acknowledged.
1. S. Iijima, Nature 354, 56 (1993). 2. S. Iijima, T. Ichihashi, and Y. Ando, Nature 356, 776 ( 1992). 3. T. W. Ebbesen and P. M. Ajayan, Nature 358, 220 (1992).
4. Y. Ando and S. Iijima, Jpn. J. Appl. Phys. 32, L107
(1993). 5. T. W. Ebbesen, H. Hiura, J. Fujita, Y. Ochiai, S. Matsui, and K. Tanigaki, Chem. Phys. Lett. 209, 83 (1993). 6. Y. Saito, T. Yoshikawa, M. Inagaki, M. Tomita, and T. Nayashi, Chem. Phys. Lett. 204, 277 (1993).
zyxwvutsrqp zyxwvu z zyxwvu zyxwvut zyxwvutsr zyxwvu X. K. WANGet ai.
7. Z. Zhang and C . M. Lieber, Appl. Phys. Lett. 62,2792 (1993). 8. S. N. Song, X. K. Wang, R. P. H. Chang, and J. B. Ketterson, Phys. Rev. Lett. 72, 697 (1994). 9. D. Ugarte, Nature 359, 707 (1992). 10. S. Iijima, P. M. Ajayan, and T. Ichihashi, Phys. Rev. Lett. 69, 3100 (1992). 11. R. A. Jishi, M. S. Dresselhaus, and G. Dresselhaus, Phys. Rev. B 48, 11385 (1993). 12. L. Langer, L. Stockman, J. P. Heremans, V. Bayot, C. H. Olk, C . V. Haesendonck, and Y. Bruynseraede, J. Mater. Res. 9, 927 (1994). 13. J. W. Mintmire, B. I. Dunlap, and C. T. White, Phys. Rev. Lett. 68, 631 (1992). 14. D. H. Robertson, D. W. Brenner, and J. W. Mintmire, Phys. Rev. B 45, 12592 (1992). 15. N. Hamada, S. I. Sawana, and A. Oshiyama, Phys. Rev. Lett. 68, 1579 (1993). 16. R. Saito, M. Fujita, G . Dresselhaus, and M. S. Dresselhaus, Mater. Res. SOC. Symp. Proc. 247, 333 (1992). 17. G. Dresselhaus, M. S. Dresselhaus, and R. Saito, Phys. Rev. B45, 6234 (1992). 18. H. W. Kroto, J. R. Heath, S. C. O’Brien, R. E Curl, and R. E. Smalley, Nature 318, 162 (1985). 19. R. Tycko, R. C . Haddon, G. Dabbagh, S. H. Glarum, D. C. Douglass, and A. M. Mujsce, J. Phys. Chem. 95, 518 (1991). 20. S. Iijima and T. Ichihashi, Nature 363, 603 (1993). 21. D. S. Bethune, C. H. Klang, M. S. deVries, G. Gorman, R. Savoy, J. Vazqiez, and R. Beyers, Nature 363, 605 (1993). 22. X. W. Lin, X. K. Wang, V. P. Dravid, R. P. H. Chang, and J. B. Ketterson, Appl. Phys. Lett. 64, 181 (1994). 23. R. E. Haufler, J. Conceicao, L. P. E Chibante, Y. Chai, N. E. Byme, S. Flanagan, M. M. Haley, S. C. O’Brien, C. Pan, Z. Xiao, W. E. Billups, M. A. Ciufolini, R. H. Hauge, J. L. Margrave, L. J. Wilson, R. F. Curl, and R. E. Smalley, J. Phys. Chem. 94, 8634 (1990). 24. V. Elser and R. C. Haddon, Nature 325, 793 (1987). 25. R. C. Haddon, L. F. Schneemeyer, J. V. Waszczak, S. H. Glarum, R. Tycko, G. Dabbagh, A. R. Kortan, A. J. Muller, A. M. Mujsce, M. J. Rosseinsky, S. M. Zahurak, A. V. Makhija, F. A. Thiel, K. Raghavachari, E. Cockayne, and V. Elser, Nature 350, 46 (1991).
26. A. Pasquarello, M. Schluter, and R. C . Haddon, Science 257, 1660 (1992). 27. P. W. Fowler, P. Lazzeretti, M. Malagoli, and R. Zanasi, Chem. Phys. Left. 179, 174 (1991). 28. T. G. Schmalz, Chem. Phys. Lett. 175, 3 (1990). 29. R. S. Ruoff, D. Beach, J. Cuomo, T. McGuire, R. L. Whetten, and E. Diederich, J. Phys. Chem. 95, 3457 (1 991). 30. H. Ajiki and T. Ando, J. Phys. SOC.Japan 62, 2470 1993. 31. V. P. Dravid, X. W. Lin, Y. Y. Wang, X. K. Wang, A. Yee, J. B. Ketterson, and H. P. H. Chang, Science259, 1601 (1993). 32. X. K. Wang, X . W. Lin, V. P. Dravid, J. B. Ketterson, and R. P. H. Chang, Appl. Phys. Lett. 62, 1881 (1993). 33. J. C. Slonczewski and P. R. Weiss, Phys. Rev. 109, 272 (1958). 34. J. W. McClure, Phys. Rev. 199, 606 (1960). 35. R. M. White, Quantum Theory of Magnetism, Springer Series in Solid State Sciences, Springer-Verlag Berlin, Heidelberg, New York (1983). 36. X. K. Wang, R. P. H. Chang, A. Patashinski, and J. E. Ketterson, J. Mater. Res. 9, 1578 (1994). 37. S. Saito and A. Oshiyama, Phys. Rev. Lett. 66, 2637 (199 1). 38. L. Pauling, J. Chem. Phys. 4 , 637 (1936). 39. S. N. Song, X. K. Wang, R. P. H. Chang, and J. B. Ketterson, Phys. Rev. Lett. 72, 679 (1994). 40. J. Callaqay, In Quantum Theory of the Solids, p. 614, Academic Press, New York (1976). 41. P. Delhaes, P. de Kepper, and M. Uhlrich, Philos. Mag. 29, 1301 (1974). 42. M. Ge and K. Sattler, Appl. Phys. Lett. 64, 710 (1994). 43. M. J. Yacaman, M. M. Yoshida, L. Rendon, and J. G. Santiesteban, Appf. Phys. Lett. 62, 657 (1993). 44. M. Endo and H. W. Kroto, J. Phys. Chem. 96, 6941 (1992). 45. J. R. Brock and P. Lim, Appl. Phys. Lett. 58, 1259 (1991). 46. 0. Zhou, R. M. Fleming, 0. W. Murphy, C. H. Chen, R. C. Haddon, A. P. Ramire, and S. H. Glarum, Science 263, 1774 (1994). 47. R. E. Smalley, Mater. Sci. Engin. B19, 1 (1993).
zyxwvu zyxw zyxw zyxw
ELECTRONIC PROPERTIES OF CARBON NANOTUBES: EXPERIMENTAL RESULTS J.-P. ISSI,’ L. LANGER,’J. HEREMANS? and C. H.
‘Unite PCPM, Universitt Catholique de Louvain, Louvain-la-Neuve, Belgium 2General Motors Research and Development Center, Warren, MI 48090, U.S.A.
(Received 6 February 1995, accepted 10 February 1995)
Abstract-Band structure calculations show that carbon nanotubes exist as either metals or semiconductors, depending on diameter and degree of helicity. When the diameters of the nanotubes become comparable to the electron wavelength, the band structure becomes noticeably one-dimensional. Scanning tunneling microscopy and spectroscopy data on nanotubes with outer diameters from 2 to 10 nm show evidence of onedimensional behavior: the current-voltage characteristics are consistent with the functional energy dependence of the density-of-states in 1D systems. The measured energy gap values vary linearly with the inverse nanotube diameter. Electrical resistivity and magnetoresistance measurements have been reported for larger bundles, and the temperature dependence of the electrical resistance of z single microbundle was found t o be similar to that of graphite and its magnetoresistance was consistent with the formation of Landau levels. Magnetic susceptibility data taken on bundles of similar tubes reveal a mostly diamagnetic behavior. The susceptibility at fields above the value at which the magnetic length equals the tube diameter has a graphite-like dependence on temperature and field. At low fields, where electrons sari.ple the effect of the Finite tube diameter, the susceptibility has a much more pronounced temperature dependence.
Key W70rds--Carbon nanotubes, scanning tunneling microscopy, spectroscopy, magnetoresistance, electrical resistivity, magnetic susceptibility.
perimental challenges result from the fact that tubes are often produced in bundles, so that obtaining data on single, well-characterized tubes has not yet been achieved. We review here some experimental observations relevant to the electronic structure of individual nanotubes or on bundles of nanotubes: combined scanning tunneling microscopy and spectroscopy, temperature-dependent resistivity, magnetoresistance (MR), and magnetic susceptibility.
The existence of carbon nanotubes with diameters small compared to the de Broglie wavelength has been described by Iijima[l,2,3] and others[4,5]. The energy band structures for carbon nanotubes have been calculated by a number of authors and the results are summarized in this issue by M.S. Dresselhaus, 6.Dresselhaus, and R. Saito. In short, the tubules can be either metallic or semiconducting, depending on the tubule diameter and chirality[6,7,8]. The calculated density of states shows I/(KEj)’’’ singularities characteristic of one-dimensional (1D) systems. The separation between the singularities around the Fermi energy is the energy gap for the tubes that are semiconducting, and scales linearly with the inverse of the tube outer diameter[7,8]. This contrasts with the case of a rod-shaped quantum wire, for which the gap is expected to scale with the inverse square of the diameter. The relevant energy scale for the gap in carbon nanotubes is the nearest-neighbor overlap integral in graphite (3.14 eV). This makes room-temperature observation of the quantum size effects, in principle, possible in nanotubes with diameters in the nm range, because the sublevel energy separations are of the order of 1 eV. Experimental measurements to test these remarkable theoretical predictions of the electronic structure of carbon nanotubes are difficult to carry out because of the strong dependence of the predicted properties on tubule diameter and chirality. Ideally, electronic or optical measurements should be made on individual single-wall nanotubes that have been characterized with regard to diameter and chiral angle. Further ex-
2. SCANNING TUNNELING SPECTROSCOPY STUDIES
Scanning tunneling spectroscopy (STS) can, in principle, probe the electronic density of states of a singlewall nanotube, or the outermost cylinder of a multi-wall tubule, or of a bundle of tubules. With this technique, it is further possible to carry out both STS and scanning tunneling microscopy (STM) measurements at the same location on the same tubule and, therefore, to measure the tubule diameter concurrently with the STS spectrum. No reports have yet been made of a determination of the chiral angle of a tubule with the STM technique. Several groups have, thus far, attempted STS studies of individual tubules. The first report of current-voltage (I-V) measurements by Zhang and Lieber[lO] suggested a gap in the density of states below about 200 MeV and semiconducting behavior in the smallest of their nanotubes (6 nm diameter). The study that provides the most detailed test of the theory for the electronic properties of the 1D carbon nanotubes, thus far, is the combined STM/STS study by Olk and Heremans[111, even though it is still preliminary. In this study, more than nine
zyxwvutsrqpo zyxwvutsrq zyxwvut J.-P. ISSI et ul.
Fig. 1. Topographic STM scan of a bundle of nanotubes. STS data were collected at points (I), (2), and (3), on tubes with diameters of 8.7, 4.0,and 1.7 nm, respectively. The diameters were determined from image cross-sections of the variations in height in a direction perpendicular to the tubes (adapted from Olk et u/.[ll]).
individual multilayer tubules with diameters ranging from 2 to 10 nm, prepared by the standard carbon-arc technique, were examined. STM measurements were taken first, and a topographic STM scan of a bundle of nanotubes is shown in Fig. 1. The exponential relation between the tunneling current and the tip-totubule distance was experimentally verified to confirm that the tunneling measurements pertain to the tubule and not to contamination on the tubule surface. From these relations, barrier heights were measured to establish the range in which the current-voltage characteristics can be taken for further STS studies. The image in Fig. 1 is used to determine the diameter of the individual tubule on which the STS scans are carried out. During brief interruptions in the STM scans, the instrument was rapidly switched to the STS mode of operation, and I-V plots were made on the same region of the same tubule as was characterized for its diameter by the STM measurement. The I-V plots for three typical tubules, identified (1)-(3), are shown in Fig. 2. The regions (1)-(3) correspond to interruptions in the STM scans at the locations identified by crosses in the topographic scan, Fig. 1. Although acquisition of spectroscopic data in air can be complicated by contamination-mediated effects on the tunneling gap, several studies on a wide variety of surfaces have been reported[l2]. Trace (1) in Fig. 2 , taken on a tube with 8.7 nm diameter, has an ohmic behavior, providing evidence for the metallic nature of that tubule. Two tu-
bules (trace 2 for a tubule with diameter = 4.0 nm, and trace 3 for a tubule with diameter = 1.7 nm) show plateaus in the I/V characteristics at zero current. This rectifying behavior is the signature of semiconducting tubules. The dI/dV plot in the inset crudely mimics a 1D density of states, the peaks in the dI/dV plot be-
Fig. 2. Current-voltage characteristics taken at points (l), (2), and (3) in Fig. 3. The top insert shows the conductance versus voltage plot, for the data taken at point (3) (adapted from Olk et ul.[ll]).
zyxwvuts zyxwvutsrqp zyxw zyxwvutsr zyxwvut Electronic properties of carbon nanotubes
ing attributed to [I/(&, - E)’”] -type singularities in the 1D density of states seen in the density of states versus energy diagrams calculated in. Several I-V curves were collected along the length of each tube. Reproducible spectra were obtained on 9 tubes with different diameters. The energy gap of the semiconducting tubes was estimated around V = 0 V by drawing two tangents at the points of maximum slope nearest zero in the I-V spectra, and measuring the voltage difference between the intercepts of these tangents with the abscissa. A plot of these energy gaps versus inverse tube diameter for all samples studied is shown in Fig. 3. Surface contamination may account for the scatter in the data points, though the correlation between Egand the inverse diameter shown in Fig. 3 is illustrated by the dashed line. The data in Fig. 3 is consistent with the predicted dependence on the inverse diameter[ 131. The experimentally measured values of the bandgaps are, however, about a factor of two greater than the theoretically estimated ones on the basis of a tight binding calculation (full line in Fig. 3)[7,13]. Further experimental and theoretical work is needed to reach a detailed understanding of these phenomena. 3. ELECTRICAL RESISTIVITY AND MAGNETORESISTANCE
The remarkable theoretical predictions mentioned above are even more difficult to verify by experimental measurements in the case of electrical conductivity. Ideally, one has to solve two experimental problems. First, one has to realize a four-point measurement on an individual nanotube. That means four contacts on a sample with typical dimensions of the order of a nm
diameter and a few pm length. Second, this sample with its contacts must be characterized to determine its exact diameter and helicity. To take up this challenge it is necessary to resort to nanotechnologies. Before reviewing the results of different measurements, we need to first briefly describe the nature of the deposit formed during the carbon-arc experiment in a way first proposed by EbbesentS]. He suggested that the carbon nanotubes produced by classical carbon arc-discharge present a fractal-like organization. The deposit on the negative electrode consists of a hard gray outer shell and a soft black fibrous core containing the carbon nanotubes. If we examine in detail this core material by scanning electron microscopy, we observe a fractal-like structure. This means that the black core is made of fiber-like entities that are, in reality, bundles of smaller fiber-like systems. These smaller systems are, in turn, formed of smaller bundles, and so on. The micro-bundle, which is the smallest bundle, consists of a few perfectly aligned nanotubes of almost equal lengths. Finally, each of these individual nanotubes is generally formed of several concentric single-shell nanotubes. The fractal-like organization led, therefore, to conductivity measurements at three different scales: (1) the macroscopic, mm-size core of nanotube containing material, (2) a large (60 pm) bundle of nanotubes and, (3) a single microbundle, 50 nm in diameter. These measurements, though they do not allow direct insights on the electronic properties of an individuai tube give, nevertheless, at a different scale and within certain limits fairly useful information on these properties. Ebbesen was the first to estimate a conductivity of the order of Qm for the black core bulk material existing in two thirds of tubes and one third of nanoparticles. From this observation, it may naturally be inferred that the carbon arc deposit must contain material that is electricaliy conducting. An analysis of the temperature dependence of the zerofield resistivity of similar bulk materials[ 14,151 indicated that the absolute values of the conductivity were very sample dependent. Song et al.  reported results relative to a fourpoint resistivity measurement on a large bundle of carbon nanotubes (60 pm diameter and 350 pm in length between the two potential contacts). They explained their resistivity, magnetoresistance, and Hall effect results in terms of a conductor that could be modeled as a semimetal. Figures 4 (a) and (b) show the magnetic field dependence they observed on the high- and low-temperature MR, respectively. At high temperature, the conductivity was found to increase linearly with temperature and the observed high-temperature MR was positive. In fact, by fitting the data using a simple two-band model[l7] the authors obtained the theoretical curve in Fig. 4 (a). The fitting parameters showed that the ratio u,/a,, where up and a, are the partial conductivities of holes and electrons, respectively, decreases with increasing tem-
Fig. 3. Energy gap versus inverse nanotube diameter, for the nine nanotubes studied; the dashed line is a regression through the points, the full line is a calculation for semiconducting zigzag nanotubes[7,13] (adapted from Olk et aL[ll]).
zyxwvutsrqpon zyxwvu zyxwvutsr J.-P. ISSI et al.
nanotube structures like microbundles, or even better, single nanotubes. A rather sophisticated technique, namely submicronic lithographic patterning of gold films with a scanning tunneling microscope[ 181, was developed by Langer et al. [ 191 to attach two electrical contacts to a single microbundle. This direct electrical resistance measurement on this quasi-1D system excludes the errors that may result from the situations described in (2) and (4) in the last paragraph. The reported temperature dependence measured from 300 K down to 0.3 K by Langer et al.  is shown in Fig. 5. Above 2 K, some interesting information was obtained by fitting the experimental zero-field resistance data to a simple two-band (STB) model successfullyapplied by Klein[20-22] to semimetallic graphite. In this STBmodel, the electron and hole densities, n andp, respectively, can be expressed by:
+ exp[(A - EF)/kBTII
zyxwvu p = C,k,Tln[l
Fig. 4. (a) Magnetic field dependence of the high- and lowtemperature MR, respectively. The solid lines are calculated using a simple two-band model for (a) and the 2D weak localization theory for (b) (after Song et a/.).
perature implying that, as the temperature increases the Fermi level shifts closer to the conduction band. The increase in total conductivity, a, up,with temperature was attributed to an increase in electron concentration. Song et al.  attributed the fact that above 60 K the conductivity increases almost linearly with temperature, as opposed to an exponential or variable range hopping-type temperature dependence, to a semimetallic behavior. At low temperature and low field, the observed MR was found to be negative, Fig. 4 (b), while positive MR contributions were increasingly important for higher fields. While 1D weak localization (WL) was found by Song et al. [lq to be inadequate to describe the data, they claimed that 2D WL fit the experimental results for the temperature dependence of the resistivity and the MR at low temperature and low fields. They estimated a resistivity of 0.65 x lop4 Qm at 300 K and 1.6 x Om at 5 K. However, the actual resistivity of the metallic tubules along their axis should be much lower than these values for many reasons: (1) as predicted by the theory described in , only one third of the tubules are conducting; (2) the filling factor of a large bundle like the measured one is less than 1; (3) when the tubes are not single-walled, the cross-section of the nanotubes where conduction occurs is unknown and affected by their inner structure and, finally, (4) the nanotube is anisotropic. To avoid the problems described above relative to the interpretation of the results, it is necessary to work at a lower scale. In other words, modern nanotechnology must be used to contact electrically smaller
zyxwvut zyxwvutsr '8
zyxwvuts zyxwvut zyxwvutsrq zyxwvutsrqp zyxwvutsrqpo zyxwvuts zyxwvut Electronic properties of carbon nanotubes
where Ef is the Fermi energy and A is the band overlap. C, and C, are the fitting parameters. The results of this fit, which is shown in Fig. 5, is obtained for A = 3.7 MeV and with the Fermi energy right in the middle of the overlap. Ideally, an overlap of the order of 40 MeV is expected for the case of multilayered nanotubes with an interlayer configuration similar to that of crystalline graphite. For real nanotubes instead, a turbostratic stacking of the adjacent layers would reduce drastically the interlayer interactions, as in disordered graphite, and so it is not surprising to find a band overlap 10 times smaller than in crystalline graphite. This implies also that, within the frame of the STB model, the carrier density is 10 times smaller. The apparent electrical resistivity (4 x Om) measured at low temperature is certainly still higher than the resistivity of a single nanotube. In fact, the conductance of the system is dominated by that of the nanotubes with the highest conductance (Le., the semimetallic nanotubes). All these nanotubes are not necessarily in contact with the measuring probes. Finally, the inner structure of each individual nanotube in this microbundle remains unknown. By applying a magnetic field normal to the tube axis, Langer et ai. I191 observed a MR (Fig. 6) which, in contrast to the case of graphite, remains negative at all fields. The negative MR was found consistent with the formation of Landau levels. Ajiki and Ando have predicted that a magnetic field applied perpendicularly to the sample axis should introduce a Landau level at the crossing of the valence and conduction bands. It results in an increase of the density of states at the Fermi level and, hence, a reduction of the resistance, which is in agreement with the experimental data. Moreover, the theory predicts a MR that is temperature independent at low temperature and decreasing when kBTbecomes larger than the Landau level. This is also what was experimentally observed. Thus, in contrast to what was reported by Song et a/.,
these results are not consistent with WL. In the framework of WL, the observed temperature independent MR below 10 K and down to 1 K could only be explained in the presence of large amounts of magnetic impurities, as is the case for some pyrocarbons. However, in the present case, the spectrographic analysis performed by Heremans et al.  excludes the presence of magnetic impurities. Below 2 K, an unexpected temperature dependence of the resistance and MR is observed. As shown in Fig. 5, the resistance presents, after an initial increase, a saturation or a broad maximum and an unexplained sharp drop when a magnetic field is applied (see Fig. 6). Further theoretical work is needed to get a better understanding of these striking physical observations. Finally, it is interesting to note that Whitesides and Weisbecker developed a technique to estimate the conductivity of single nanotubes by dispersing nanotubes onto lithographicallydefined gold contacts to realize a 'nano-wire' circuit. From this 2-point resistance measurement and, after measuring the diameter of the single nanotubes by non-contact AFM, they estimated the room-temperature electrical resistivity along the nanotube axis to be 9.5 x low5Qm. This is consistent with the values obtained for a microbundle by Langer et a/. 1191. The most promising way to study the electrical conductivity of a single nanotube is, thus, tightly dependent on the development or/and the adaptation of modern nanolithographic techniques. The goal to achieve is within reach and a detailed study of the electronic properties with reference to helicity and diameter will provide instrumental information about these fascinating materials.
4. MAGNETIC SUSCEPTIBILITY
The presence of aromatic-like electrons strongly determines the magnetic susceptibility of the diverse forms of carbons. The susceptibility of diamond emu/g) is ascribed to diamagnetic con(-4.9 x tributions from core and valence electrons, and a Van Vleck paramagnetic term. Graphite has an anisotropic diamagnetic susceptibility. The susceptibility of graphite[29,30] parallel to the planes is about equal to the free atom susceptibility of -5 x emu/g, but when the magnetic field is aligned parallel to the c-axis, the susceptibility of graphite (-30 X lop6 emu/g below loOK) is due mainly to free electron contributions and is much larger. The magnetic emulg) and C70 susceptibility of C60 (-3.5 x (-5.9 x 1 0 - ~emu/g) is small again[31,32], as a result of a cancellation between a diamagnetic and a paramagnetic term. In the light of these results, it is not surprising that a very large anisotropy has been calculated to exist in the magnetic susceptibility of nanotubes. The susceptibility with the field parallel to the tube axis is predicted to be as much as 3 orders of magnitude smaller than that with the field perpendicular. Again,
MAGNETIC FIELD [TI
Fig. 6. The magnetic field dependence of the magnetoresistance at different temperature for the same microbundle measured in Fig. 5 (after Langer et n1.).
zyxwvu zyxwvutsr zyxwvut
J.-P. ISSI et al.
measurements on individual single-wall well-charac0.0 terized tubes have not been published to date. Experiments usually involve gathering nanotube material (r from several growths, to obtain quantities of material \-0.2 on the order of tens of mg. A measurement on ori2 E ented bundles of tubes at 0.5 T as a function of a, temperature gives evidence for anisotropy. Such a "-0.4 CI measurement is, however, easily affected by a small c a misalignment of the sample. It is, therefore, possible E -0.6 that the data reported for the case where the field is 0 r parallel to the tube axis are, in fact, dominated by contributions from the perpendicular susceptibility. -0.8 A second study  on samples that contain a mixture of nanotubes, together with several percent -1 .o "buckyonion"-type structures, was carried out at tem0 20000 40000 60000 Magnetic Field (Oe) peratures between 4.5 and 300 K, and fields between 0 and 5.5 T. The moment M i s plotted as a function Fig. 8. Field dependence of the moment of carbon nanotubes of field in Fig. 7, for the low-field range, and in Fig. 8 at the temperatures shown at high magnetic fields (after Herefor the high-field range. The field dependence is mans et al. ). clearly non-linear, unlike that of graphite, in which both the basal plane and the c-axis moments are linear in field, except for the pronounced de Haas-van the tube diameter. The sample, however, consists of a Alphen oscillations at low temperature. mixture of semiconducting and metallic tubes. The The a.c. susceptibility (x = dM/dH, where M i s the component of x perpendicular to the tube axis domimoment), measured at 5,0.4, and 0.04 T, is shown as nates the measured susceptibility, and the value is exa function of temperature in Fig. 9. Three regimes of pected to scale with 1/EF. The electrical resistivity magnetic fields are identified in ref. . The highdata show that, even in the metallic samples, the enfield susceptibility (at 5 T) has a temperature depen- ergy gap is on the order of a few MeV. At room dence similar to that of graphite, but a magnitude temperature kBT> EF for both metallic and semiconreduced by a factor of 2. In this regime, the magnetic ducting samples. Thus, a thermally activated behavior radius (hb/eB)"' becomes shorter than the tube diamis expected for the average susceptibility. Furthermore, eter. The electronic diamagnetism is then a local probe carriers may be scattered at a temperature-dependent of the graphene planes, and its value is expected to be rate, for instance by acoustic phonons. These two the geometrical average of that of rolled-up graphene. mechanisms are consistent with the much more proBecause with the field in the basal plane, x is much nounced temperature dependence of the low-field smaller than along the c-axis, this geometrical average susceptibility of nanotubes than of graphite. More comes out to be about +.The low-field susceptibilquantitative models remain to be developed. In the inity (at 0.04 T) is a better probe of the finite size effects of the tubes, because the magnetic length is larger than
zyxwv zyxwvutsrq L'
4? -0.08 -0.12
1000 2000 3000 4000 5000 6000
Magnetic Field (Oe) Fig. 7. Field dependence of the moment of carbon nanotubes at the temperatures shown at low magnetic fields (after Heremans et al.).
Fig. 9. Susceptibility of carbon nanotubes versus temperature at the different fields identified in the figure (after Heremans el a/.).
Electronic properties of carbon nanotubes
termediate field regime (around 0.5 T), x is probably sensitive to the fact that the sample consists of a mixture of semiconducting and metallic tubes. Furthermore, the tubes in that mixture have different diameters and, thus, go from the low-field to the high-field regime at different fields. Figure 10 shows a summary of the a.c. susceptibilitiesof various forms of carbon, as an easy ready reference. The values for diamond and the basal plane of graphite represent the atomic contributions, and the c-axis of graphite and the susceptibilities of nanotubes are dominated by free carrier contributions.
model developed by Ajiki and Ando[%]. From the temperature dependence of the electrical resistance of this microbundle, it appears that the measured nanotubes are semimetallic and behave like rolled-up graphene sheets. Below 1 K, the results are puzzling and yet unexplained. Susceptibility was measured on 20-mg samples containing a large variety of tubes. Free carrier contributes to the diamagnetic behavior of nanotubes, which is similar to that of graphite when the magnetic length is smaller than the tube diameter. The low-field diamagnetism contains more information about the specific band structure of the tubes.
Acknowledgements-The authors gratefully acknowledge much help from M.S. Dresselhaus and G . Dresselhaus in the preparation of this article.
zyxwvu zyxwvu zyxwv
The purpose of this work is to review experimental data on the electronic properties of carbon nanotubes. Although most of the theoretical work has been focused on single-walled individual tubes, performing transport and other measurements on such entities is extremely difficult and remains unachieved. Combined STM and STS measurements access single tubes within bundles containing a few a tubes. They provide experimental evidence that graphite nanotubes behave as nanowires, with a density of states and an energy gap dependence on inverse diameter as predicted. Studies in ultra-high vacuum are needed to provide more quantitative data on the dependence of the gap on diameter. No electrical resistance measurements are currently available on a well-characterized single nanotube. However, electrical resistivity measurements performed at low temperature on a large nanotube bundle were interpreted in terms of a 2D WL. On the other hand, MR data obtained for a single microbundle were consistent with the formation of Landau levels using the
1. S. Iijima, Nature (London) 354, 56 (1991). 2. S. Iijima, Mater. Sci. Eng. B19, 172 (1993). 3. S. Iijima, T. Ichihashi, and Y. Ando, Nature (London) 356, 776 (1992). 4. T. W. Ebbesen and P. M. Ajayan, Nature (London) 358, 220 (1992). 5. T. W. Ebbesen, H. Hiura, J. Fujita, Y. Ochiai, S. Matsui, and K. Tanigaki, Chem. Phys. Lett. 209, 83 (1993). 6. J. C. Charlier and J. P. Michenaud, Phys. Rev. Lett. 70, 1858 (1993). J. C. Charlier, Carbon Nunotubes and Fullerenes. PhD thesis, Catholic University of Louvain, May 1994. 7. C. T. White, D. H. Roberston, and J. W. Mintmire, Phys. Rev. B 47, 5485 (1993). 8. R. Saito, G. Dresselhaus, and M. S. Dresselhaus, J. Appl. Phys. 73, 494 (1993). M. S. Dresselhaus, G. Dresselhaus, and R. Saito, Solid State Commun. 84, 201 (1992). 9. R. Saito, M. Fujita, G. Dresselhaus, and M. S. Dresselhaus, In Electrical, Optical and Magnetic Properties of Organic Solid State Materials, MRS Symposia Proceedings, Boston (Edited by L. Y. Chiang, A. E Garito, and D. J. Sandman), vol. 247, page 333. Materials Research Society Press, Pittsburgh, PA (1992). 10. 2. Zhang and C. M. Lieber, Appl. Phys. Lett. 62,2792 (1993). 11. C. H. Olk and J. P. Heremans, J. Mater. Res. 9, 259 (1994). 12. N. Venkateswaran, K. Sattler, U. Muller, B. Kaiser, 6. Raina, and J. Xhie, J. Vac. Sci. Technol.B9, 1052 (1991). M. Jobin, R. Emch, F. Zenhausern, S. Steinemann, and P. Descouts, J. Vac. Sci. Technol. B9, 1263 (1991). 2. Zhang, C. M. Lieber, D. S. Ginley, R. J. Baughman, and B. Morosin, J. Vac. Sci. Technol. B9, 1009 (1991). H. Enomoto, H. Ozaki, M. Suzuki, T. Pujii, and M. Yamaguchi, J. Vac. Sci. Technol. B9, 1022 (1991). 13. M. S. Dresselhaus, R. A. Jishi, G. Dresselhaus, and Riichiro Saito, Fullerenes (1994). St. Petersburg, Russia Fullerene workshop, October 1993. 14. R. Heyd, A. Charlier, J. F. Marechi, E. McRae, and 0. V. Zharikov, Solid State Commun. 89, 989 (1994). 15. R. Seshardi, H. N. Aiyer, A. Govindaraj, and C. N. Rao, Solid State Commun. 91, 195 (1994). 16. S. N. Song, X. K. Wang, R. P. H. Chang, and J. B. Ketterson, Phys. Rev. Lett. 12, 697 (1994). 17. K. Noto and T. Tsuzuku, Jpn. J. Appl. Phys. 14, 46 (1975). 18. L. Stockman, G. Neuttiens, C. Van Haesendonck, and Y. Bruynseraede, Appl. phys. Lett. 62, 2935 (1993).
zyxwvu zyxwvutsrqp zyxwvut zyxw zyxwvutsrqp zyxwvutsrq J
Grappite, H in-plane 0-0 -0-